SCALING OF STRUCTURAL STRENGTH
SCALING OF STRUCTURAL STRENGTH Second edition Zdenˇek P Baˇzant
AMSTERDAM • BOSTON • ...

Author:
Zdenek P. Bazant

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

SCALING OF STRUCTURAL STRENGTH

SCALING OF STRUCTURAL STRENGTH Second edition Zdenˇek P Baˇzant

AMSTERDAM • BOSTON • HEIDELBERG • LONDON • NEW YORK • OXFORD PARIS • SAN DIEGO • SAN FRANCISCO • SINGAPORE • SYDNEY • TOKYO

Elsevier Butterworth-Heinemann Linacre House, Jordan Hill, Oxford OX2 8DP 30 Corporate Drive, Burlington, MA 01803 First published by Hermes Penton Ltd 2002 Second edition 2005 c 2005, Elsevier Ltd. All rights reserved Copyright The right of Zdenˇek P Baˇ zant to be identiﬁed as the author of this Work has been asserted in accordance with the Copyright, Designs And Patents Act 1988 No part of this publication may be reproduced in any material form (including photocopying or storing in any medium by electronic means and whether or not transiently or incidentally to some other use of this publication) without the written permission of the copyright holder except in accordance with the provisions of the Copyright, Designs and Patents Act 1988 or under the terms of a licence issued by the Copyright Licensing Agency Ltd, 90 Tottenham Court Road, London, England W1T 4LP. Applications for the copyright holder’s written permission to reproduce any part of this publication should be addressed to the publisher. Permissions may be sought directly from Elsevier’s Science and Technology Rights Department in Oxford, UK: phone: (+44) (0) 1865 843830; fax: (+44) (0) 1865 853333; e-mail: [email protected] You may also complete your request on-line via the Elsevier homepage (http://www.elsevier.com), by selecting ‘Customer Support’ and then ‘Obtaining Permissions’. British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library Library of Congress Cataloguing in Publication Data A catalogue record for this book is available from the Library of Congress ISBN

0 7506 6849 0

For information on all Elsevier Butterworth-Heinemann publications visit our website at http://books.elsevier.com Typeset by Newgen Imaging Systems (P) Ltd., Chennai, India Printed and bound in Great Britain

Working together to grow libraries in developing countries www.elsevier.com | www.bookaid.org | www.sabre.org

viii

Scaling of Structural Strength

9.8

Size Eﬀect Law Anchored in Both Small and Large Size Asymptotics . . . . . . . . . . . . . . . . . . . . . . . . . Recapitulation . . . . . . . . . . . . . . . . . . . . . . . .

213 215

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale . . . . . . . . . . . . . . . . . . . . . . . . . . . .

219

9.9 10

10.1. Scaling of Dislocation Based Strain-Gradient Plasticity 10.2. Scaling of Original Phenomenological Theory of Strain-Gradient Plasticity . . . . . . . . . . . . . . . 10.3. Scaling of Strain-Gradient Generalization of Incremental Plasticity . . . . . . . . . . . . . . . . . 10.4. Closing Observations . . . . . . . . . . . . . . . . . . 11

. . .

219

. . .

228

. . . . . .

236 237

Future Perspectives . . . . . . . . . . . . . . . . . . . . . . . . .

239

Addendum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A1. Size Eﬀect Derivation by a New Method for Asymptotic Matching . . . . . . . . . . . . . . . . . . . . . . . . . . . A2. Size Eﬀect of Finite-Angle Notches . . . . . . . . . . . . . A3. Size Eﬀect on Flexural Strength of Fiber-Composite Laminates . . . . . . . . . . . . . . . . . . . . . . . . . . A4. Size Eﬀect in Fracture of Closed-Cell Polymeric Foam . . . A5. Variation of Cohesive Softening Law Tail in Boundary Layer of Concrete . . . . . . . . . . . . . . . . . . . . . . A6. Can Fracture Energy Be Measured on One-Size Specimens with Diﬀerent Notch Lengths? . . . . . . . . . . . . . . . . A7. Notched–Unnotched Size Eﬀect Method and Standardization of Fracture Testing . . . . . . . . . . . . . . . . . . . . . . A8. Designing Reinforced Concrete Beams against Size Eﬀect . . A9. Scaling of Probability Density Distribution (pdf) of Failure Load . . . . . . . . . . . . . . . . . . . . . . . . . A10. Recent Debates on Fractal Theory of Size Eﬀect and Their Impact on Design Codes . . . . . . . . . . . . . . . . A11. Boundary Layer Size Eﬀect in Thin Metallic Films at Micrometer Scale . . . . . . . . . . . . . . . . . . . . . . . A12. Size Eﬀect on Triggering of Dry Snow Slab Avalanches . . .

241 241 249 252 254 255 258 260 262 264 264 265 267

Bibliography . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

269

Subject Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

313

Reference Citation Index

321

. . . . . . . . . . . . . . . . . . . . . . . .

34

Scaling of Structural Strength

0.0

0.0

2 1

2 1 -0.2

Concrete

SiC Ceramic

Gf = 0.041 N/mm -0.4 cf = 15 mm Ba zant & Pfeiffer (1987) -0.6 -0.8 -0.4

0.0

0.4

-0.8

0.4

0.8

0.0

Gf = 0.49 N/mm cf = 0.83 mm Ba zant & Zhou (2003) -1.2 0.0 0.4 0.8 1.2

1.6

2.0

0.0

log (σN / σ0)

Al Alloy

-0.2

Gf = 117 N/mm cf = 11.6 mm Ba zant, Lee, Pfeiffer

-0.4

-0.3

- 0.1

Limestone

-0.2

-0.2

1 Gf = 0.061 N/mm cf = 9.3 mm 2 Baz ant, Gettu & Kazemi (1991) -0.5 0.0

-0.4

0.0

-0.6

-0.4

-0.2

2

Marti (1989)

-1.0

-0.5

-0.5

fast medium slow Ba zant & Gettu (1992)

-0.7 -0.6 0.0

-0.2

Concrete

-0.2

0.2

0.6

2 1

-0.2

Concrete

Gf = 0.041 N/mm -0.4 cf = 15 mm Bazant & Pfeiffer (1987) -0.6 -1.0 -0.6 -0.2

1.0

0.5

0.0

0.0 2

1

1 -0.3

0.0

Double Punch

0.0

2 -0.1

2

Concrete

1

1

(1987) -0.3 -1.2 -0.8

2

0.0

2 -0.1

1

Gf = 0.109 N/mm cf = 17 mm -0.2 Ba zant, Prat & Tabbara (1990)

-0.8

0.0

0

1 -0.1

Vinyl Foam

-0.4

-1.5 -1

0.0 1

-0.4

Gf = 252 N/mm cf = 6.09 mm Ba zant, Daniel, Li (1996)

-0.4 -1.2

0.6

1

2 1

Carbon Composite

D ≤ 80 m

2

J. Dempsey et al. (1993) Arctic Ocean

0.0

2

Sea Ice

-1.0

-0.4 Gf = 0.039 N/mm cf = 1.36 mm McKinney & Rice -0.6 (1981) -0.2 0.2

0.0

-0.2

-0.5

-0.2

Concrete

0.2

G = 0.041 N/mm -0.4 c f = 15 mm f Ba zant & Pfeiffer (1987) -0.6 0.6 -0.8 -0.4 0.0

0.4

0.8

2 1

-0.4

SiO 2 Ceramic

Gf = 0.009 N/mm cf = 0.61 mm McKinney & Rice -0.8 (1981) -0.2 0.2 0.6

1.0

log (D / D0)

Figure 2.6: Nominal strength data and their ﬁts by size eﬀect law for notched specimen tests of carbon-epoxy composites (Baˇzant, Daniel and Li 1996), sea ice (Dempsey et al. 1999; record size range, up to 80 × 80 × 1.8 m), SiC and Si)O2 ceramics (McKinney and Rice 1981); Indiana limestone (Baˇzant, Gettu and Kazemi 1991), vinyl foam Divinycell 100 (Baˇzant and Zhou 2003), normal concrete (Baˇzant and Pfeiﬀer 1987, Baˇzant, Prat and Tabbara 1990) and tough aluminum alloy (Baˇzant, Lee and Pfeiﬀer 1987); all tests are in mode I except the cylinder test, which is in mode III

228

Scaling of Structural Strength

10.2. Scaling of Original Phenomenological Theory of Strain-Gradient Plasticity The development of strain-gradient plasticity for micrometer scale was pioneered by Fleck and Hutchinson (1993). Their ﬁrst version, called the couple-stress theory (CS theory), was later improved under the name of stretch and rotation gradients theory (SG theory) (Fleck and Hutchinson 1997). In this section, which closely follows the exposition in Baˇzant and Guo (2002a), the scaling of this, by now classical, theory, will be examined.

Fleck and Hutchinson’s Formulation In CS and SG theories, the strain energy density W is assumed to depend on the strain gradient tensor η of components ηijk ≡ uk,ij as well as the linearized strain tensor of components ij ≡ 12 (ui,j + uj,i ) (attention is here restricted to small strains). This assumption comes from the classical work of Toupin (1962) and Mindlin (1965), conﬁned to elastic behavior, and is expressed as 1 W = λii jj + µij ij + a1 ηijj ηikk + a2 ηiik ηkjj 2 + a3 ηiik ηjjk + a4 ηijk ηijk + a5 ηijk ηkji

(10.25)

where λ and µ are the normal Lam´e constants and an are additional elastic stiﬀness constants of the material. As in the classical theory, Cauchy stress σij is deﬁned as ∂W/∂ij , and is work-conjugate to ij . Furthermore, a higherorder stress tensor τ , work-conjugate to the strain gradient tensor η, is deﬁned as τijk = ∂W/∂ηijk . If W is deﬁned by (10.25), the constitutive relation is of course linear. So (10.25) is appropriate to linear isotropic elastic materials only. To extend it to general nonlinear elastic materials, a new variable, an invariant named combined strain quantity, E, is introduced by Fleck and Hutchinson (1997); it is deﬁned as a function of both the strain tensor and the strain gradient tensor, while the strain energy density W is assumed, for general nonlinear elastic material, to be a nonlinear function of E. To deﬁne E, Fleck and Hutchinson (1997) decompose the strain gradient tensor η into its hydrostatic part η H and deviatoric part η ; H ≡ ηijk

1 (δik ηjpp + δjk ηipp ); 4

η = η − ηH

(10.26)

To simplify the problem, only incompressible materials are considered in the H = 0 (which implies devimodeling of metals, in which case ij = ij and ηijk atoric strain gradient ηijk = ηijk ). Furthermore, Fleck and Hutchinson (1997)

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale

229

introduce the orthogonal decomposition η = η (1) + η (2) + η (3)

(10.27)

in which the three tensors are deﬁned in the component form as (1)

S ηijk = ηijk − (2)

1 S S S δij ηkpp + δki ηjpp + δjk ηipp 5

(10.28)

1 eikp ejlm ηlpm (10.29) + ejkp eilm ηlpm + 2ηijk − ηjki − ηkij 6 1 −eikp ejlm ηlpm = − ejkp eilm ηlpm + 2ηijk − ηjki − ηkij 6 1 S S S δij ηkpp + (10.30) + δjk ηipp + δki ηjpp 5

ηijk = (3)

ηijk

Here η S is a fully symmetric tensor deﬁned as S ηijk =

1 ηijk + ηjki + ηkij 3

(10.31)

Using the foregoing three tensors η (i) , Fleck and Hutchinson (1997) deﬁne the combined strain quantity E as E2 =

2 (1) (1) (2) (2) (3) (3) + 21 ηijk ηijk + 22 ηijk ηijk + 23 ηijk ηijk 3 ij ij

(10.32)

where i are three length constants which are given diﬀerent values in the CS and SG theories (which is the only major diﬀerence between these two theories): 5 1 CS (10.33) For CS: 1 = 0, 2 = CS , 3 = 2 24 5 1 CS For SG: 1 = CS , 2 = CS , 3 = (10.34) 2 24 Here CS is called the material characteristic length. Based on the combined strain quantity E as deﬁned, the strain energy density W can be deﬁned as a function of E instead of . Then Cauchy stress tensor σ and the higher-order stress tensor τ (couple stress tensor) can be expressed as: ∂W dW ∂E = ∂ik dE ∂ik ∂W dW ∂E = = ∂ηijk dE ∂ηijk

σik =

(10.35)

τijk

(10.36)

230

Scaling of Structural Strength

Using (10.32) and the condition of incompressibility, one has 2ik ∂E (10.37) = ∂ik 3E (1) (2) (3) ∂E 1 (1) ∂η (2) ∂η (3) ∂η 21 ηlmn lmn + 22 ηlmn lmn + 23 ηlmn lmn = ∂ηijk E ∂ηijk ∂ηijk ∂ηijk =

2CS Cijkmnl ηmnl E

(10.38)

where Cijkmnl is a six-dimensional constant dimensionless tensor which could be determined from (10.28), (10.29), (10.30) and (10.38). Obviously, the CS and SG theories will be characterized by diﬀerent tensors C, although, for each of them, tensor C is constant, that is, independent of , η and CS . For the sake of simplicity, the following power law is assumed for the strain energy density W (Fleck and Hutchinson 1997): n Σ0 E0 W = n+1

E E0

(n+1)/n (10.39)

where Σ0 , E0 and the strain hardening exponent n are taken to be material constants (and, for hardening materials, n ≥ 1; typically n ≈ 2 to 5). Thus (10.35) and (10.36) yield the constitutive relations σik τijk

1/n 1 2 = Σ0 E (1−n)/n ik 3 E0 1/n 1 = Σ0 2CS E (1−n)/n Cijklmn ηlmn E0

(10.40) (10.41)

The principle of virtual work yields the following ﬁeld equations of equilibrium (Fleck and Hutchinson 1997): σik,i − τijk,ij + fk = 0

(10.42)

Dimensionless Variables To analyze scaling, conversion to dimensionless variables (labeled by an overbar) is needed. Among many possible sets of such variables, the following

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale

231

will be convenient: x ¯i = xi /D, η¯ijk

u ¯i = ui /D, ¯ij = ij , = ηijk D, f¯k = fk D/σN

τ¯ijk = τijk /(Σ0 CS ), (l)

(l)

η¯ijk = ηijk D

where

σ ¯ik = σik /Σ0 ,

(10.43) E¯ = E

l = 1, 2, 3

(10.44) (10.45)

Here D is the characteristic length of the structure and σN is the nominal strength. Using these dimensionless variables, the constitutive law of the SGP theory can be rewritten as: 1/n 2 1 (10.46) σ ¯ik = E¯(1−n)/n ¯ik 3 E0 1/n CS 1 τ¯ijk = (10.47) Cijklmn E¯(1−n)/n η¯lmn E0 D The ﬁeld equations of equilibrium transform as ∂i σ ¯ik −

CS σN ¯ ∂i ∂j τ¯ijk + fk = 0 D Σ0

(10.48)

¯i = derivatives with respect to the dimensionless coordinates. where ∂i = ∂/∂ x After substituting (10.46) and (10.47) into (10.48), we obtain the diﬀerential equations of equilibrium in the form: 1/n 2 1 ∂i E¯(1−n)/n ¯ik 3 E0 2 1/n CS 1 σN ¯ − ∂i ∂j Cijklmn E¯(1−n)/n η¯lmn = − fk (10.49) D E0 Σ0 To avoid struggling with the formulation of the boundary conditions, consider ﬁrst that they are homogeneous, i.e., the applied surface tractions and applied couple stresses vanish at all parts of the boundary where the displacements are not ﬁxed as 0. All the loading characterized by nominal stress σN is applied as body forces fk whose distributions are assumed to be geometrically similar; σN is considered as the parameter of these forces, all of which vary proportionally to σN . Then the transformed boundary conditions are also homogeneous. In terms of the dimensionless coordinates, the boundaries of geometrically similar structures of diﬀerent sizes are identical. When the structure is not at maximum load but is hardening, one must decide which are the σN values that are comparable. What is meaningful is to compare structures of diﬀerent sizes for the same dimensionless displacement ﬁeld u ¯k . Thus, the comparable structures will have same ¯ik and η¯ijk .

232

Scaling of Structural Strength

Scaling and Size Eﬀect The problem of scaling and size eﬀect can now be fully discussed. The limit D/CS → ∞ is simple because the dimensionless third-order stresses τ¯ijk vanish and all the equations reduce to the standard ﬁeld equations of equilibrium on the macroscale. The combined strain quantity E reduces to the classical eﬀective strain, and (10.39) becomes the normal strain energy density function. The opposite asymptotic behavior for D/CS → 0 is a little more complex. From (10.32) we know that when D/CS → 0, 2 1 (1) (1) (2) (2) (3) (3) E¯ = ij ij + 2 21 η¯ijk η¯ijk + 22 η¯ijk η¯ijk + 23 η¯ijk η¯ijk ∝ D−1 (10.50) 3 D It is useful to deﬁne another dimensionless variable as follows:

(1) (1) (2) (2) (3) (3) ¯ = 1 H 21 η¯ijk η¯ijk + 22 η¯ijk η¯ijk + 23 η¯ijk η¯ijk CS

(10.51)

¯ is independent of size D, and we have Obviously H CS ¯ H E¯ ≈ D

when D/CS → 0

(10.52)

After substituting (10.52) into (10.49), we obtain the diﬀerential equations of equilibrium in the form: (1−n)/n 1/n 2 CS 1 ¯ (1−n)/n ¯ik ∂i H 3 D E0 (1+n)/n 1/n CS 1 ¯ (1−n)/n η¯lmn − ∂i ∂j Cijklmn H D E0 σN ¯ (10.53) =− fk Σ0 Now we multiply this equation by (D/CS )(n+1)/n and take the limit of the left-hand side for D → 0. This leads to the following asymptotic form of the ﬁeld equations: ∂i ∂j

¯ (1−n)/n η¯lmn = χf¯k , Cijklmn H

1 σ N with χ = E¯0n Σ0

D CS

n+1 n

(10.54)

Since D is absent from the foregoing ﬁeld equation (and from the boundary conditions, too, because they are homogeneous), the dimensionless displacement ﬁeld as well as the parameter χ must be size independent. Thus we obtain the following small-size asymptotic scaling law for Fleck and Hutchinson’s theories

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale

of gradient plasticity: σN or

−1/n = Σ0 χE¯0

CS D

233

(n+1)/n

σN ∝ D−(n+1)/n

(10.55) (10.56)

For hardening materials, we have 1 < (n + 1)/n ≤ 2. Since the surface loads may be regarded as the limit case of body forces applied within a very thin surface layer, the same scaling law must also apply when the load is applied at the boundaries. Although the result (10.56) applies only to the special case of strain energy density function (10.39), the same analytical technique can be used for general strain energy functions. Equation (10.56) indicates that the asymptotic behavior on the microscale depends on the hardening relation on the macroscale since the macro-strain-hardening exponent n is involved. Moreover, the asymptotic behavior depends only on that exponent. Generally, the present technique can be used for any strain energy function deﬁned in terms of the strain and strain gradient tensors, even if no combined strain quantity were deﬁned. For example, a similar technique can also be used for the strain energy density function (10.25) deﬁned for linear isotropic elastic material for which the combined strain quantity is not used. The constitutive relation in that case is: ∂W σik = = λδik ll + 2µik = (2µδil δkm + λδik δlm ) lm ∂ik = Diklm lm ∂W τijk = = [2a1 δil δjk δlm + a2 (δin δjk δlm + δij δkl δmn ) (10.57) ∂ηijk + 2a3 δij δlm δkn + 2a4 δil δjm δkn + 2a5 δin δjm δkl ]ηlmn =

Cijklmn ηlmn

(10.58)

where the dimension of tensor Diklm is that of a stress, and the dimension of tensor Cijklmn is that of a force. The dimensionless variables deﬁned in (10.43) can again be adopted. In terms of the dimensionless variables, the diﬀerential equations of equilibrium are: 1 1 1 ∂i (Diklm ¯lm ) − 3 ∂i ∂j Cijklmn η¯lmn + f¯k σN = 0 (10.59) D D D ¯ will vanish and (10.59) will become the For suﬃciently large D, the term with η classical diﬀerential equation of equilibrium. For the opposite case, for which

234

Scaling of Structural Strength

D is suﬃciently small, the term with ¯ will vanish, and we get the following asymptotic behavior: σN ∝ D−2

(10.60)

Of course, (10.60) is a special case of (10.56) because, for a linear material, the strain hardening exponent n = 1.

Examples It is instructive to verify the scaling law in (10.56) for the basic types of experiments. One important test is that of micro-torsion. It was initially the size eﬀect in this test (Fleck et al. 1997) which motivated the development of gradient plasticity. An eﬀective stress measure Σ may be deﬁned as the work conjugate to E: Σ=

dW (E) dE

(10.61)

A simple power law relationship between Σ and E may be adopted; Σ = Σ0 E N

(10.62)

Compared with (10.39), one sees that N = 1/n. For the analysis of size eﬀect, the radius of the wire, D, may be chosen as the characteristic dimension (size). The deformation is characterized by the twist per unit length, κ. For geometrically similar structures of diﬀerent sizes, we compare the nominal stresses corresponding to the same dimensionless twist κ ¯ = κD. The nominal stress σN may be deﬁned as T /D3 , where T is the torque. If the CS theory is used, one has 1 2 (N +3)/2 N +3 T 6π CS CS Σ0 κ + σN = 3 = (10.63) ¯N − 3 D N +3 D D For CS /D → ∞,

1 + 3

CS D

2 (N +3)/2 N +3 N +3 2 D CS CS N +3 − ≈ D 2 3CS D

(10.64)

σN ∝ D−N −1 = D−(n+1)/n

(10.65)

from which

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale

235

Small-Size Asymptotic Load-Deﬂection Response For some special cases such as the pure torsion of a long thin wire or the bending of a slender beam, the displacement distribution can be ﬁgured out by the arguments of symmetry and the relative displacement proﬁle remains constant during the loading process. For such problems, the asymptotic loaddeﬂection curve for a very small size D can be determined very easily (Baˇzant 2001, 2002). For such loading, all the dimensionless displacements u ¯k at all the points in a structure of a ﬁxed geometry increase in proportion to one parameter, w, such that u ¯k = wˆ uk where u ˆk is not only independent of D but also invariable during the proportional loading process. Parameter w may be deﬁned as the displacement norm, w = u ¯k . From (10.31), (10.28), (10.29), (10.30) and (10.32), we know that E¯ = wEˆ

(10.66)

where Eˆ is a function of dimensionless coordinates that does not change during the loading process when size D is very small. Substituting this into the dimensionless constitutive law (10.46) and (10.47), we have σ ¯ik = w1/n σ ˆik ,

τ¯ijk = w1/n τˆijk

(10.67)

where σ ˆik and τˆijk are constant during the loading process if the size D is small enough. Thus the load fk can now be expressed as a function of w as well as the size D. Since the ﬁrst two terms on the left-hand side of (10.48) are proportional, respectively, to the functions w1/n D(n−1)/n ,

w1/n D−(n+1)/n

(10.68)

one reaches the conclusion that f¯k ∝ w1/n

(10.69)

For hardening materials, we have 1/n ≤ 1. So the load deﬂection curve begins with a vertical tangent, similar to the MSG theory. We conclude that the smallsize asymptotic load-deﬂection response is similar to the stress–strain relation for the macroscale, except that the initial elastic response gets wiped out when D → 0.

236

Scaling of Structural Strength

10.3. Scaling of Strain-Gradient Generalization of Incremental Plasticity Finally, a brief look at the theory of Acharya and Bassani (2000) and Bassani (2001) is appropriate. These authors developed a simple gradient theory which diﬀers signiﬁcantly from the previous four theories. It is a generalization of the classical incremental theory of macro-scale plasticity, rather than the deformation (total strain) theory. In contrast to the previous four theories, in which the strain gradient tensor η is deﬁned as a third-order tensor representing the gradient of total strain, the lattice incompatibility is measured by a second-order tensor deﬁned by the following contraction of the gradient of plastic strain pij : αij = ejkl pil,k (10.70) where ejkl is the alternating symbol. The plastic hardening is assumed to be governed by the invariant: α = 2αij αji (10.71) Then the basic equations of the classical J2 ﬂow theory are modiﬁed as follows: σ σij ij τ= (10.72) = τcr , τ˙ = τ˙cr = h(γ p , α)γ˙ p 2 p 2 p p γ˙ p p p σij , σ˙ ij = Cijkl (˙kl − ˙kl ), γ = ˙ij = (10.73) 2τ 3 ij ij The variables used in the above are almost the same as in the classical J2 ﬂow theory except that the instantaneous hardening-rate function h depends not only on plastic strain invariant γ p but also on α. The following hardening function h(γ p , α) is used by Bassani (2001) for numerical simulation of the micro-torsion test: p 1/2 N −1 γ l2 (α/γ0 )2 1+ h(γ p , α) = h0 +1 (10.74) γ0 1 + c(γ p /γ0 )2 where l is a material length introduced for dimensionality reasons, and h0 , γ0 , c and N are further material constants (all positive). Although a full analysis of scaling of this theory is beyond the scope of this paper, some simple observations can be made. From the scale transformations u ¯i = ui /D, ¯il,k = il,k D, it follows that αij = α ¯ ij /D, where the overbars again denote the dimensionless variables. Since γ¯ p = γ p , the plastic hardening modulus deﬁned by (10.74) scales for D → 0 as p N −1 −1/2 α γ ¯ l h(γ p , α) = h0 1 + c(γ p /γ0 )2 +1 (10.75) ∝ D−1 γ0 γ0 D

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale

237

This means that, at the same strain level, the slope of the plastic hardening curve increases as D−1 when D → 0. When the plastic strain becomes much larger than the elastic strain, and when the strain distributions and history are similar, then of course the nominal stress σN must also scale asymptotically as D−1 . This is again a curiously strong asymptotic size eﬀect, not much less strong than that found for the MSG and CS theories. Even though this excessive size eﬀect is approached only outside the range of applicability of the theory, one must expect that it would impair the representation of test data in the middle range. The excessive asymptotic size eﬀect could be avoided by redeﬁning the plastic hardening modulus in (10.74) as follows: h(γ p , α) = h0

1/2 N −1 γp lα/γ0 1+ +1 γ0 1 + c(γ p /γ0 )

(10.76)

With this revision, which should be checked against test data, the asymptotic scaling would become h(γ p , α) ∝ D−1/2

when D → 0

(10.77)

which seems more reasonable and similar to Baˇzant’s (2000) proposal for revision of MSG theory, as well as to the TNT theory.

10.4. Closing Observations The small-size asymptotic scaling laws for the nominal stress σN in all the existing theories are power laws, but there are wide disparities among them. For Gao et al.’s (1999) MSG theory, in general, σN ∝ D−5/2 , which is an unreasonably strong size eﬀect. For two special cases of this theory, σN ∝ D−2 and D−3/2 , which is also very strong. For the classical Fleck and Hutchinson (1963, 1997) CS and SG theories, σN ∝ D−(n+1)/n where n is the exponent of the strain hardening law on the macroscale, and typically σN ∝ D−1.3 , which is also quite strong. For the TNT theory, as well as for the modiﬁcation of the MSG theory proposed by Baˇzant (2002, 2000), σN ∝ D−1/2 , which seems reasonable. The plastic hardening modulus in the theory of Acharya and Bassani (2000) scales asymptotically as D−1 , which also seems excessive. However, a simple modiﬁcation can achieve the scaling of D−1/2 .

238

Scaling of Structural Strength

Although the small-size asymptotic behavior is closely approached only at sizes much smaller than the range of applicability of the strain-gradient theories of plasticity (which is about 0.1 µm–100 µm), the knowledge of this behavior is useful for developing asymptotic matching approximations for the realistic middle range. Knowledge of both the large-size and small-size makes it possible to obtain good analytical approximations for the middle range of interest, agreeing with experimental as well as numerical results (see Baˇzant and Guo 2002a). The availability of such formulae means that the stress analysis for the middle range, which is much more diﬃcult than the asymptotic analysis, can in principle be avoided. Such an approach is, of course, possible only if the small-size asymptotic behavior is realistic. The detrimental consequence of unrealistic small-size asymptotic properties is that the possibility of asymptotic matching approximations is lost.

Addendum Most of the manuscript for the ﬁrst printing was completed in 2000. Since then research in strength scaling has been progressing rapidly; recent advances are brieﬂy described in this Addendum, and some additional references are added at the end of the bibliography. A1. Size Eﬀect Derivation by a New Method for Asymptotic Matching Summary of asymptotic properties of cohesive crack model A simpler, more general and more fundamental derivation of the scaling laws can be obtained by combining dimensional analysis with a new method of asymptotic matching of the known asymptotics of the cohesive crack model (Baˇzant 2004a). Asymptotic matching is a broad range of diverse techniques used for a long time in ﬂuid mechanics (Barenblatt 1996, 2003), none of which, however, seems suited for fracture mechanics of solids. The basic hypothesis is that the cohesive crack model represents a good enough compromise between reality and simplicity. The fracture process zone (FPZ) at the crack front is modeled as a ﬁctitious line crack transmitting cohesive (crack-bridging) stresses σ = f (w); w = crack opening (separation), f (w) = monotonically decreasing (softening) function characterizing the material (Fig. A.1 bottom left), with f (0) = ft = tensile strength of material. The initial tangent of f (w) is assumed to have a ﬁnite negative slope f (0), which is proportional to fracture energy Gf . In Chapter 2 and 9 it was shown that, depending on the ﬁrst two non-zero terms of the asymptotic expansions of σN in terms of powers of D and of D−1 , there exist three and only three types of size eﬀect (Baˇzant 2001): For D → 0 : σN = b0 − c0 D + · · · For D → ∞: σN = b1 + c1 D−1 + · · · σN = D

−1/2

σN = D

−1/2

(all types)

(A1.1)

(type 1)

(A1.2)

[b2 − c2 D

−1

+ · · · ] (type 2)

(A1.3)

[b3 − c3 D

−2

+ · · · ] (type 3)

(A1.4)

where b0 , c0 , . . . , c3 are positive constants determined by structure geometry. Type 1 (Fig. A.1 left) occurs if the geometry is such that Pmax is reached at crack initiation from an FPZ attached to a smooth surface, i.e., as soon as the FPZ is fully formed. Type 2 (Fig. A.1 right) occurs if there is a large notch or preexisting stress-free (fatigued) crack and if the geometry is positive, i.e., such

242

Scaling of Structural Strength

1

Type 1

log(σN/σ0)

r

Type 3

1

FM LE

1

Type 2 0.1

Weibu m n ll 1

10

100

2 1

0.1 0.1

1

10

100

log (D/D0) Figure A.1: Size eﬀects of types 1, 2, and 3, and their asymptotes

that Pmax occurs while the FPZ is still attached to the tip. Type 3 occurs if a large crack can grow stably prior to Pmax (negative geometry). The size eﬀect types 1 and 2 are very diﬀerent, but types 2 and 3 are quite similar and hardly distinguishable in fracture testing (note that, in Chapter 9, type 1 was called Case 2, type 2 Case 1, and type 3 Case 3).

Asymptotic matching law for the case of large notch or crack From Buckingham’s Π-theorem of dimensional analysis (Barenblatt 1979), two special size eﬀects have been proven in section 1.7:

(a) If the failure depends on ft (dimension N/m2 ) but not Gf , then there is no size eﬀect, i.e., σN = constant (this is so for all elasto-plastic failures). (b) If the failure depends on Gf (dimension J/m2 ) but not on ft , then there is a size eﬀect of the type σN D−1/2 (this is so for LEFM, if the cracks or notches are geometrically similar).

Addendum

243

Nothing more can be deduced from dimensional analysis alone. We can, however, deduce more information upon considering the physical meaning of the material characteristic length governing the FPZ size, l0 = EGf /ft2 , introduced by Irwin (1958). The length and width of the FPZ for D → ∞ are ηl0 and η l0 , in which η and η are constants of the order of 1, depending on microstructure characteristics (note that the parameter le = Gf /E, which is also a length, is irrelevant for failure and controls only the ratio of deformation to stress intensity factor KI in LEFM). Depending on the ratio D/l0 , two asymptotic cases may be distinguished: (a) If D/l0 → 0, the body is much smaller than a fully developed FPZ. Then a derivative of potential energy with respect to the crack length makes no sense, and so Gf cannot matter. Therefore, the case of no size eﬀect, σN = constant, is the small-size asymptote. (b) If D/l0 → ∞, the FPZ becomes a point in dimensionless coordinates ξ = x/D and the stress ﬁeld approaches the LEFM singularity. So, ft cannot matter. Therefore, the LEFM scaling, σN ∝ D−1/2 , is the largesize asymptote of quasibrittle failure (which is represented by a straight line of slope −1/2 in the plot of log σN versus log D). The size eﬀect curve for the intermediate sizes may be expected to be a gradual transition between these two asymptotes. The approximate form of this transition can be deduced upon noting how the asymptotes are approached, i.e., by exploiting the higher-order asymptotic terms in (A1.1) and (A1.3). By transformation to dimensionless variables in the formulation of the boundary value problem with cohesive crack, one concludes that (if the ratios of structural dimensions characterizing the structure geometry are ﬁxed) σN depends on only three parameters, ft , D and Kc , where, for plane stress states, Kc =(EGf )1/2 = mode I fracture toughness and E = Young’s modulus (for plane strain states, E needs to be replaced by E = E/(1 − ν 2 ) where ν = Poisson ratio). Therefore, we have now four governing parameters, σN , D, ft and Kc . Since they involve 2 independent physical dimensions (length and force), the Π-theorem (Barenblatt 1979) implies that there can be only 4 − 2, i.e., 2 independent dimensionless parameters, Π1 and Π2 . So, the equation governing failure may be written as F (Π1 , Π2 ) = 0 where function F may be assumed to be suﬃciently smooth. Although many diverse choices of Πi (i = 1, 2) are possible, the key idea was to make a choice for which, in each asymptotic case, all Πi vanish except one (Baˇzant 2004a). If consideration is limited to dimensionless monomials, this can be most generally achieved by choosing: Π1 = (σN /ft )p (D/l0 )u ,

Π2 = (σN /ft )q (D/l0 )v

where p, q, u, v are four unknown real constants.

(A1.5)

244

Scaling of Structural Strength

If we let Π1 = 0 correspond to D → 0, then F (0, Π2 ) = 0. This implies that Π2 = constant or σN q Dv = constant for D → 0, which must be the case of no size eﬀect; hence v = 0. If we let Π2 = 0 correspond to D → ∞, then F (Π1 , 0) = 0, which implies that Π1 = constant or σN p Du = constant, or σN ∝ D−u/p for D → ∞. This must be the LEFM scaling; hence u/p = 1/2 or u = p/2. To ﬁnd p and q, we expand function F into Taylor series about the state Π1 = Π2 = 0, and truncate this series after the linear terms; i.e., F (Π1 , Π2 ) ≈ F0 + F1 Π1 + F2 Π2 = 0 √ or F1 (σN D/ft l0 )p + F2 (σN /ft )q = −F0

(A1.6) (A1.7)

where F1 = [∂F/∂Π1 ]0 and F2 = [∂F/∂Π2 ]0 (evaluated at Π1 = Π2 = 0) and F0 = F (0, 0) (F0 , F1 , F2 = 0). Now we need to compare the last equation with the asymptotic expansion in (A1.3). But this cannot be done in general because, for general p/q, the last equation cannot be solved explicitly for σN . But it can be solved for D, which gives 2/p

D = l0 ft 2 (−F0 /F1 )2/p σN −2 [1 + (F2 /F0 ftq )σN q ]

(A1.8)

which may be compared to the inverse expansion of the large-size asymptotic expansion in (A1.3). This inverse expansion has the form D = B2 σN −2 [1 − C2 σN 2 + · · · ]

for σN → 0

(A1.9)

where B2 and C2 are positive constants. Evidently, matching of the ﬁrst two terms of this expansion requires that p = q = 2. Then Eq. (A1.7) can be solved for σN . This yields, and veriﬁes, the size eﬀect law, Eq. (2.8), i.e., σN = σ0 ( 1 + D/D0 )−1/2 in which

Bft = ft (−F0 F2 )−1/2 ,

D0 = l0 F2 /F1

(A1.10) (A1.11)

For D → 0, Eq. (2.8) has the approximation: σN ≈ Bft (1 − D/2D0 )

(A1.12)

which veriﬁes that the form of the second term of small-size expansion in (A1.1) can be matched, too. So, Eq. (A1.10) is the simplest formula for type 2 size eﬀect that can match the form of four asymptotic terms, two for D → 0 and two for D → ∞. If, however, not only the form of the second-order terms but also the values of all four coeﬃcients b0 , c0 , b2 , c2 are given, a slightly more general formula with four adjustable parameters is needed. This formula was recently developed and examined in Baˇzant and Yu (2002), with the purpose of a identifying fracture

Addendum

245

energy Gf from the maximum load of notched and unnotched test specimens of relatively small sizes. More complex formulas of the same asymptotic accuracy, but more ﬂexible in data ﬁtting, can be obtained by replacing (A1.5) with dimensionless polynomials (or other monotonic functions of Π1 and Π2 ). Such formulas can make a signiﬁcant diﬀerence only if the size eﬀect needs to be modeled for a size range exceeding about 1 21 order of magnitude of D. Their merit is that they can capture a spectrum of fracture energies (Baˇzant 2002f), each of which is associated with a diﬀerent order of magnitude of D (see section 9.7). The type 3 (Case 3) size eﬀect formula (Fig. A.1 right) can be derived similarly. Asymptotic matching law for failures at crack initiation (type 1 scaling) The deterministic (type 1) size eﬀect for failures at macrocrack initiation from a smooth surface necessitates a somewhat diﬀerent approach. As explained in section 2.8 (Fig. 2.13), the source of this size eﬀect is the stress redistribution due to a boundary layer of cracking (or formation of the FPZ at the surface), which is associated with energy release. The deterministic type 1 size eﬀect is also called the strain gradient eﬀect, but this is not quite accurate because, aside from the local strain gradient at the surface, the geometry of the whole structure also has some (albeit small) inﬂuence on the strain redistribution and energy release. This is clear from the alternative approach used in section 2.7, in which the type 1 failure has been treated as a limit case of ﬁnite crack for a0 → 0 (Baˇzant 1997, 1998), with the energy release rate approaching zero. For general dimensional analysis, we need a slightly diﬀerent procedure than for type 2. Let us consider the deterministic type 1 ﬁrst (m → ∞). Because, according to (A1.1) and (A1.2), both asymptotes in the plot of log σN versus log D must be horizontal, the size eﬀect curve of σN versus log D must have an inﬂexion point. Thus it is convenient to postulate the existence of what is called an intermediate asymptote (Barenblatt 1979, 2003), which consists of some unknown power law. Because the intermediate asymptote separates the large-size and small-size asymptotics, we must ﬁrst match the large-size asymptotic terms alone (which was the approach taken in sections 2.7 and 9.4.2). We choose the large-size asymptote to correspond to Π1 = 0, i.e., to F (0, Π2 ) = 0. This requires that Π2 = constant for D → ∞, and so v = 0 in (A1.5). We again truncate the Taylor series expansion of function F (Π1 , Π2 ) after the linear terms, i.e., use the linear approximation (A1.6). This equation cannot, in general, be solved

246

Scaling of Structural Strength

for σN , but it can for D, which yields: l0 /D = (−F0 /F1 )−1/u [(ft /σN )p + (F2 /F0 )(ft /σN )p−q ]−1/u

(A1.13)

The large-size expansion (A1.2) may be generalized as σN = (b1 + rc1 D−1 + · · · )1/r (r = arbitrary constant = 0). Although we cannot match the asymptotic expansion (A1.2) directly, we can match the inverse expansion, which can be shown to be 1/D = (−b1 + σN r + · · · )/rc1

(A1.14)

Matching of (A1.13) obviously requires that u = −1 and p = q = −r in (A1.5). So (A1.15) Π1 = (ft /σN )r l0 /D, Π2 = (ft /σN )r With these particular expressions, Eq. (A1.6) can be solved for σN . This yields, and thus also veriﬁes, the type 1 size eﬀect law 1/r

σN = fr0 (1 + rλ/D)

(type 1, m → ∞)

(A1.16)

(equivalent to Eq. 2.39), in which λ = F1 /rF2 ,

fr0 = ft (−F2 /F0 )1/r

(A1.17)

Second, consider the statistical generalization, i.e., Weibull modulus m < ∞. Instead of the horizontal asymptote (A1.1), the mean large-size asymptotic size eﬀect (as explained in section 3.1, Eq. 3.6) is now given by the Weibull power law (A1.18) for D → ∞ : σN = k0 D−n/m + · · · (type 1) where m = Weibull modulus, k0 = constant, and n = number of dimensions in which the structure is scaled (n = 1, 2, 3); typically, m = 10 to 40 and n/m 1. In the plot of log σN versus log D, this power law represents an inclined straight line asymptote of slope −n/m. The Weibull power law size eﬀect (A1.18) must apply for failures at crack initiation if the FPZ is negligible compared with D. We again choose the large size asymptote to correspond to Π1 = 0 and Π2 = constant. To match (A1.18), it is necessary that σN = C1 D−n/m ∝ ft (D/l0 )−v/q , and so, v/q = n/m. If we should not loose the deterministic limit already ﬁgured out, we must keep p = q = −r and u = −1. With these values, Eq. (A1.6) can now be solved for σN . This leads to the mean type 1 energetic-statistical size eﬀect: 1/r σN = fr0 (λl0 /D)rn/m + rκ(λl0 /D) (A1.19) equivalent to Eq. 3.9; here fr0 = λ−n/m (−F2 /F0 )1/r , κ = λrn/m−1 F1 /F2 r, and r is a parameter of the order of 1, sensitive to structure geometry. For

Addendum

247

large D, the ﬁrst term dominates, and so σN ∝ D−n/m , which agrees with the asymptotic requirement in (A1.18). Furthermore, for m → ∞, the asymptotic scaling of Eq. (A1.2) is matched because Eq. (A1.19) takes the form σN = s0 (1 + κrλl0 /D)1/r ≈ s0 (1 + κλl0 /D). Eq. (A1.19), however, is separated by the intermediate asymptote from the small-size asymptotics in (A1.1), and does not match that asymptotics. It must, therefore, be further modiﬁed, but without aﬀecting the ﬁrst two large-size asymptotic terms. To bridge the small-size and intermediate asymptotes, we could engage in similar arguments as we did for bridging the large-size and intermediate asymptotes. Suﬃce to say, the complete law for the mean size eﬀect of type 1 (Fig. A.1 left), matching the small-size asymptotics in (A1.1), can simply be obtained by replacing λl0 /D in Eq. (A1.19) with θ, as follows: 1/rs σN = fr0 θrn/m + rsκθ , θ = (1 + D/sηl0 )−s λ/η (A1.20) where η = positive constant of the order of 1, and s may be taken as 1. Note that the intermediate asymptote is deﬁned by inﬁnite separation of the characteristic lengths involved, ηl0 and λl0 . If we let ηl0 D λl0 , i.e., if we consider the limiting process λ/η → ∞, Eq. (A1.20) converges to an intermediate asymptote, given by the power law σN = fr0 (la /D)1/r

(A1.21)

in which la = sη(rsκλ/η)1/r = constant, and becomes inﬁnitely close to the small-size asymptote of (A1.19), as well as to the large size asymptote of σN = fr0 θn/m (given by Eq. 3.6), which passes through the aforementioned inﬂexion point. The physical reason for the existence of an intermediate asymptote is that normally the size of averaging domain in nonlocal Weibull theory (roughly equal to FPZ width) is much smaller than the FPZ length. Eq. (A1.20) is supported by ﬁnite element simulations with nonlocal Weibull theory, as well as test data from ten diﬀerent labs (all combined in one dimensionless plot in Fig. 3.6). However, test data for concrete and composites show that the D values for which the diﬀerence between (A1.19) and (A1.20) is signiﬁcant are less than the material inhomogeneities, which means that (A1.19) should mostly suﬃce in practice. For bending of laminates or unreinforced concrete beams, the Weibull statistical component in (A1.19) or (A1.20) is usually insigniﬁcant for normal sizes (Baˇzant Zhou, Nov ’ak and Daniel 2004). It becomes signiﬁcant only for bending of very large structures, such as arch dams. For bending of unreinforced concrete beams or plates, for which the size eﬀect is generally of type 1, the Weibull statistical component normally becomes signiﬁcant only for cross sections at least several meters thick (as typical of arch dams).

248

Scaling of Structural Strength

Universal Size Eﬀect Law The size eﬀect for crack initiation from a smooth surface (a0 = 0) has been shown to be very diﬀerent from the size eﬀect for large notches or large stressfree (fatigued) cracks at maximum load (for which a0 /D is not too small). As far as the mean nominal strength of structure, σN , is concerned, the former is always energetic (i.e. purely deterministic), while the latter is purely energetic only for small enough sizes and becomes statistical for large enough sizes. It is of interest to ﬁnd a universal size eﬀect law that includes both of these size eﬀects and spans the transition between them. A formula for this purpose was proposed in Baˇzant and Li (1996) (also Baˇzant and Chen 1997); see Eq. (2.52) and Fig. 2.14. However, that formula is not smooth and does not include the statistical (Weibull) part for crack initiation failures. A better formula (Baˇzant and Yu 2004) is shown in Fig. A.2—on the left (Fig. A.2a) without, and on the right (Fig. A.2b) with, the statistical (Weibull)

Figure A.2: Universal size eﬀect law (improvement of Fig. 2.14); top left—without, and top right—with Weibull statistics; bottom—proﬁles obtained from the universal size eﬀect law, compared to Duan and Hu’s (2003) approximation

Addendum

249

part (E = eﬀective Young’s modulus for plane stress or plane strain), ft = local tensile strength of material; g0 , g0 , g0 are values of dimensionless energy release function g(a) and its derivatives at α0 = a0 /D; l0 = E Gf /f t2 = Irwin’s characteristic length (corresponding to the initial fracture energy Gf ); g(a) = [k(a)]2 , k(a) is the dimensionless stress intensity factor; m = Weibull modulus of concrete (about 24), n = number of dimensions for scaling; r, k = empirical positive constants; and cf = constant (the ratio cf /l0 depends on the softening curve shape, and cf ≈ l0 /2 for triangular softening). The formulas in Figs. F1a,b were derived by asymptotic matching of 7 cases: the small-size and large-size asymptotic behaviors (ﬁrst two terms of expansion for each), of the large-notch and vanishing-notch behaviors, and of Weibull size eﬀect. A2. Size Eﬀect of Finite-Angle Notches In elastic bodies, a sharp notch of a ﬁnite angle (Fig. A.3) causes stress singularity σ ≈ rλ−1 that is weaker than the crack singularity (i.e., λ > 0.5) and is given by Williams’ (1952) formulas (a)–(e) shown in Fig. A.3, in which r, φ = polar coordinates and σ = σrr , σφφ , σrφ = near-tip stresses. If the structure has a positive geometry, it will fail as soon as a FPZ of a certain characteristic length 2cf is fully formed at the notch tip. In the limit of D → ∞, the structure will fail as soon as a crack can start propagating from the notch tip, in which case the critical energy release rate must equal Gf . Experiments show that the load (or nominal stress σN ) at which this occurs increases with angle γ. In previous studies (e.g., Carpinteri 1987, Dunn et al. 1997a,b), some arguments in terms of a non-standard ‘stress intensity factor’ Kγ corresponding to singularity exponent 1−λ < 0.5 were used to propose that the nominal stress σN ∝ Dλ−1 . A notch of ﬁnite angle cannot propagate, and a stress singularity of a power other than 1/2 cannot supply a ﬁnite energy ﬂux. So, a realistic approach requires considering that a cohesive crack must propagate from the notch tip (Fig. A.3 left; Baˇzant and Yu 2004). Circular bodies with notches of various angles 2γ (and ligament dimension D, Fig. A.3a) were simulated by ﬁnite elements with a mesh progressively reﬁned as r → 0 (the ﬁrst and second rings of elements spanned from 0 to r = D/6000 and then to D/3000). The circular boundary was loaded by normal and tangential surface tractions equal to stresses σrr and σrφ taken from Williams symmetric (mode I) solution; P = load parameter representing the resultant of these tractions; and σN = P/bD = nominal stress (b = 1). First, ligament D was considered to be so large that the length of the FPZ, lc , was less than 0.01D. In that case, the angular distribution of stresses along each circle with r ≥ 0.1D ought to match Williams functions frr , frφ , fφφ . Indeed, the numerical results cannot be visually

250

Scaling of Structural Strength

Figure A.3: (a) Angle-notched circular specimen considered for analysis. (b) Numerically computed singularity exponent compared to Williams’ elastic solution. (c) Computed variation of nominal strength with notch angle. (d) Curve of analytical size eﬀect law for angular notches compared to the results of cohesive crack model distinguished from these functions. The logarithmic plots of the calculated stress versus r for any ﬁxed φ (and any γ) were straight lines, and their slopes agreed with the exponent λ − 1 required by Williams solution; see Fig. A.3 (right). This serves to conﬁrm the correctness of the cohesive ﬁnite element simulation. From Eqs. (b), (f), and (g) of Williams’ LEFM solution in Fig. A.3, σN = (r/D)1−λ σφφ ψ(γ)/fφφ (0, γ)

(8)

(A2.1)

According to the equivalent LEFM approximation of cohesive fracture, σφφ for r = cf (the middle of FPZ), should be approximately equal to material tensile strength ft . This condition yields σN = ft (D/Hr )λ(γ)−1 ,

Hr = cf [fφφ (0, γ)/ψ(γ)]

(9)

(A2.2)

Addendum

251

which is for D ≥ 250l0 indistinguishable graphically. Eq. (A1.19), however, violates the small-size asymptotics in (A1.1), and must therefore be further modiﬁed, but without aﬀecting the ﬁrst two large-size asymptotic terms. To bridge the small-size and intermediate asymptotes, we could engage in similar arguments as we did for bridging the large-size and intermediate asymptotes. Suﬃce to say, the complete law for the mean size eﬀect of type 1 (Fig. A.1d), matching the small-size asymptotics in (A1.1), is obtained by replacing λ/D in Eq. (A1.19) with θ: 1/r σN = fr0 θrn/m + rκθ , θ = (1 + D/sη)−s λ/η (A2.3) where η = positive constant of the order of 1 and s may be taken as 1; λ(γ) is the λ value for angle γ. To check this equation, geometrically similar scaled circular bodies of diﬀerent ligament dimensions D (Fig. A.3) were analyzed by ﬁnite elements for various angles γ using the same linear softening stressseparation diagram of cohesive crack. The numerically obtained values of log σN for various ﬁxed D/cf are plotted in Fig. A.3c as a function of angle γ. We see that this size eﬀect curve matches perfectly the curve of Eq. (A2.2) for D/cf > 500, conﬁrming that the equivalent LEFM approximation obtained for r = cf is good enough. A general approximate formula for the size eﬀect of notches of any angle, applicable to any size D, may be written as follows: λ(γ)−1 H0 D σN = σ0 1 + (A2.4) Hγ D0 where H0 = hγ -value for γ = 0, and D0 is given in terms of g(α) and is the same as for a crack (γ = 0). Eq. (A2.4), which is of course valid only for large enough notches penetrating through the boundary layer of concrete, has been derived by asymptotic matching of the following asymptotic conditions: 1. for γ → 0, the classical size eﬀect law σN = σ0 (1 + D/D0 )−1/2 must be recovered; 2. for D/l0 → 0, there must be no size eﬀect; 3. for D/l0 → ∞, Eqs. A2.4 and A2.2 must coincide; 4. for γ = π/2 (ﬂat surface), the formula must give no size eﬀect for D → ∞. In reality, there is of course a size eﬀect in the last case, but it requires a further generalization of Eq. (A2.4) (which will be presented separately). Therefore, Eqs. (A2.4) and (A2.2) can be applied only when the notch is deeper than

252

Scaling of Structural Strength

the boundary layer, which is at least one aggregate size. Complete generality will require amalgamating Eq. (A2.4) with the universal size eﬀect law in Fig. A.2. The plot of log σN versus log D for γ = π/3 according to Eq. (F28) is compared to the ﬁnite element results for notched circular bodies with cohesive cracks in Fig. A.3d. The agreement is seen to be excellent.

A3. Size Eﬀect on Flexural Strength of Fiber-Composite Laminates The failure of ﬁber-polymer laminates is in general practice still treated according to the strength theory or plastic limit analysis, which exhibits no size eﬀect, and all the size eﬀects are considered as purely statistical. A recent systematic analysis by Baˇzant, Zhou and Daniel (2003), based on the ﬂexural strength tests of Jackson (1992), Johnson et al. (2000), Wisnom (1991), Wisnom and Atkinson (1997) and others, conﬁrms that such practice in unrealistic. The problem is that if the available size eﬀect data on ﬂexural strength of ﬁber-polymer laminates are considered alone, they can be ﬁtted well enough by Weibull statistical size eﬀect theory. However, to conclude that this theory applies is deceptive for two reasons: (1) the size range of the existing data is quite limited, and the energetic theory for size eﬀect at crack initiation due to a boundary layer can ﬁt these data equally well; and (2) checks of the coefﬁcient of variation of ﬂexural strength, ωW , have been omitted. These checks are essential. Weibull statistical theory cannot be correct if the ωW -value does not agree with the value of Weibull modulus m, and if this agreement is not obtained for every size. The ωW values must satisfy the well-known formula of Weibull theory, Eq. (3.3), i.e., ωW = [(Γ(1 + 2/m))/(Γ2 (1 + 1/m) − 1]−1/2 . Even though the available size eﬀect data for laminate ﬂexure did not include measurements of ωW , it is easy to ascertain that the foregoing equation is not satisﬁed. For example, Jackson et al.’s (1992) tests included four diﬀerent layups—unidirectional, quasi-isotropic, cross-ply and angle ply. To ﬁt these size eﬀect data, the optimum m values vary widely from case to case, ranging from m = 5 to m = 30. According to the foregoing relation, ωW = 22.8% for m = 5,

ωW = 4.18% for m = 30

(A3.1)

for angle-ply and unidirectional laminates, respectively. Although the coeﬃcient of variation of ﬂexural strength has not been reported for the test data considered, such huge diﬀerences in scatter go against all experience, and are evidently implausible. The angle-ply laminate, due to its greater ductility

Addendum

253

Figure A.4: Type 1 size eﬀect plot for Jackson’s data from ﬂexural tests of laminates of four diﬀerent layups, in dimensionless coordinates

(lower brittleness), might be expected to give a somewhat smaller scatter (larger m) than the unidirectional, cross-ply or quasi-isotropic laminate, but the opposite is systematically noted in pure Weibull ﬁtting of the data. Therefore, the classical hypothesis of a purely statistical size eﬀect in ﬂexural strength of laminates is untenable. On the other hand, as shown by Baˇzant, Zhou and Daniel (2003), the data of Jackson can be ﬁtted consistently by the energetic-statistical theory, with the same value of m for all the data; see Fig. A.4 in which the data for various layups are plotted in dimensionless coordinates, after optimal ﬁtting for each individual layup. However, it must further be noted that these data can be ﬁtted about equally well by a purely energetic theory. From this it follows that the Weibull-type statistical part of size eﬀect becomes signiﬁcant only for laminate thicknesses well beyond the normal usage (this observation is similar to that made for ﬂexural strength of concrete, for which the statistical part of size eﬀect becomes important only for concrete thickness found, for example, in arch dams).

254

Scaling of Structural Strength

A further implication is that fracture mechanics, rather than some strength criterion (or material failure criterion expressed in terms of stresses and strains), needs to be used for evaluating the strength of laminates. The fracture analysis of laminates must take into account the quasibrittle (or cohesive) nature of fracture.

A4. Size Eﬀect in Fracture of Closed-Cell Polymeric Foam Very light closed-cell polymeric (vinyl) foam is a favored material for the core of sandwich structures for ships. In classical works (e.g., Gibson and Ashby 1997, Shipsha et al. 2000, Gdoutos et al. 2001), the failure of this material in tension or compression has usually been described as ductile, involving a yield plateau followed by locking, and failure criteria expressed in terms of stresses have been used. Such failure can exhibit no size eﬀect. Such ductile response, however, does not take place when high tensile stress concentrations exist, induced for example by notches in laboratory specimens, or various structural holes or accidental damage of real structures. In such a case, the failure of the foam may be brittle. This was ﬁrst revealed by the notched specimen tests of Zenkert and B¨acklund (1989) in which the fracture toughness of foam was measured, by the tests of holed panels tests by Fleck and co-workers in Cambridge in (2001), and by the ﬁnite element studies of foam based on microplane model for foam by Brocca et al. (2001). Consequently, the foam, when notched or damaged, must be expected to exhibit size eﬀect, and this is what is conﬁrmed by a recent study (Baˇzant, Zhou, Nov´ ak and Daniel 2004), in which the size eﬀect in Divinycell H100 foam, both the case of failure with large cracks or notches (type 1) and failure at crack initiation (type 2). In this study, geometrically similar single edge-notched prismatic specimens of various sizes were tested under tension. The results were shown to agree with Baˇzant’s size eﬀect law. Fitting this law to the test results furnished the values of the fracture energy Gf of the foam as well as the characteristic size cf of the fracture process zone. Fracture analysis based on these properties was shown to match the test data of Fleck, Olurin and co-workers (2001) obtained on dissimilar panels with holes of diﬀerent sizes. These results were also matched using the eigenvalue method for ﬁnite element analysis based on the cohesive crack model with properties corresponding to the size eﬀect law. Finally, compressed foam specimens with V-shaped notches (with an angle wide enough to prevent the notch faces from coming into contact) were found to exhibit no size eﬀect. This implies that the cell collapse at the tip of the notch must be essentially a plastic process rather than a softening damage process.

Addendum

255

The results demonstrate that the current design practice, in which the tensile failure of foam is generally predicted on the basis of strength criteria or plasticity, is acceptable only for small structural parts. In the case of large structural parts, the size eﬀect must be taken into account, especially if the foam can suﬀer large fatigue cracks or large damage zones prior to critical loading to failure.

A5. Variation of Cohesive Softening Law Tail in Boundary Layer of Concrete It has been well established experimentally that the total fracture energy GF of a heterogeneous material such as concrete, deﬁned as the area under the cohesive softening curve, is not constant but varies during crack propagation across the ligament. The variation of GF at the beginning of fracture growth, which is described by the R-curve, is known to be only an apparent phenomenon which is perfectly consistent with the cohesive crack model (with a ﬁxed softening stress-separation law), and can in fact be calculated from it. However, the variation during crack propagation through the boundary layer at the end of the ligament is not consistent with the cohesive crack model and implies that the softening curve of this model is not an invariant property in the boundary layer. The analysis of this problem by Baˇzant and Yu (2004) will now be presented. The fact that the fracture energy representing the area under the softening curve should decrease to zero at the end of the ligament was pointed out in a paper by Baˇzant (1996), motivated by the experiments of Hu and Wittmann (1991 and 1992a), and was explained by a decrease of the fracture process zone (FPZ) size, as illustrated on the left of Fig. A.5a reproduced from Baˇzant’s (1996) paper. An experimental veriﬁcation and detailed justiﬁcation of this property was provided in the works of Hu (1997, 1998), Hu and Wittmann (1992b, 2000), Duan, Hu and Wittmann (2002, 2003), and Karihaloo, Abdalla, and Imjai (2003). As mentioned by Baˇzant (1996), as well as Hu and Wittmann, the consequence of these experimental observations is that: ∞ D 1 ¯ G(a) = P du = Γ(x) dx < GF (A5.1) D − a0 0 a0 ¯ where G(a) = average fracture energy in the ligament (Fig. A.5b), D = specimen size (Fig. A.5a), a0 = notch depth, P = load, u = load-point deﬂection, Γ(x) = local fracture energy ∞ as a function of coordinate x along the ligament (Fig. A.5a left), GF = 0 σ dw = Γ(x)-value at points x remote from the

256

Scaling of Structural Strength

Figure A.5: (a) Variation of local fracture energy Γ(x) across the ligament, decreasing in the boundary layer (reproduced from Baˇzant 1996). (b) Average fracture energy GF . (c) Required modiﬁcation of cohesive (or ﬁctitious) crack model boundary (= area under the complete σ(w)-diagram, Fig. A.5c), σ = cohesive (crack-bridging) stress, and w = crack opening = separation of crack faces. Is this behavior compatible with the cohesive crack model? To check it, consider a decreasing FPZ attached to the boundary at the end of ligament, Fig. A.5a. Extending to this situation Rice’s (1968) approach, we calculate the J-integral along a path touching the crack faces as shown in Fig. A.6a,b:

D ∂ui dv(x) ¯ J= U − ti σ (A5.2) ds (2) = 2 ds − [t2 ∆w]end dx dx xtip ∞ = σ(w)dw − [σ∆w]end = Area below σend (A5.3) 0

= Jend (D) or Jtail (x) or Jmiddle [(x + D)/2]

(A5.4)

in which s = integration contour length; x = x1 , y = x2 are the cartesian coordinates; ui = displacements; ti = tractions acting on the contour from the

Addendum

257

Figure A.6: (a,b) J-integral path. (c,d,e) Ambiguity in J-integral variation. (f,g,h,i) Fracture energies corresponding to J-integral. (j) Test data ﬁtted by modiﬁed cohesive crack model with variable tail

outside; U = strain energy density; v = w/2; x = D is the end point of the ligament; wend is the opening at the end of ligament (Fig. A.6b). From these equations, we see that the instantaneous ﬂux of energy, J, into the shrinking FPZ attached to the end of ligament (Fig. A.5a) represents the area below the line σ = σend in the softening diagram, cross-hatched in Fig. A.6i. It is, however, a matter of choice with which coordinate x in the FPZ this ﬂux J should be associated. If we associate J with the front, the tail, or the middle (Fig. A.6b) of the FPZ, we get widely diﬀerent plots of Γ = Jend , Jtail , Jmiddle , as shown in Fig. A.6(c,d,e), respectively (the ﬁrst one terminating with Dirac delta function). This ambiguity means that the boundary layer eﬀect, experimentally documented by Hu and Wittmann, cannot be represented by the standard cohesive crack model, with a ﬁxed stress-separation diagram. Can the cohesive crack model be adapted for this purpose? It follows from Eq. (A5.4) and Fig. A.6(h,i) (and has been computationally veriﬁed)

258

Scaling of Structural Strength

that Wittmann et al.’s (1990) and Elices et al.’s (1992) data can be matched (Fig. A.6j) if the slope of the tail segment of the bilinear stress-separation diagram for concrete is assumed to decrease (Fig. A.5c) in proportion to diminishing distance r = D − x (Fig. A.6b) from the end of ligament. After such an adaptation, the cohesive (or ﬁctitious) crack model has a general applicability, including the boundary layer. However, the consequence is that the total fracture energy GF (area under the complete stress-separation curve) is not constant. Noting that, the larger the structure, the smaller is the length fraction of the boundary layer, one must conclude that the diminishing tail slope in Fig. A.5c automatically implies a certain size eﬀect on the apparent GF , as given by Eq. (A5.4). It further follows from Fig. A.6(h,i), and has been computationally veriﬁed, that the initial tangent of the stress-separation diagram, the area under which represents the initial fracture energy Gf (Baˇzant 2002f, Baˇzant and BecqGiraudon 2002, Baˇzant, Yu and Zi 2002), can be considered as ﬁxed—in other words, Gf , unlike GF , is a material constant. Aside from the fact that the maximum loads of specimens and structures are generally controlled by Gf , not GF , this suggests that the standard fracture test that should be introduced is that which yields not GF but Gf (the size eﬀect method, as well as the method of Guinea, Planas and Elices, 1994a,b, and the zero brittleness method of Baˇzant, Yu and Zi 2002, serve this purpose, while the work-of-fracture method does not). This conclusion is not surprising in the light of the abundance of experimental data revealing that GF is statistically much more variable than Gf (Baˇzant and Becq-Giraudon 2002, Baˇzant, Yu and Zi 2002). Jir´ asek (2003) showed that Hu and Wittmann’s data can be matched by a nonlocal continuum damage model in which the characteristic softening curve is kept ﬁxed. Consequently the nonlocal model is a more general, and thus more fundamental, characterization of fracture than the cohesive (or ﬁctitious) crack model. This ﬁnding should be taken into account in fracture testing. It appears that GF would better be deﬁned by the area under the softening curve of the nonlocal model, multiplied by the characteristic length of material corresponding to the eﬀective width of FPZ, which equals the minimum possible spacing of parallel cracks (Baˇzant 1985, Baˇzant and Jir´ asek 2002), to be distinguished from Irwin’s characteristic length l0 = EGf /f t2 . A6. Can Fracture Energy Be Measured on One-Size Specimens with Diﬀerent Notch Lengths? The fact that specimens of diﬀerent sizes are needed for the size eﬀect method of measuring Gf is considered by some a disadvantage. For this

Addendum

259

reason, Baˇzant and Kazemi (1990), Baˇzant and Li (1996) and Tang et al. (1996) generalized the size eﬀect method to dissimilar specimens, the dissimilarity being caused by the use of diﬀerent notch lengths a0 in specimens of one size. If the random scatter of test data were small (coeﬃcient of variation CoV < 4%), this approach would work. However, for the typical scatter of maximum loads of concrete specimens (CoV = 8%), the range of brittleness numbers attainable by variation of notch length in a specimen of any geometry (about 1:3, Baˇzant and Li 1996) does not suﬃce to get a sharp trend in the regression of test data, and thus prevents determination of Gf accurately. Recently, this problem was considered independently by Duan and Hu (2003). They proposed the semi-empirical formula: σn = σ0 (1 + a/a∗∞ )−1/2

(A6.1)

where σ0 = ft for small 3PB specimens; a∗∞ is a certain constant; and σn represents the maximum tensile stress in the ligament based on a linear stress distribution over the ligament, σn = σN /A(a0 ). This alternative formula, intended for specimens of the same size when the notch length a0 is varied, in eﬀect attempts to replace the proﬁle of the universal size eﬀect law (Fig. A.2) at constant size D, scaled by the ratio σn /σN = 1/A(a0 ), where A(a0 ) depends on specimen geometry; A(a0 ) = (1 − a0 )2 for notched three-point bend beams. However, the curve of the proposed formula has, for a0 → 0, a size independent limit approached, in log a0 scale, with a horizontal asymptote, while the correct curve, amply justiﬁed by tests of modulus of rupture (or ﬂexural strength) of unnotched beams (Baˇzant and Li 1995, Baˇzant 1998, 2001, 2002f, Baˇzant and Nov´ ak 2000a,b,c), terminates with a steep slope for a0 → 0 and has a size dependent limit, as seen in the aforementioned proﬁles in Fig. A.2a,b, and better in Fig. A.2c. Fig. A.2d,e shows the proﬁles in D and in a, and it is seen that they cannot be matched well by Duan and Hu’s approximation converted from σn to σN . The test data on the dependence of σn on a0 , which Duan and Hu ﬁtted by their formula, should be ﬁtted, more accurately, with the usual size eﬀect law (Baˇzant and Kazemi 1990, Baˇzantand Planas 1998, and Baˇzant 1997, 2002f) σn = σN /A(a0 ) in which σN = E Gf [g (α0 )cf + g(α0 )D]−1/2 where D is constant and α0 = a0 /D is varied (and function g(α0 ) is available from handbooks). However, very short or zero notches (α0 < 0.15D) must be excluded, which means that the value of strength ft cannot be used with Duan and Hu’s approach. To use it, it is necessary to adopt either the approach of Guinea et al. (1994a,b) or the zero-brittleness method (Baˇzant, Yu and Zi 2002).

260

Scaling of Structural Strength

A7. Notched–Unnotched Size Eﬀect Method and Standardization of Fracture Testing Accurate simulations with the cohesive crack model (Guinea et al. 1997, Baˇzant and Yu 2002) revealed that, at maximum load, the cohesive stresses through the entire process zone in concrete fracture specimens (as well as normal-size structures) remain on the initial straight sloping segment of the stress-separation curve (Fig. 9.1, bottom left, Fig. A.7 top left). This means that (for type 2 fracture), the long tail of the stress-separation curve, and thus also the total fracture energy GF representing the area under the entire curve, do not matter. The maximum load depends only on the initial fracture energy Gf , representing the area under the initial tangent of this curve. Furthermore, statistical studies of published test data (Baˇzant and Becq-Giraudon 2002) as well as lattice particle simulations of microstructure (Cusatis et al. 2003a,b) revealed that the scatter of Gf has a much smaller coeﬃcient of variation than the scatter of GF (about one half). For these two reasons, it is preferable that a standard fracture test of concrete would yield directly Gf rather than GF . This means that the size eﬀect method is, in principle, preferable because it provides directly Gf , rather than GF . However, the need to use in this method specimens of very diﬀerent sizes may be seen as inconvenient. When GF is measured directly by the work-offracture method, one can roughly estimate Gf ≈ 0.4GF (Baˇzant 2002f, Baˇzant and Becq-Giraudon 2002). But this relation involves a large error. So, together with greater scatter of GF , this leads to a much greater uncertainty in Gf (and thus maximum load prediction), compared to direct measurement of Gf . Guinea et al. (1997) found that, if an accurate solution with the cohesive crack model is available for the given specimen geometry, then the initial slope of the stress-separation curve (and thus Gf ) can be easily obtained by measuring only the maximum loads of: (1) the maximum load of a small notched specimen (the smallest practical), and (2) an unnotched specimen. No testing method can be simpler and more robust. However, in view of large random scatter in fracture testing of concrete, statistical evaluation is important. In this regard, the simple method of Guinea et al. (1997) can still be improved—by recasting it in the form of zero-brittleness size eﬀect method (Baˇzant and Li 1996b), in a way that permits simultaneous statistical regression of the data for notched and unnotched tests. The key is to realize that the maximum load of unnotched specimens is independent of Gf , and thus depends only on material tensile strength ft . This is the property of the zero-size limit, σN = Bft , of the size eﬀect curve. So it suﬃces to relate B to the zero-size limit B0 ft of the exact size eﬀect curve of the cohesive crack

Addendum

261

model for the given geometry, which can be computed once for all for a chosen standardized specimen geometry (Baˇzant, Yu and Zi 2002). This exact size eﬀect curve is, for normal sizes, very close to the classical size eﬀect law σN = Bft (1 + D/D0 )−1/2 (Eq. 2.8) (and is identical to it for very large sizes). But for extrapolation to zero size, D → 0, a correction is needed. To this end, the size eﬀect curve of cohesive crack model for any ﬁxed specimen geometry may be written in a dimensionless form as (ft /σN )2 = g(α0 )ξ + B −2 − ∆(ξ),

with ξ = D/l1 , l1 = E Gf /ft

(A7.1)

where g(α0 ) = dimensionless energy release rate for the given geometry, and ∆(ξ) = deviation from the classical size eﬀect law in Eq. (2.8), which is calculated accurately from the cohesive crack model (and vanishes for large ξ); ∆(ξ) can be ignored in the usual size eﬀect method (section 2.5) (Baˇzant, Yu and Zi 2002) (l1 must not be confused with l0 = E GF /ft ). The statistical regression of test data may proceed as follows: m 1 1. Calculate the mean tensile strength f¯t = m i=1 ft i . Then, for each of the notched tests (j = 1, 2, . . . , n), calculate ηj = (f¯t /σN j )2 . After that, from the inverse relation of (A7.1) (determined explicitly once for all in advance), calculate ξj = ψ(ηj ) (the vertical line on the right of each plot on the top of Fig. A.7). Then calculate ∆j = ∆(ξj ) (j = 1, 2, . . . , n), and compute the notched specimen data for linear regression (Fig. A.7 right): (j = 1, 2, . . . , n) (A7.2) Yν+j = (ηj + ∆j )/(f¯t )2 (these are the points that would ideally lie on the straight size eﬀect asymptote, if there were no scatter). Set Yi = 1/(Bft i )2 (i = 1, 2, . . . , ν). 2. Consider the standard linear regression relation Y = AX + C of the size eﬀect method (Fig. A.7, top) where X = D, and set Xi = 0 for i = 1, 2, . . . , ν and Xi = D for i = ν + 1, ν + 2, . . . , ν + n. Then run linear regression of all data points (Xi , Yi ), i = 1, 2, . . . , ν + n, using the weights wi = 1/ν for i = 1, . . . , ν and wi = 1/n for i = ν + 1, ν + 2, . . . , N (N = ν + n). The well known regression formulas yield the mean slope A¯ ¯ and also the coeﬃcients of variation of regression and mean intercept C, N slope and intercept, ωA , ωC where ωA = [ i=1 (Yi − Yi )2 /(N − 2)]1/2 /Y¯ , N Y¯ = i=1 (Yi − Yi ) /N and Yi = AXi + C = values on the regression line. Finally, according to the formulas of the size eﬀect method (section 2.5), estimate the mean fracture energy and its coeﬃcient of variation: ¯ f ≈ g(α0 ) / E ¯ A, ¯ ωG ≈ ω 2 + αE ω 2 . G f A E

262

Scaling of Structural Strength

Figure A.7: Left bottom: Regression line based on classical size eﬀect law (Eq. 2.8, dashed line) and deviation ∆(ξ) from this line for small specimen sizes (solid line), computed from the cohesive crack model (the ﬁst vertical dash-dot line indicates the smallest possible specimen for which D ≈ 6 aggregate sizes, and the second one the smallest size for the deviation ∆(ξ) can be ignored). Left top: The smallest cohesive stress in the FPZ, calculated for a standard bilinear softening law with GF = 2.5Gf (‘knee’ = point of slope). Right: Regression of data for notched and unnotched specimens randomly generated according to Weibull distribution with modulus m = 24 (after Baˇzant, Yu and Zi 2002)

A minor weak point of the foregoing procedure is that the initial calculation of ξj is based on the mean of the ft rather than the random ft -data. This may be avoided by a certain kind of iteration (Baˇzant, Yu and Zi 2002).

A8. Designing Reinforced Concrete Beams against Size Eﬀect The time has become ripe for adding size eﬀect in a rational form to all the design speciﬁcations dealing with brittle failures of concrete structures

Addendum

263

Figure A.8: Improved design formula for shear failure of reinforced concrete beams without stirrups (the circle areas represents the weights, which are taken inversely proportional to the histogram of beam depths in the database) (shear and torsion of R.C. beams with or without stirrups, slab punching, column failure, bar embedment length, splices, bearing strength, plain concrete ﬂexure, compression failure of prestressed beams, etc.). In ACI Standard 318, so far, only the recently introduced formula for anchor pullout (which is of the LEFM type) includes size eﬀect. By analysis of the latest ACI 445 database with 398 data (Reineck et al. 2003), representing an update of 1984 and 1986 Northwestern University databases (with 296 data), an improved formula for shear failure of reinforced concrete beams without stirrups, having the simplicity desired by concrete designers, has recently been developed by second-order asymptotic matching (Baˇzant and Yu 2003); see the comparison with database in Fig. A.8, with CoV of the vertical deviations from data points (the solid line is the mean formula, the dashed line is a formula scaled down to achieve additional safety, as practiced in ACI; vc = σN = mean shear stress in the cross section at failure, d = beam depth from top face to the reinforcement centroid, fc = standard compression strength of concrete).

264

Scaling of Structural Strength

In the derivation of these formulas, the following three principles were adhered to: 1. Only theoretically justiﬁed formulas must be used in data ﬁtting because the size eﬀect (which is of main interest for beam depth d ranging from 1 m to 10 m) requires enormous extrapolation of the ACI 445 database (in which 86% of data pertain to d ≤ 0.6 m, 99% to d ≤ 1.1 m and 100% to d ≤ 1.89 m). 2. The validity of the formula must be assessed by comparing it only with (nearly) geometrically scaled beams of broad enough size range (only 11 such test series exist, among 398). 3. The entire database must be used only for the ﬁnal calibration of the chosen formula (but not for choosing the best formula, because data for many diﬀerent concretes and geometries are mixed in the database, and only 2% of the data have a non-negligible size range). A9. Scaling of Probability Density Distribution (pdf ) of Failure Load In practice, structures must typically be designed for failure probabilities pf of the order of 10−7 . Such a low probability cannot be determined experimentally, especially for large structures. It can be assessed only theoretically. One must deduce the size eﬀect on the pdf of σN by a rational argument. This can be done on the basis of the nonlocal Weibull theory expounded in section 3.2. For D → 0, failure is non-propagating and must occur nearly simultaneously along the entire failure surface. So the pdf of σN must be Gaussian (except in far-oﬀ tails), as deduced from Daniels’ (1945) ﬁber bundle model. With increasing D, the asymptotic size eﬀect on the mean strength is nil and the coeﬃcient of variation (CoV) asymptotically decreases as D−1/2 . For D → ∞, the pdf must be Weibull, corresponding to the weakest-link chain model, which implies a size-independent CoV. The gradual transition of pdf from Gaussian to Weibull, exempliﬁed by various load-sharing models (Phoenix and Beyerlein 2000, Mahesh et al. 2002), can be obtained by asymptotic matching (Baˇzant 2004a, 2004b) and calibrated by a chain-of-bundles model (Fig. A.1f middle) (Baˇzant and Pang 2004). A10. Recent Debates on Fractal Theory of Size Eﬀect and Their Impact on Design Codes An engineering ﬁeld such as aeronautical can exist without simple design codes because only a few large aircraft are designed annually. But structural

Addendum

265

engineering, in which many thousands of structures are designed annually, each of them diﬀerent, cannot get by without codes. During the last few years, the need to introduce the size eﬀect into the design code speciﬁcations guarding against brittle failures of concrete structures has ﬁnally been widely recognized on all continents. Members of the code-making committees of course notice that there are currently promulgated two radically diﬀerent theories of size eﬀect in concrete structures—the energetic-statistical theory expounded here and a purely fractal theory. Therefore, unless the conﬂict between the proponents of these two theories is resolved, these committees would opt for a purely empirical approach. Yet, an empirical approach is doomed to yield an incorrect formula because a statistically signiﬁcant set of test results on a suﬃciently large number of identical large structures can hardly ever be acquired, because of prohibitive cost. The largest concrete structures, sea ice bodies or rock formations are way beyond the range of failure testing, and small-size data vastly dominate, because of cost. For instance, 86% of the data for shear failure of beams pertain to beam depths less than 0.6 m, and 99% less than 1.1 m, while the main interest is in beam depths from 1 m to 10 m. Consequently, the design of large structures must rely on extrapolation from the range of testing. A theoretical basis for such an extrapolation is, therefore, imperative. But progress on the design code appears impossible unless the fractal-nonfractal conﬂict is resolved. Motivated by the need to resolve the conﬂict, an extensive critical study has recently been undertaken (Baˇzant and Yavari 2004). It greatly expands the analysis of fractal approach in sections 3.5 and 3.6, and focuses on the recent arguments.

A11. Boundary Layer Size Eﬀect in Thin Metallic Films at Micrometer Scale Recent pure tension tests of free polycrystal thin metallic ﬁlms of Au, Al and Cu, conducted by H. Espinosa at Northwestern University revealed a surprising and very strong size eﬀect. The strength of these ﬁlms increases by a factor of 3 to 5 when the thickness is reduced from 5 µm to 0.5 µm, while for smaller thickness the size eﬀect in pure tension apparently disappears. This size eﬀect can be explained by the existence of a boundary layer of a ﬁxed thickness, located at the face of ﬁlm that was during deposition in contact with the substrate. The boundary layer, having a thickness of the order of the crystal grain size of metal, has a signiﬁcantly higher yield strength than the rest of ﬁlm. The layer forms during ﬁlm deposition on the face of the substrate and is inﬂuenced by the epitaxial eﬀects of crystal growth on the dislocation density and texture.

266

Scaling of Structural Strength

The increase of yield strength of the epitaxial boundary layer is considered to be caused partly by a diﬀerence in the mean density of statistically stored dislocations due to blockage of dislocation movements at grain boundaries and formation of dislocation pile-ups near grain boundaries, compared to the rest of ﬁlm, and partly also by prevalent crystal orientation unfavorable to dislocation glide, which are engendered in the granular epitaxial boundary layer by the substrate during ﬁlm deposition. Assuming a simple error function decay of the yield strength across the ﬁlm thickness from the substrate side leads to a good agreement with pure tension tests, and well as other kinds of experimental observations. The characteristic length l0 governing the boundary layer size eﬀect is the natural grain size of the metal, l0 ≈ 0.5 µm. Therefore the boundary layer size eﬀect is expected to vanish for ﬁlm thickness D < l0 and D > 10l0 , and this is what is observed in tests. The boundary layer size eﬀect does not conﬂict with Hutchinson and Fleck’s strain gradient size eﬀect. That size eﬀect, which has been used to explain micro-indentation tests down to 1 µm, dominates for the range 5–100 µm. In the range from 1 to 5 µm, in which both kinds of size eﬀect overlap, the ﬁt of the micro-indentation and micro-bending test data by the strain gradient theory is not very close. The epitaxial boundary layer model captures the extra plastic hardening due to statistically stored dislocations, whereas the strain gradient theory explained in section 10.1 captures the eﬀect of geometrically necessary dislocations. A combined theory is found to be necessary in order to ﬁt with the same theory the ﬁlm test data on both pure tension and bending. Thin metallic ﬁlms of thickness less than 5 µm are found to fail in a quasibrittle manner, exhibiting gradual postpeak softening, which can also be explained and ﬁtted by the epitaxial boundary layer model if the damage due to void or microcrack growth is taken into account. The classical Hall-Petch relation for the dependence of yield strength on the natural grain size, as well as Nix’s model for the strength of ﬁlms thinner than the grain size, needs to be included in the formulation to obtain a general model with proper asymptotics, the former for very thick ﬁlms (D > 100 µm) and the latter for extremely thin ﬁlms (D < 0.3 µm). Inclusion of the Hall-Petch formula is important when not only the ﬁlm thickness but also the grain size is varied. To this end, the HallPetch formula is enhanced by a smooth approach to a cutoﬀ yield strength for very small grain size. In the case of ﬁlms thinner than than the natural grain size, in which the crystal grains are ﬂattened to ﬁt the ﬁlm thickness, the grain size to be substituted into the Hall-Petch formula is the ﬁlm thickness, which means that the Hall-Petch eﬀect disappears for very thin ﬁlms (being replaced by Nix’s eﬀect).

Addendum

267

A12. Size Eﬀect on Triggering of Dry Snow Slab Avalanches A size eﬀect model analogous to that expounded in this book has recently been formulated for dry snow slab avalanches in a study by Baˇzant, Zi and McClung (2003). The ratio of the thickness of snow layer to the length is, in that study, assumed to be small enough for one-dimensional analysis to be applicable. Equivalent LEFM is used to obtain the law of the decrease of the nominal shear strength of the snow layer with an increasing thickness of snow. This law is shown to closely agree with two-dimensional numerical solutions according to the cohesive crack model for mode II fracture with ﬁnite residual shear stress. By ﬁtting these solutions for various snow thicknesses D with the structural size eﬀect law, an approximate one-to-one relationship between the material parameters in the size eﬀect law and the cohesive crack model is established. The failure mode and size eﬀect are found to depend on the pre-existing (initial) shear stress τi in a fracture-triggering weak layer that normally exists at the base of snow slab. There exists a critical stress τi = τcr and a critical snow depth Dcr such that, for D > Dcr or τi < τcr , there is no structural size eﬀect, no peak load, and no postpeak softening. The value of τcr is approximately 85% of the residual shear stress at the base of a sliding layer. Because the fracture process zone can be many meters long, it is not easy to perform laboratory experiments simulating avalanches. Direct measurement of the size eﬀect per se is next to impossible because the eﬀects of snow weight and snow aging prevent ﬁnding diﬀerent-sized samples with similar mechanical properties. The size eﬀect law needs to take into account the dependence of snow properties in the weak layer at base on the snow slab thickness. This is achieved by replacing the constant fracture toughness and the limiting zero-size strength with quantities that increase with snow slab thickness. Fitting of the data from over a hundred ﬁeld observations of avalanches suggests that this increase is very strong, with the toughness increasing roughly as (snow thickness)1.8 .

Bibliography

305

Relevant Author’s Works after the First Printing (up to 2004) Baˇzant, ZP (2001a), “Probabilistic modeling of quasibrittle fracture and size eﬀect” (principal plenary lecture), (Proc., 8th Int. Conf. on Structural Safety and Reliability (ICOSSAR), held at Newport Beach, Cal., 2001), RB Corotis, GI Schueller and M Shinozuka, eds., Swets & Zeitinger (Balkema), 1–23. Baˇzant, ZP (2001b), “Scaling of failure of beams, frames and plates with softening hinges.” Meccanica (Kluwer Acad. Publ.) 36, 67–77, 2001 (special issue honoring G Maier). Baˇzant, ZP (2001c), “Size eﬀects in quasibrittle fracture: Apercu of recent results.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-4 Int. Conf., Paris), R de Borst, J Mazars, G Pijaudier-Cabot and JGM van Mier, eds., Swets & Zeitlinger (A.A. Balkema Publishers), Lisse, 651–658. Baˇzant, ZP (2001d), “Scaling laws for sea ice fracture.” Proc., IUTAM Symp. on Scaling Laws in Ice Mechanics and Ice Dynamics (held in Fairbanks, June 2000), ed. by JP Dempsey and HH Shen, Kluwer Academic Publ., Dordrecht, 195–206. ˇ Baˇzant, ZP, Caner, FC, and Cervenka, J (2001), “Vertex eﬀect and conﬁnement of fracturing concrete via microplane model M4.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-4 Int. Conf., Paris), R de Borst, J Mazars, G Pijaudier-Cabot and JGM van Mier, eds., Swets & Zeitlinger (A.A. Balkema Publishers), Lisse, 497–504. ˇ Baˇzant, ZP, Cervenka, J, and Wierer, M (2001), “Equivalent localization element for crack band model and as alternative to elements with embedded discontinuities.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-4 Int. Conf., Paris), R de Borst, J Mazars, G Pijaudier-Cabot and JGM van Mier, eds., Swets & Zeitlinger (A.A. Balkema Publishers), Lisse, 765–772. Baˇzant, ZP and Nov´ ak, D (2001a), “Proposal for standard test of modulus of rupture of concrete with its size dependence.” ACI Materials Journal 98 (1), 79–87. Baˇzant, ZP and Nov´ ak, D (2001b), “Nonlocal Weibull theory and size eﬀect in failures at fracture initiation.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-4 Int. Conf., Paris), R de Borst, J Mazars, G PijaudierCabot and JGM van Mier, eds., Swets & Zeitlinger (A.A. Balkema Publishers), Lisse, 659–664.

306

Scaling of Structural Strength

Baˇzant, ZP and Nov´ ak, D (2001c), “Nonlocal model for size eﬀect in quasibrittle failure based on extreme value statistics.” (Proc., 8th Int. Conf. on Structural Safety and Reliability (ICOSSAR), Newport Beach, Cal., 2001), RB Corotis, ed., Swets & Zeitinger (Balkema), 1–8. Brocca, M and Baˇzant, ZP (2001), “Size eﬀect in concrete columns: Finite element analysis with microplane model.” J. of Structural Engineering ASCE 127 (12), 1382–1390. Carol, I, Jir´ asek, M, and Baˇzant, ZP (2001), “A thermodynamically consistent approach to microplane theory. Part I: Free energy and consistent microplane stresses.” Int. J. of Solids and Structures 38 (17), 2921–2931. Planas, J, Baˇzant, ZP, and Jir´ asek, M (2001), “Reinterpretation of Karihaloo’s size eﬀect analysis for notched quasibrittle structures.” Intern. J. of Fracture 111, 17–28. Baˇzant, ZP, Zhou, Y, Nov´ ak, D, and Daniel, IM (2001), “Size eﬀect in fracture of sandwich structure components: foam and laminate.” Proc., ASME Intern. Mechanical Engrg. Congress (held in New York), Vol. AMD-TOC (paper 25413), Am. Soc. of Mech. Engrs., New York, pp. 1–12. Baˇzant, ZP (2002a), “Reminiscences on four decades of struggle and progress in softening damage and size eﬀect”. Concrete Journal (Tokyo) 40 (2), 16–28 (JCI Anniversary); Expanded version republished in Mechanics (Am. Academy of Mech.) 32 (5–6), 2003, 1–10. Baˇzant, ZP (2002b), “Size eﬀect theory and its application to fracture of ﬁber composites and sandwich plates.” Continuum Damage Mechanics of Materials and Structures, O Allix and F Hild, eds., Elsevier, Amsterdam, pp. 353–381. Baˇzant, ZP (2002c), “Size eﬀect theory and its application to fracture of ﬁber composites and sandwich plates.” Continuum Damage Mechanics of Materials and Structures, O Allix and F Hild, eds., Elsevier, Amsterdam, pp. 353–381. Baˇzant, ZP (2002d), “Scaling of sea ice fracture—Part I: Vertical penetration.” J. of Applied Mechanics ASME 69 (Jan.), 11–18. Baˇzant, ZP (2002e), “Scaling of sea ice fracture—Part II: Horizontal load from moving ice.” J. of Applied Mechanics ASME 69 (Jan.), 19–24. Baˇzant, ZP (2002f), “Concrete fracture models: testing and practice.” Engineering Fracture Mechanics 69 (2), 165–206 (special issue on Fracture of Concrete and Rock, M Elices, ed.).

Bibliography

307

Baˇzant, ZP (2002g), “Scaling of dislocation-based strain-gradient plasticity.” J. of the Mechanics and Physics of Solids 50 (3), 435–443 (based on Theor. & Appl. Mech. Report No. 2000-12/C699s, Northwestern University 2000; see also Errata, Vol. 52, 2004, p. 975). Baˇzant, ZP and Becq-Giraudon, E (2002), “Statistical prediction of fracture parameters of concrete and implications for choice of testing standard.” Cement and Concrete Research 32 (4), 529–556. Baˇzant, ZP and Frangopol, DM (2002), “Size eﬀect hidden in excessive dead load factor.” J. of Structural Engrg. ASCE 128 (1), 80–86. Baˇzant, ZP and Guo, Z (2002a), “Size eﬀect and asymptotic matching approximations in strain-gradient theories of micro-scale plasticity.” Int. J. of Solids and Structures 39, 5633–5657; see also Errata, Vol. 40 (2003), p. 6215). Baˇzant, ZP and Guo, Z (2002b), “Size eﬀect on strength of ﬂoating sea ice under vertical line load.” J. of Engrg. Mechanics 128 (3), 254–263. Baˇzant, ZP and Jir´ asek, M (2002), “Nonlocal integral formulations of plasticity and damage: Survey of progress.” ASCE J. of Engrg. Mechanics 128 (11), 1119–1149 (ASCE 150th anniversary article). Baˇzant, ZP, Yu, Q, and Zi, G (2002), “Choice of standard fracture test for concrete and its statistical evaluation.” Int. J. of Fracture 118 (4), Dec., 303–337. Caner, FC and Baˇzant, ZP (2002), “Lateral conﬁnement needed to suppress softening of concrete in compression.” J. of Engrg. Mechanics ASCE 128 (12), 1304–1313. Jir´ asek, M and Baˇzant, ZP (2002), Inelastic Analysis of Structures. J. Wiley & Sons, London and New York (735 + xviii pp.). Lin, F-B, Yan, GY, Baˇzant, ZP, and Ding, F (2002), “Nonlocal strain-softening model of quasibrittle materials using boundary element method.” Engrg. Analysis with Boundary Elements 26, 417–424. Baˇzant, ZP (2003a), “Asymptotic matching analysis of scaling of structural failure due to softening hinges. I. Theory.” J. of Engrg. Mech. ASCE 129 (6), 641–650. Baˇzant, ZP (2003b), “Asymptotic matching analysis of scaling of structural failure due to softening hinges. II. Implications.” J. of Engrg. Mech. ASCE 129 (6), 651–654. Baˇzant, ZP and Nov´ ak, D (2003), “Stochastic models for deformation and failure of quasibrittle structures: recent advances and new directions.”

308

Scaling of Structural Strength

Computational Modelling of Concrete Structures (Proc., EURO-C Conf., St. Johann im Pongau, Austria), N Bi´cani´c, R de Borst, H Mang and G Meschke, eds., A.A. Balkema Publ., Lisse, Netherlands, 583–598. Baˇzant, ZP, Zhou, Y, Zi, G, and Daniel, IM (2003), “Size eﬀect and asymptotic matching analysis of fracture of closed-cell polymeric foam.” Int. J. of Solids and Structures 40, 7197–7217. Baˇzant, ZP and Zi, G (2003), “Asymptotic stress intensity factor proﬁles for smeared-tip method for cohesive fracture.” Int. J. of Fracture 119 (2), 145–159. Baˇzant, ZP, Zi, G and McClung, D (2003), “Size eﬀect law and fracture mechanics of the triggering of dry snow slab avalanches.” J. of Geophysical Research 108 (B2), 2119–2129. Cusatis, G, Baˇzant, ZP, and Cedolin, L (2003a), “Conﬁnement-shear lattice model for concrete damage in tension and compression: I. Theory.” J. of Engrg. Mechanics ASCE 129 (12), 1439–1448. Cusatis, G, Baˇzant, ZP, and Cedolin, L (2003b), “Conﬁnement-shear lattice model for concrete damage in tension and compression: I. Computation and validation.” J. of Engrg. Mechanics ASCE 129 (12), 1449–1458. Nov´ ak, D, Baˇzant, ZP, Voˇrechovsk´ y, M (2003), “Computational modeling of statistical size eﬀect in quasibrittle structures.” Applications of Statistics and Probabiltity in Civil Engineering (Proc., 9th Int. Conf., ICASP-9, held in San Francisco), A Der Kiureghian, S Madanat and JM Pestana, eds., Millpress, Rotterdam, 621–628. Sl´ adek, J, Sl´ adek, V, and Baˇzant, ZP (2003), “Non-local boundary integral formulation for softening damage.” Int. J. for Numerical Methods in Engrg. 57, 103–116. Zi, G and Baˇzant, ZP (2003), “Eigenvalue method for computing size eﬀect of cohesive cracks with residual stress, with application to kink bands in composites.” Int. J. of Engrg. Science 41 (13–14), 1519–1534 (special issue honoring K Willam, ed. by ZP Baˇzant, I Carol and P Steinmann). Baˇzant, ZP, Caner, FC, Cedolin, L, Cusatis, G, and Di Luzio, G (2004), “Fracturing material models based on micromechanical concepts: Recent advances.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-5, 5th Int. Conf. on Fracture Mech. of Concrete and Concr. Structures, Vail, Colo.), Vol. 1, VC Li, KY Leung, Willam, KJ, and Billington, SL, eds., IA-FraMCoS, 83–90. Baˇzant, ZP, Pang, SD, Voˇrechovsk´ y, M, Nov´ ak, D and Pukl, R (2004), “Statistical size eﬀect in quasibrittle materials: Computation and extreme value

Bibliography

309

theory.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-5, 5th Int. Conf. on Fracture Mech. of Concrete and Concr. Structures, Vail, Colo.), Vol. 1, VC Li, KY Leung, Willam, KJ, and Billington, SL, eds., IA-FraMCoS, 189–196. Baˇzant, ZP and Yu, Q (2004), “Size eﬀect in concrete specimens and structures: New problems and progress.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-5, 5th Int. Conf. on Fracture Mech. of Concrete and Concr. Structures, Vail, Colo.), Vol. 1, VC Li, KY Leung, Willam, KJ, and Billington, SL, eds., IA-FraMCoS, 153–162. Baˇzant, ZP, Zhou, Y, Nov´ ak, D, and Daniel, IM (2004), “Size eﬀect on ﬂexural strength of ﬁber-composite laminate.” J. of Engrg. Materials and Technology ASME 126 (Jan.), 29–37. Baˇzant, ZP (2004a), “Scaling theory for quasibrittle structural failure.” Proc., National Academy of Sciences 101, in press. Baˇzant, ZP (2004b), “Probability distribution of energetic-statistical size eﬀect in quasibrittle fracture.” Probabilistic Engineering Mechanics, in press. Baˇzant, ZP and Caner, FC (2004), “Microplane model M5 with kinematic and static constraints for concrete fracture and anelasticity.” J. of Engrg. Mech. ASCE, in press. Baˇzant, ZP, Guo, Z, Espinosa, H, Zhu, Y and Peng, B (2004), “Epitaxially Inﬂuenced Boundary Layer Model for Size Eﬀect in Thin Metallic Films.” Theor. & Appl. Mech. Report, Northwestern University; J. of Appl. Physics, submitted to. Baˇzant, ZP and Yu, Q (2004), “Designing against size eﬀect on shear strength of reinforced concrete beams without stirrups.” J. of Structural Engineering ASME, in press. Baˇzant, ZP and Yavari, A (2004), “Is the cause of size eﬀect on structural strength fractal or energetic-statistical?” Engrg. Fracture Mechanics 43, in press.

Additional References for Addendum (up to 2004) Acharya, A and Bassani, JL (2000), “Lattice incompatibility and a gradient of crystal plasticity.” J. of the Mechanics and Physics of Solids 48, 1565–1595. Carpinteri, A (1987), “Stress-singularity and generalized fracture toughness at the vertex of re-entrant corners.” Engineering Fracture Mechanics 26, 143–155.

310

Scaling of Structural Strength

Daniels, HE (1945), “The statistical theory of the strength of bundles & threads.” Proc. Royal Soc. A183, London, 405–435. Duan, K and Hu, XZ (2003), “Scaling of quasi-brittle fracture: Boundary eﬀect.”, submitted to Engineering Fracture Mechanics. Duan, K, Hu, XZ, and Wittmann, FH (2002), “Explanation of size eﬀect in concrete fracture using non-uniform energy distribution.” Materials and Structures 35, 326–331. Duan, K, Hu, XZ, and Wittmann, FH (2003), “Boundary eﬀect on concrete fracture and non-constant fracture energy distribution.” Engrg. Fracture Mechanics 70, 2257–2268. Dunn, ML, Suwito, W, and Cunningham, SJ (1997), “Stress Intensities at notch singularities.” Engineering Fracture Mechanics 57(4), 417–430. Dunn, ML, Suwito, W, and Cunningham, SJ (1997), “Fracture initiation at sharp notches: correlation using critical stress intensities.” Int. J. Solids Structures 34(29), 3873–3883. Elices, M, Guinea, GV, and Planas, J (1992), “Measurement of the fracture energy using three-point bend tests: Part 3-inﬂuence of cutting the P-d tail.” Materials and Structures 25, 327–334. Fleck, NA and Hutchinson, JW (1993), “A phenomenological theory for strain gradient eﬀects in plasticity.” J. of the Mechanics and Physics of Solids 41, 1825–1857. Fleck, NA and Hutchinson, JW (1997), “Strain gradient plasticity.” Advances in Applied Mechanics, vol. 33, JW Hutchinson and TY Wu, eds., Academic Press, New York, 295–361. Fleck, NA, Olurin, OB, Chen, C, and Ashby, MF (2001), The Eﬀect of Hole Size upon the Strength of Metallic and Polymeric Foams. Journal of the Mechanics and Physics of Solids 49, 2015–2030. Gibson, LJ and Ashby, MF (1997), Cellular Solids: Structure and Properties, 2nd ed. Cambridge University Press, Cambridge, UK. Guinea, GV, Planas, J, and Elices, M (1994a), “Correlation between the softening and the size eﬀect curves.” Size Eﬀect in Concrete (edited by Mihashi, H, Okamura, H, and Baˇzant, ZP), E&FN Spon, London, 233–244. Guinea, GV, Planas, J, and Elices, M (1994b), “A general bilinear ﬁtting for the softening curve of concrete.” Materials and Structures 27, 99–105. Guinea, GV, Elices, M, and Planas, J (1997), “On the initial shape of the softening function of cohesive materials.” Int. J. of Fracture 87, 139–149.

Bibliography

311

Hu, XZ (1997), “Toughness measurements from crack close to free edge. “International Journal of Fracture 86(4), L63–L68. Hu, XZ (1998), “Size eﬀects in toughness induced by crack close to free edge.” Fracture Mechanics of Concrete Structures (ed. by Mihashi, H, and Rohugo, K), Proc. FraMCoS-3, Japan, 2011–2020. Hu, XZ and Wittmann, FH (1991), “An analytical method to determine the bridging stress transferred within the fracture process zone: I. General theory.” Cement and Concrete Research 21, 1118–1128. Hu, XZ and Wittmann, FH (1992a), “An analytical method to determine the bridging stress transferred within the fracture process zone: II. Application to mortar.” Cement and Concrete Research 22, 559–570. Hu, XZ and Wittmann, FH (1992b), “Fracture energy and fracture process zone.” Materials and Structures 25, 319–326. Hu, XZ and Wittmann FH (2000), “Size eﬀect on toughness induced by crack close to free surface.” Engineering Fracture Mechanics 65, 209–221. Jackson, KE (1992), “Scaling Eﬀects in the Flexural Response and Failure of Composite Beams,” AIAA Journal, Vol. 30(8), pp, 2099–2105. Johnson, DP, Morton, J, Kellas, S, and Jackson, KE (2000), “Size Eﬀect in Scaled Fiber Composites Under Four-Point Flexural Loading,” AIAA Journal, Vol. 38(6), 1047–1054. Jir´ asek, M (2003), Keynote lecture presented at EURO-C, St. Johann in Pongau, Austria. Karihaloo, BL (1999), “Size eﬀect in shallow and deep notched quasi-brittle structures.” International Journal of Fracture 95, 379–390. Karihaloo, BL, Abdalla, HM, and Imjai, T (2003), “A simple method for determining the true speciﬁc fracture energy of concrete.” Magazine of Concrete Research 55(5), 471–481. Karihaloo, BL, Abdalla, HM, and Xiao, QZ (2003), “Size eﬀect in concrete beams.” Engineering Fracture Mechanics 70, 979–993. Lavoie, JA, Soutis C, and Morton, J (2000), “Apparent Strength Scaling in Continuous Fiber Composite Laminates.” Composite Science and Technology, Vol. 60, pp. 283–299. Mahesh, S, Phoenix, SL and Beyerlein, IJ (2002), “Strength distributions and size eﬀects for 2D and 3D composites with Weibull ﬁbers in an elastic matrix.” Int. J. of Fracture 115, 41–85.

312

Scaling of Structural Strength

Mindlin, RD (1965), “Second gradient of strain and surface tension in linear elasticity.” Int. J. Solids Struct. 1, 417–438. Phoenix, SL and Beyerlein, IJ (2000), “Distribution & size scalings for strength in a one-dimensional random lattice with load redistribution to nearest & next nearest neighbors.” Phys. Review E 62, 1622–1645. Reineck, K, Kuchma, DA, Kim, KS, and Marx, S (2003), “Shear database for reinforced concrete members without shear reinforcement.” ACI Structural Journal 100, No. 2, 240-249; with discussions by Baˇzant and Yu, Vol. 101, No. 1 (Jan.-Feb. 2004). Rice, RJ (1968), “Mathematical analysis in the mechanics of fracture.” Fracture-An Advanced Treatise, Vol. 2 (ed. by Liebowitz, H), Academic Press, New York, 191–308. RILEM Committee QFS (ZP Baˇzant, chairman) (2004), “Quasibrittle fracture scaling and size eﬀect.” Materials and Structures (Paris) 37, in press. Tang, T, Baˇzant, ZP, Yang, S, and Zollinger, D (1996), “Variable-notch one-size test method for fracture energy and process zone length.” Engrg. Fracture Mechanics 55(3), 383–404. Toupin, RA (1962), “Elastic materials with couple stresses.” Arch. Ration. Mech. Anal. 11, 385-414. Williams, ML (1952), “Stress singularities resulting from various boundary conditions in angular corners of plates in extension.” Journal of Applied Mechanics 74, 526–528. Wisnom, MR (1991), “The Eﬀect of Specimen Size on the Bending Strength of Unidirectional Carbon Fiber-Epoxy,” Composite Structures, Vol. 18, pp. 47–63. Wisnom, MR and Atkinson, JA (1997), “Reduction in Tensile and Flexural Strength of Unidirectional Glass Fiber-Epoxy with Increasing Specimen Size,” Composite Structures, Vol. 38, pp. 405–412. Wittmann, FH, Mihashi, H, and Nomura, N (1990), “Size eﬀect on fracture energy of concrete.” Engrg. Fracture Mech. 35, 107–115 Zenkert, D and B¨ acklund J (1989), PVC Sandwich Core Materials: Mode I Fracture Toughness. Composite Science and Technology 34, 225–242. Zenkert, D (1989), PVC Sandwich Core Materials: Fracture Behaviour under Mode II and Mixed Mode Loading. Materials Science and Engineering 108, 233–240.

Subject Index activation energy, 151, 152 asymptotic analysis, 21–49 power scaling law large sizes, 14 small sizes, 14 small sizes, 16 smeared-tip method, 177–217 transitional size, 17 boundary layer concrete, cohesive softening law tail, 255 eﬀect, 10 of cracking, 42, 43, 45 Prandtl’s theory, 1, 25, 193 stress redistribution, 38, 43, 44 boundary value problem, xi, 18, 78, 181 bridging stress and crack opening, 165, 180 and stress intensity factor, 205 deformations in the FPZ, 181 distribution, 166, 180 in kink band, 137, 145 residual, 133 brittleness concept, 26 inﬂuence of loading rate, 153, 154 of ﬂoating sea ice, 35 brittleness number analysis of size eﬀect tests, 29, 30, 47 Baˇzant’s, 25, 26, 47

characteristic length absence, 11, 18 characteristic material length absence, 7, 11–13, 17, 20, 56 and fracture process zone, 21, 22, 156 discrete elements, 174 eﬀect of viscosity, 156 ﬁnite elements, 172 ﬂoating sea ice, 78, 84 in nominal strength, 23 in stress distribution, 28 inelastic hinges, 90 Irwin’s, 93, 188 localization limiter, 174 microplane model, 167, 172 small structure sizes, 14 characteristic structure size, 11, 56, 89, 94, 99, 111, 135, 137, 182 characteristic time, 156 closed cell polymeric foam fracture, 254 CMOD, see crack mouth opening displacement cohesive crack model, 167, 177, 178 and Rice’s J-integral, 187 asymptotic analysis, 24, 26 basic hypothesis, 177 broad size range, 210 conversion to an eigenvalue problem, 165 crack opening, 165 energetic aspect, 178

314

Scaling of Structural Strength

ﬁtting formula, 193 for ﬁber composites, 148 fracture energy, 32, 180, 210, 211 in historical context, 7 kink band failure, 147 limitations, 179, 181, 193 nonstandard, 185, 187, 215, 216 plastic analysis, 202 small size asymptotics, 204 softening curve, 145 standard, 181, 182, 198, 199, 203, 204, 215 standard and nonstandard equivalence, 185 stress proﬁle resolution, 165 stress-displacement curve, 185 stress-displacement law, 179, 180 time dependent formulation, 152, 153 compliance calculation from KI expressions, 88 Green’s functions, 179, 204 method, for equivalent crack length, 21, 40 compression failure basic mechanisms, 121 buckling phenomena, 122 by splitting crack band, 91, 122, 124, 133 crushing phenomena, 92, 101, 116, 130, 131 hinge softening, 90 internal buckling phenomena, 122 of concrete beams, 90, 130, 131 of ice plate, 87 size eﬀect on nominal strength, 124

concrete structures design codes, 110–117 no-tension design, 117–119 plain, see unreinforced concrete reinforced, see reinforced concrete crack band model basic idea, 170, 178 comparison with cohesive crack model, 177, 178 comparison with test data, 45 in historical context, 7–9 mesh dependence, 125, 172 crack growth fatigue, see fatigue crack growth stable, 38, 47, 53, 55, 57, 59, 70, 71, 111 crack inﬂuence function, 171 crack initiation failures, 245 crack mouth opening displacement, 153 crack opening proﬁle and stress intensity factor, 184 calculation form KI expressions, 87 calculation from KI expressions, 182, 183 creep, 10, 153 viscoelasticity, 153, 156, 209 critical crack tip opening displacement, 32, 199 critical stress intensity factor, see fracture toughness CS theory, 237 cycling loading, see fatigue crack growth design codes, fractal theory, 264 dimensionless variables, 230 discrete element method, 37, 170, 174–176 dry snow slab avalanches, triggering, 267

Subject Index

eigenvalue analysis, 165, 166 energy balance, 16, 122, 124 energy release analysis of steel-concrete composite beams, 102, 104, 106, 107 complementary potential energy, 106 complementary shear strain energy, 106 slip of studs, 107, 109 and deterministic size eﬀect, 2, 15, 55 asymptotic analysis, 21, 29, 58 axial splitting cracks, 122–124, 131 complementary energy analysis, 22, 23 crack band, 124 for large structure sizes, 15 for small structure sizes, 16 in approximate analysis, 7 in breakout of boreholes in rock, 132 in continuum damage model, 170, 172, 173 in kink bands, 138, 140 142 inelastic hinge, 90–92, 95 potential energy analysis, 22 strain energy density, 29 stress redistributions, 55, 57 energy release function, 27, 40, 135, 179, 182, 196, 198, 206 energy release rate, 17, 22, 23 and material orthotropy, 135 at zero crack length, 40 critical, 19 dimensionless expression, 23, 24 for a system of loads, 48 for ﬂoating ice plates vertical penetration, 82, 84 in nonlocal LEFM, 206

315

equivalent LEFM analysis, 21, 27, 29, 40, 69, 86, 107, 133, 145, 148, 199, 203, 206, 216 Espinosa, H, 265 failure load (pdf), 264 fatigue crack growth, 7, 38, 154, 189 ﬁbre-composite laminates, ﬂexural strength, 252 ﬁnite angle notches, size eﬀect, 249 Fleck and Hutchinson’s formulation, 228 ﬂoating sea ice force applied to ﬁxed structures, 87–89 line load, 99–101 thermal bending fracture, 77–78 vertical penetration, 78–86 FPZ, see fracture process zone fractal curve, 69, 70, 72 dimension, 71–74 fracture energy, 71 lacunar, 72–76 fractal and multifractal scaling law, 42, 49, 73, 75, 111, 134 fracture energy, 29, 32, 76, 84, 138, 211 according to fractal theories, 70–72 and broad-range size eﬀect law, 210, 217 and characteristic material length, 22 deﬁnition, 15 for a splitting crack band, 91, 124, 131 for concrete, 32, 211 from the load-deﬂection curve of a notched beam, 211 from the load-deﬂection curve of a notched beam, 32, 211

316

Scaling of Structural Strength

in slip of studs, 107 in the cohesive crack model, 32, 180, 187, 206, 210 in the crack band model, 170 of a kink band, 141, 143, 145 relation to the J-integral, 68 fracture mechanics in historical context, 5, 7 linear elastic, see linear elastic fracture mechanics of fractal cracks, 71 fracture process zone and characteristic material length, see characteristic material length, fracture process zone and fractal theories, 72 and inhomogeneity size, 15, 38, 86 and stress proﬁle, 165, 167, 180, 181 and transition of behavior, 27 and Weibull theory, 60, 66 eﬀective length of the R-curve, 21 equivalent crack length, 21, 40 ﬂux of energy, 28 in a composite beam, 103 in fractal theories, 72 in historical context, 6 J-integral path, 67, 139, 187 Poisson eﬀect, 10 size, 60, 66, 77, 86, 92, 107, 153, 156, 167, 177, 183, 188 fracture testing, 260 fracture toughness, 17, 88, 118, 156, 183 G, see energy release rate Gb , see fracture energy GF , see fracture energy Gf , see fracture energy

geometry dependence, see shape dependence Hall-Petch formula, 266 incremental plasticity, scaling strain-gradient, 236 J-Integral, 27 and the cohesive crack model, 178, 180, 187 and Weibull size eﬀect, 67 application to kink bands, 137–140, 142, 143 calculation of a ﬂux of energy, 28 critical value, 138, 143 dimensionless expression, 29 expression, 142, 143 path, 28, 140 independence, 67 KI , see stress intensity factor Kc , see fracture toughness large notch or crack, 241 LEFM, see linear elastic fracture mechanics linear elastic fracture mechanics equivalent analysis, see equivalent LEFM analysis generalization to orthotropy, 135 nonlocal, 206, 217 power law exponent −1/2, 7, 12, 13, 24, 59, 60, 78, 109, 112 stress intensity factor, 17 localization, see strain softening localization limiter, see strain softening, localization limiter material characteristic length, 229 mesh bond slip, 125 dependence, 170, 172, 173, 175 discrete elements, 175 inclined crack band, 125, 172

Subject Index

reinforced concrete columns, 125, 127 remeshing, 170, 172 MFSL, see fractal and multifractal scaling law MSG theory, 237 micromechanical model, 72, 76, 121, 170, 172, 230 microplane model, 125, 167–169, 172 multifractal scaling law, see fractal and multifractal scaling law nominal strength, 23, 109 and elastic buckling, 19 asymptotic, 16, 21, 23, 26, 40, 66, 124, 198, 202 data, 31, 34–38, 95, 125, 126, 153 dimensionless, 89 expression, 40, 41, 43, 68, 91, 99, 124, 186 for transitional size range, 13, 14 in compression failure, 124 in historical context, 4, 5, 7 of a composite beam, 103 of sea ice, 20, 81 of stud, 109 pullout, 109 residual, 26 shear loading, 131 time dependence, 153 Weibull-type scaling law, 13, 68 nonlocal damage mechanics, see nonlocal model nonlocal model averging rule, 171 and ﬁnite element size, 172 characteristic length, 172 cohesive law, 181 ﬁnite element analysis, 15, 172, 176, 177

317

of cohesive crack, 26 for damage, 57, 171, 172, 174, 176, 177, 193, 205, 217 in historical context, 5, 9 generalization for Weibull statistical size eﬀect, see Weibull, statistical size eﬀect, nonlocal generalization in historical context, 172 nonlocal LEFM, see linear elastic fracture mechanics, nonlocal physical justiﬁcation, 171 theories for strain localization, 58, 62 with crack interactions, 37 notch length, fracture energy, 258 R-curve, 21–24, 48, 169, 170, 199, 203, 206 random particle model, see discrete element method rate dependence, see time dependence reinforced concrete beams compression failure, 90, 91 diagonal shear failure, 35, 37, 55, 57, 111, 113, 130, 131 torsional failure, 113 columns, 112, 113, 124–126, 128 cylinders double-punch loading, 36 ﬁber-reinforced concrete, 133 size eﬀect laws for, 110, 112 slabs punching shear failure, 113 relaxation, 153, 209, 212 scaling and size eﬀect, 232 shape dependence, 14, 24, 27, 40, 56, 62, 67, 69, 91, 110, 133, 148, 183–186, 188,

318

Scaling of Structural Strength

198, 199, 204, 207, 215–217 shrinkage, 10 SIF, see stress intensity factor small size asymptotic load-deﬂection response, 235 snapback, 16, 17, 96, 98, 157, 158, 161, 162, 167 splitting crack band, see compression failure, by splitting crack band steel-concrete composite beams, 101–110 strain-gradient plasticity, scaling of, 228 Fleck and Hutchinson formulation, 228 strain softening and distributed cracking, 43 and energy dissipation, 91, 173 and loading rate, 10, 156, 157, 173 and wave speed propagation, 173 eﬀective numerical methods, 172 eﬃcient numerical methods, 169 elasto-plastic stability, 89, 90 in cohesive crack model, 181, 217 in elasto-plastic stability, 20 in historical context, 7 in microplane model, 168 loading rate, 173 localization limiter, 170, 173, 174 nonlocal theories, 58, 60 stress intensity factor, 87, 194, 204, 207, 208, 215 at fracture initiation, 196 case of many loads, 133

critical, see fracture toughness density proﬁles, 179, 183, 184, 187, 207 dimensionless, 182 ductility analysis, 162 eccentric loading, 118 fatigue loading, 154 function, 179, 189, 198 of cohesive crack, 166, 178, 183, 184, 204, 207 sea-ice radial bending crack, 81 shape dependence, 198 sharp craft without FPZ, 135 stress relief zone, 15 stud, see steel-concrete composite beams surface energy, 72, 151 thermal bending fracture, 77, 78 thin metallic ﬁlms, boundary layer eﬀect, 265 three-point bend notched beams experimental results, 8, 21, 26, 30, 61, 162 time dependence, 151 creep, 10, 153 due bond ruptures, 154 due to bond ruptures, 151, 152 due to diﬀusion phenomena, 10 due to viscosity, 10, 151, 154, 156, 157 dur to bond ruptures, 154 fatigue, see fatigue crack growth of cohesive crack, 152, 153 of fracture growth, 151 of length scale, 10, 156 TNT theory, 237 toughness, see fracture toughness universal size eﬀect law, 248 unreinforced concrete beams, 113 torsional failure, 113 beams or plates, 90

Subject Index

dams, 57, 113, 117 retaining walls, 113, 117 viscoelasticity, 151, 152, 156, 209, 211, 212 Weibull distribution, 53, 55, 56, 60, 73 energetic-statistical approach, 66–68 nominal strength, 68 size eﬀect law parameters, 57, 59, 62, 66, 74 statistical size eﬀect, 4, 6, 7, 13 and fractality, 72–74, 76 asymptotic analysis, 66 basic hypothesis, 53 for concrete, 35, 57, 111 for quasibrittle structures, 53, 56 limitations, 13, 38, 56, 59, 62 nonlocal generalization, 58–60, 62 stress, 54, 67 weakest link model, 6, 55, 67, 198 Weibull modulus, 53, 57, 66, 67, 74 Weibull theory, 247 weight function, 169, 171, 181, 206 yield plateau, 138

319

Reference Citation Index Acharya and Bassini (2000), 236, 237 ACI 318 (1989), 112 Argon (1972), 134 Ashby and Hallam (1986), 121 Assur (1963), 78 Bao, Ho, Suo and Fan (1992), 135 Barenblatt (1959), 7, 177 Barenblatt (1962), 7, 177 Barenblatt (1979), 12, 17, 25, 193 Barenblatt (1987), 17, 20, 193 Barenblatt (1979, 2003), 245 Barenblatt (1996, 2003), 241 Barr (1995), 9 Bassini (2001), 245 Baˇzant (1967), 122 Baˇzant (1976), 7, 161, 170, 177 Baˇzant (1982), 9, 170 Baˇzant (1983), 18, 19, 25, 145, 191, 216 Baˇzant (1984), 5, 15, 18, 25, 145 Baˇzant (1984a), 7, 10, 86, 191, 216 Baˇzant (1984b), 9, 171, 172 Baˇzant (1984c), 168 Baˇzant (1985), 258 Baˇzant (1985a), 193 Baˇzant (1985b), 193, 209 Baˇzant (1986), 29 Baˇzant (1987), 25 Baˇzant (1987a), 144 Baˇzant (1990a), 179, 184 Baˇzant (1992a), 79

Baˇzant (1992b), 77, 78 Baˇzant (1993), 12, 13, 78, 122, 124, 152 Baˇzant (1994b), 171 Baˇzant (1995), 42 Baˇzant (1995c), 152 Baˇzant (1995d), 32, 38, 46, 69 Baˇzant (1996), 130, 255, 256 Baˇzant (1996a), 23, 32, 46, 131 Baˇzant (1996b), 113, 117, 118 Baˇzant (1997a), 21, 57, 133, 191, 206 Baˇzant (1997b), 9, 42, 71 Baˇzant (1997c), 42 Baˇzant (1998), 42 Baˇzant (1998a), 133, 197, 216 Baˇzant (1998b), 133 Baˇzant (1999a), 11 Baˇzant (1999b), 11, 212 Baˇzant (2000), 114, 115, 179, 191, 237 Baˇzant (2001, 2002), 235, 259 Baˇzant (2001a), 51, 212 Baˇzant (2001b), 219, 223 Baˇzant (2001c), 55 Baˇzant (2001d), 212 Baˇzant (2001e), 230 Baˇzant (2002), 245, 258, 259, 260 Baˇzant (2004a), 241 Baˇzant and Xi (1991), 62 Baˇzant and S ¸ ener (1997), 113 Baˇzant and Becq-Giraudon (1999), 162

322

Scaling of Structural Strength

Baˇzant and Becq-Giraudon (2001), 32 Baˇzant and Becq-Giraudon (2002), 258, 260 Baˇzant and Beissel (1994), 184 Baˇzant and Cao (1986a), 130 Baˇzant and Cao (1986b), 130 Baˇzant and Cao (1987), 113, 130 Baˇzant and Cao (2002a), 238 Baˇzant and Cedolin (1979), 7, 177 Baˇzant and Cedolin (1980), 7 Baˇzant and Cedolin (1991), 7, 17, 20, 90, 98, 158, 161, 173 Baˇzant and Chen (1997), 1, 12, 191, 248 Baˇzant and Estenssoro (1979), 10 Baˇzant and Frangopol (2000), 114, 117 Baˇzant and Gettu (1990), 32 Baˇzant and Gettu (1992), 151, 153, 173 Baˇzant and Jir´ asek (2001), 92 Baˇzant and Jir´ asek (1994a), 171 Baˇzant and Jir´ asek (1994b), 171 Baˇzant and Jir´ asek (2002), 258 Baˇzant and Kazemi (1990), 259 Baˇzant and Kazemi (1991), 216 Baˇzant and Kazemi (1991a), 35, 130 Baˇzant and Kazemi (1991b), 32, 206 Baˇzant and Kim (1991), 10 Baˇzant and Kim (1997), 79, 80 Baˇzant and Kim (1998), 85, 86 Baˇzant and Kwon (1994), 112, 113, 125 Baˇzant and Li (1995), 145, 259 Baˇzant and Li (1995), 43, 80, 165 Baˇzant and Li (1995a), 166, 178, 197 Baˇzant and Li (1995b), 36, 166, 178 Baˇzant and Li (1996), 47, 259

Baˇzant and Li (1996), 47, 248, 259, 260 Baˇzant and Li (1997), 151–153, 197, 210 Baˇzant and Lin (1988a), 9, 36 Baˇzant and Lin (1988b), 9, 172 Baˇzant and Nov´ ak (2000a), 57, 62 Baˇzant and Nov´ ak (2000b), 13, 56, 62, 66, 73, 197, 198 Baˇzant and Nov´ ak (2000a), 60, 125 Baˇzant and Nov´ ak (2000b), 125 Baˇzant and Oh (1983), 9, 36, 170, 177 Baˇzant and Pang (2004), 264 Baˇzant and Pfeiﬀer (1987), 25 Baˇzant and Pijaudier-Cabot (1988), 9, 172 Baˇzant and Planas (1998), 3, 24, 29, 30, 32, 43, 47, 57, 62, 93, 145, 177, 178, 184, 186, 191, 193, 197, 199, 202, 206, 210 Baˇzant and Raftshol (1983), 10 Baˇzant and Rajapakse (1999), 9, 11 Baˇzant and Schell (1993), 156 Baˇzant and Sun (1987), 130 Baˇzant and V´ıtek (1999), 101, 102, 107 Baˇzant and Wu (1993), 151 Baˇzant and Xi (1991), 58, 60 Baˇzant and Xiang (1996), 124 Baˇzant and Xiang (1997), 122, 124, 144 Baˇzant and Xu (1991), 156 Baˇzant and Yavari (2004), 265 Baˇzant and Yu (2002), 244, 258 Baˇzant and Yu (2003), 263 Baˇzant and Yu (2004), 245, 249, 255 Baˇzant, Yu and Zi (2002), 261, 262 Baˇzant et al. (1984), 172 Baˇzant et al. (1999), 137, 142, 145, 147, 148

Reference Citation Index

Baˇzant et al. (1999a), 144 Baˇzant et al. (1999b), 144 Baˇzant, Belytschko and Chang (1984), 171 Baˇzant, Belytschko and Chang (1984), 9 Baˇzant, Caner, Carol, Adley and Akers (2000), 168 Baˇzant, Daniel and Li (1996), 135 Baˇzant, ed. (1992), 9 Baˇzant, Guo, and Faber (1995), 173 Baˇzant, Lin and Lippmann (1993), 132 Baˇzant, Tabbara et al. (1990), 36 Baˇzant, Tabbara, Kazemi and Pijaudier-Cabot (1990), 174 Baˇzant, Xi and Reid (1991), 74 Baˇzant, S ¸ ener and Prat (1988), 113 Baˇzant, S ¸ ener and Prat (1988), 130 Baˇzant and Planas (1998), 26 Baˇzant, Pijaudier-Cabot and Pan (1987a), 161 Baˇzant, Pijaudier-Cabot and Pan (1987b), 161 Baˇzant, Zhou and Daniel (2003), 252, 253 Baˇzant, Zhou, Novak and Daniel (2004), 247, 254 Baˇzant, Zi and McClung (2003), 262 Bender and Orszag (1978), 25 Beremin (1983), 54, 67 Biot (1965), 122 Borodich (1992), 9, 69, 71 Bouchaud, Lapasset et Planes (1990), 9, 69 Bridgman (1922), 17 Brocca and Baˇzant (2000), 125 Brocca et al. (2001), 254 Brown (1987), 9, 69 Buckingham (1914), 17 Buckingham (1915), 17

323

Budianski (1983), 134 Budianski and Fleck (1994), 134 Budianski, Fleck and Amazigo (1997), 134 Cahn (1989), 9 Cahn (1989), 69 Carpinteri (1984), 18 Carpinteri (1986), 6, 9, 18 Carpinteri (1987), 249 Carpinteri (1989), 6 Carpinteri (1994a), 9, 10, 69 Carpinteri (1994b), 9, 69 Carpinteri and Chiaia (1995), 9, 10, 42, 69, 73 Carpinteri and Chiaia (1995a), 9 Carpinteri and Ferro (1994), 9, 10, 42, 69 Carpinteri, Chiaia and Ferro (1994), 9, 10, 42, 69 Carpinteri, Chiaia and Ferro (1995), 9, 10, 42, 69 Carpinteri, Ferro and Intervenizzi (1995), 9, 10, 42, 69 Carter (1992), 121, 132 Carter, Lajtai and Yuan (1992), 132 ˇ Cervenka and Pukl (1994), 9, 170 Chelidze and Gueguen (1990), 9, 69 Chen and Runt (1989), 9, 69 Christensen and DeTeresa (1997), 134 Collins (1978), 130 Collins and Mitchell (1980), 130 Collins, Mitchell, Adebar and Vecchio (1996), 130 Costin (1991), 121 Cotterell (1972), 121 Cottrell (1963), 32 Cundall (1971), 174 Cundall and Strack (1979), 174 Cusatis et al. (2003a,b), 260

324

Scaling of Structural Strength

Daniels (1945), 264 da Vinci (1500s), 3 de Borst and Guti´errez (1999), 174 Dempsey, Adamson and Mulmule (1995), 33 Dempsey, Adamson and Mulmule (1999), 33, 35 Duan and Hu (2003), 248, 259 Duan, Hu and Wittmann (2002, 2003), 255 Dugdale (1960), 7, 177 Dunn et al. (1997a,b), 249 Elices et al. (1992), 258 Eligehausen and Oˇzbolt (1992), 109 Evans and Marathe (1968), 173 Fairhurst and Cornet (1981), 121 Feng, Ji, Zhuang and Ding (1995), 9, 70 Fisher and Tippett (1928), 5, 6, 56 Fleck and Hutchinson (1993), 219 Fleck and Hutchinson (1997), 219 Fleck and Hutchinson (1997), 137, 219, 228 Fleck and Hutchinson (1963, 1997), 237 Fleck and Olurin (2001), 254 Fleck and Shu (1995), 137 Freudenthal (1968), 5, 6 Fr´echet (1927), 5, 56 Galileo (1638), 4 Gao and Huang (2000), 219 Gao, Huang and Nix (1999), 219, 237 Gao, Huang, Nix and Hutchinson (1999), 219 Gibson and Ashby (1997), 254 Giles (1962), 17 Griﬃth (1921), 5

Guinea, Planas and Elices (1994a,b), 258, 259 Guinea et al. (1997), 260 Hadamard (1903), 173 Haimson and Herrick (1989), 132 Hawkes and Mellor (1970), 121 Hill (1962), 173 Hillerborg (1985a), 32 Hillerborg (1985b), 32 Hillerborg, Mod´eer and Petersson (1976), 7, 32, 165, 178 Hinch (1991), 25 Horii and Nemat-Nasser (1982), 121 Horii and Nemat-Nasser (1986), 121 Hornbogen (1989), 9, 69 Hsu (1988), 130 Hu (1997, 1998), 255 Hu and Wittmann (1991, 1992a), 255 Huang, Gao, Nix and Hutchinson (2000), 219 Hutchinson (1997), 219, 228 Iguro, Shiyoa, Nojiri and Akiyama (1985), 130 Ingraﬀea (1977), 121, 170, 172 Ingraﬀea and Heuz´e (1980), 121 Irwin (1958), 22, 135 Issa, Hammad and Chudnovsky (1992), 9, 69 Jackson (1992), 252 Jenq and Shah (1985), 32 Jir´ asek and Baˇzant (1995a), 36, 174 Jir´ asek and Baˇzant (1995b), 36, 174, 175 Jir´ asek (1996), 171 Jir´ asek (2003), 258 Johnson et al. (2000), 252

Reference Citation Index

Kachanov (1985), 171 Kachanov (1987), 171 Kani (1967), 130 Kaplan (1961), 6 Karihaloo, Abdalla and Imjai (2003), 255 Kemeny and Cook (1987), 132 Kemeny and Cook (1991), 121, 132 Kendall (1978), 122 Kesler, Naus and Lott (1971), 7 Kfouri and Rice (1977), 7, 178 Kittl and Diaz (1988), 6 Kittl and Diaz (1989), 6 Kittl and Diaz (1990), 6 Knauss (1973), 7, 178, 179 Knauss (1974), 7, 178, 179 Kuhlmann and Breuninger (1998), 102 Kupfer (1964), 130 Kyriakides et al. (1995), 134 Lange, Jennings and Shah (1993), 9, 69 Lehner and Kachanov (1996), 121 Leicester (1969), 6, 7 Leonhardt (1977), 130 Leonhardt and Walther (1962), 130 Li and Baˇzant (1997), 151, 152 Long, Suquin and Lung (1991), 9, 69 Mahesh et al. (2002), 264 Maier and Zavelani (1970), 98 M˚ aløy, Hansen, Hinrichsen and Roux (1992), 9, 69 Mandel (1964), 173 Mandelbrot (1984), 9 Mandelbrot et al. (1984), 69 Mariotte (1686), 4 Marti (1980), 130 Marti (1989), 36 Mecholsky and Mackin (1988), 9, 69

325

Mihashi (1983), 6 Mihashi and Izumi (1977), 6 Mihashi and Rokugo (1998), 9 Mihashi and Zaitsev (1981), 6 Mindlin (1965), 219 M¨ orach (1922), 130 Mosolov and Borodich (1992), 9, 69, 71 Mulmule et al. (1995), 33 Murakami (1987), 87 Nakayama (1965), 32 Needleman (1990), 178 Nesetova and Lajtai (1973), 121, 132 Nielsen and Braestrup (1975), 130 Nixon (1996), 121 Oˇzbolt and Baˇzant (1996), 36, 172 Palmer and Rice (1973), 138, 140, 143, 144 Paris and Erdogan (1967), 154 Peerlings, de Borst, Brekelmans and de Vree (1996), 174 Peirce (1926), 5 Peng and Tian (1990), 9, 69 Petersson (1981), 9, 166, 178 Pheonix and Beyerlein (2000), 264 Pijaudier-Cabot and Baˇzant (1987), 9, 172 Planas and Elices (1986), 179, 184 Planas and Elices (1988), 9 Planas and Elices (1989a), 9 Planas and Elices (1989b), 9 Planas and Elices (1992), 178, 179, 184, 199, 216 Planas and Elices (1993), 9, 10, 178, 179, 184, 199, 216 Planas, Baˇzant and Jir´ asek (2001), 11 Porter (1933), 17 Prandtl (1904), 1, 193

326

Scaling of Structural Strength

Reineck et al. (2003), 263 Reinhardt (1985), 178, 179 Rice (1968a), 140, 178, 187, 256 Rice (1968b), 143, 144 Rice (1992), 178 Rice and Levy (1972), 80 RILEM (1990), 32 Ritter (1899), 130 Rocco (1995), 67 Rokugo, Uchida, Katoh and Koyanagi (1995), 67, 197 Rosen (1965), 134 Rots (1988), 9 Ruggieri and Dodds (1996), 54 R¨ usch and Hilsdorf (1963), 173 Sammis and Ashby (1986), 121 Sanderson (1988), 121 Saouma and Barton (1994), 9, 70 Saouma, Barton and Gamal-el-Din (1990), 9, 39 Schlaich, Schafer and Jannewein (1987), 130 Schlangen and van Mier (1992), 175 Schulson (1990), 121 Schulson and Nickolayev (1995), 121 Sedov (1959), 20, 193 S ¸ ener, Baˇzant and Becq-Giraudon (1999), 113 Shioya and Akiyama (1994), 130 Shioya, Iguro, Nojiri, Akiayama and Okada (1989), 130 Shipsa et al. (2000), 254 Slepyan (1990), 78, 79 Sluys (1992), 10 Smith (1974), 178, 179 Soutis, Curtis and Fleck (1993), 147 Steif (1984), 121 Streeter and Wylie (1975), 17 Suo, Bao, and Fan (1992), 178

Tandon, Faber, Baˇzant and Li (1995), 173 Tang et al. (1996), 259 Tattersall and Tappin (1966), 32 Taylor (1938), 168 thermal bending fracture, 77 Th¨ urlimann (1976), 130 Timoshenko (1953), 5 Tippett (1925), 5 Toupin (1962), 219 Tvergaard and Hutchinson (1992), 178 van Mier and Schlangen (1993), 175 von Mises (1936), 5, 56 Walraven (1978), 130 Walraven (1995), 130 Walraven and Lehwalter (1994), 130 Walsh (1972), 7 Walsh (1976), 7 Weibull, 4, 66 Weibull (1939), 6, 10, 53, 62 Weibull (1949), 6, 53 Weibull (1951), 53 Weibull (1956), 6, 53 Wells (1961), 32 Williams (1952), 249 Willis (1967), 178, 179 Wisnom (1991), 252 Wisnom and Atkinson (1997), 252 Wittmann (1990), 255 Wittmann and Zaitsev (1981), 121 Wittmann, ed. (1994), 9 Wnuk (1974), 7, 178, 179 Xie (1987), 9, 69 Xie (1989), 9, 69 Xie (1993), 9, 69 Xie and Sanderson (1995), 9, 69 Xie, Sanderson and Peacock (1994), 9, 69

Reference Citation Index

Young (1807), 5 Yuan, Lajtai and Ayari (1992), 132 Yuan, Lajtai and Ayari (1993), 121 Zaitsev (1985), 121 Zaitsev and Wittmann (1974), 6 Zech and Wittmann (1977), 6, 13, 56, 67 Zenkert and B¨ acklund (1989), 254 Zubelewicz and Baˇzant (1987), 175

327

SCALING OF STRUCTURAL STRENGTH Second edition Zdenˇek P Baˇzant

AMSTERDAM • BOSTON • HEIDELBERG • LONDON • NEW YORK • OXFORD PARIS • SAN DIEGO • SAN FRANCISCO • SINGAPORE • SYDNEY • TOKYO

Elsevier Butterworth-Heinemann Linacre House, Jordan Hill, Oxford OX2 8DP 30 Corporate Drive, Burlington, MA 01803 First published by Hermes Penton Ltd 2002 Second edition 2005 c 2005, Elsevier Ltd. All rights reserved Copyright The right of Zdenˇek P Baˇ zant to be identiﬁed as the author of this Work has been asserted in accordance with the Copyright, Designs And Patents Act 1988 No part of this publication may be reproduced in any material form (including photocopying or storing in any medium by electronic means and whether or not transiently or incidentally to some other use of this publication) without the written permission of the copyright holder except in accordance with the provisions of the Copyright, Designs and Patents Act 1988 or under the terms of a licence issued by the Copyright Licensing Agency Ltd, 90 Tottenham Court Road, London, England W1T 4LP. Applications for the copyright holder’s written permission to reproduce any part of this publication should be addressed to the publisher. Permissions may be sought directly from Elsevier’s Science and Technology Rights Department in Oxford, UK: phone: (+44) (0) 1865 843830; fax: (+44) (0) 1865 853333; e-mail: [email protected] You may also complete your request on-line via the Elsevier homepage (http://www.elsevier.com), by selecting ‘Customer Support’ and then ‘Obtaining Permissions’. British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library Library of Congress Cataloguing in Publication Data A catalogue record for this book is available from the Library of Congress ISBN

0 7506 6849 0

For information on all Elsevier Butterworth-Heinemann publications visit our website at http://books.elsevier.com Typeset by Newgen Imaging Systems (P) Ltd., Chennai, India Printed and bound in Great Britain

Working together to grow libraries in developing countries www.elsevier.com | www.bookaid.org | www.sabre.org

viii

Scaling of Structural Strength

9.8

Size Eﬀect Law Anchored in Both Small and Large Size Asymptotics . . . . . . . . . . . . . . . . . . . . . . . . . Recapitulation . . . . . . . . . . . . . . . . . . . . . . . .

213 215

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale . . . . . . . . . . . . . . . . . . . . . . . . . . . .

219

9.9 10

10.1. Scaling of Dislocation Based Strain-Gradient Plasticity 10.2. Scaling of Original Phenomenological Theory of Strain-Gradient Plasticity . . . . . . . . . . . . . . . 10.3. Scaling of Strain-Gradient Generalization of Incremental Plasticity . . . . . . . . . . . . . . . . . 10.4. Closing Observations . . . . . . . . . . . . . . . . . . 11

. . .

219

. . .

228

. . . . . .

236 237

Future Perspectives . . . . . . . . . . . . . . . . . . . . . . . . .

239

Addendum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A1. Size Eﬀect Derivation by a New Method for Asymptotic Matching . . . . . . . . . . . . . . . . . . . . . . . . . . . A2. Size Eﬀect of Finite-Angle Notches . . . . . . . . . . . . . A3. Size Eﬀect on Flexural Strength of Fiber-Composite Laminates . . . . . . . . . . . . . . . . . . . . . . . . . . A4. Size Eﬀect in Fracture of Closed-Cell Polymeric Foam . . . A5. Variation of Cohesive Softening Law Tail in Boundary Layer of Concrete . . . . . . . . . . . . . . . . . . . . . . A6. Can Fracture Energy Be Measured on One-Size Specimens with Diﬀerent Notch Lengths? . . . . . . . . . . . . . . . . A7. Notched–Unnotched Size Eﬀect Method and Standardization of Fracture Testing . . . . . . . . . . . . . . . . . . . . . . A8. Designing Reinforced Concrete Beams against Size Eﬀect . . A9. Scaling of Probability Density Distribution (pdf) of Failure Load . . . . . . . . . . . . . . . . . . . . . . . . . A10. Recent Debates on Fractal Theory of Size Eﬀect and Their Impact on Design Codes . . . . . . . . . . . . . . . . A11. Boundary Layer Size Eﬀect in Thin Metallic Films at Micrometer Scale . . . . . . . . . . . . . . . . . . . . . . . A12. Size Eﬀect on Triggering of Dry Snow Slab Avalanches . . .

241 241 249 252 254 255 258 260 262 264 264 265 267

Bibliography . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

269

Subject Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

313

Reference Citation Index

321

. . . . . . . . . . . . . . . . . . . . . . . .

34

Scaling of Structural Strength

0.0

0.0

2 1

2 1 -0.2

Concrete

SiC Ceramic

Gf = 0.041 N/mm -0.4 cf = 15 mm Ba zant & Pfeiffer (1987) -0.6 -0.8 -0.4

0.0

0.4

-0.8

0.4

0.8

0.0

Gf = 0.49 N/mm cf = 0.83 mm Ba zant & Zhou (2003) -1.2 0.0 0.4 0.8 1.2

1.6

2.0

0.0

log (σN / σ0)

Al Alloy

-0.2

Gf = 117 N/mm cf = 11.6 mm Ba zant, Lee, Pfeiffer

-0.4

-0.3

- 0.1

Limestone

-0.2

-0.2

1 Gf = 0.061 N/mm cf = 9.3 mm 2 Baz ant, Gettu & Kazemi (1991) -0.5 0.0

-0.4

0.0

-0.6

-0.4

-0.2

2

Marti (1989)

-1.0

-0.5

-0.5

fast medium slow Ba zant & Gettu (1992)

-0.7 -0.6 0.0

-0.2

Concrete

-0.2

0.2

0.6

2 1

-0.2

Concrete

Gf = 0.041 N/mm -0.4 cf = 15 mm Bazant & Pfeiffer (1987) -0.6 -1.0 -0.6 -0.2

1.0

0.5

0.0

0.0 2

1

1 -0.3

0.0

Double Punch

0.0

2 -0.1

2

Concrete

1

1

(1987) -0.3 -1.2 -0.8

2

0.0

2 -0.1

1

Gf = 0.109 N/mm cf = 17 mm -0.2 Ba zant, Prat & Tabbara (1990)

-0.8

0.0

0

1 -0.1

Vinyl Foam

-0.4

-1.5 -1

0.0 1

-0.4

Gf = 252 N/mm cf = 6.09 mm Ba zant, Daniel, Li (1996)

-0.4 -1.2

0.6

1

2 1

Carbon Composite

D ≤ 80 m

2

J. Dempsey et al. (1993) Arctic Ocean

0.0

2

Sea Ice

-1.0

-0.4 Gf = 0.039 N/mm cf = 1.36 mm McKinney & Rice -0.6 (1981) -0.2 0.2

0.0

-0.2

-0.5

-0.2

Concrete

0.2

G = 0.041 N/mm -0.4 c f = 15 mm f Ba zant & Pfeiffer (1987) -0.6 0.6 -0.8 -0.4 0.0

0.4

0.8

2 1

-0.4

SiO 2 Ceramic

Gf = 0.009 N/mm cf = 0.61 mm McKinney & Rice -0.8 (1981) -0.2 0.2 0.6

1.0

log (D / D0)

Figure 2.6: Nominal strength data and their ﬁts by size eﬀect law for notched specimen tests of carbon-epoxy composites (Baˇzant, Daniel and Li 1996), sea ice (Dempsey et al. 1999; record size range, up to 80 × 80 × 1.8 m), SiC and Si)O2 ceramics (McKinney and Rice 1981); Indiana limestone (Baˇzant, Gettu and Kazemi 1991), vinyl foam Divinycell 100 (Baˇzant and Zhou 2003), normal concrete (Baˇzant and Pfeiﬀer 1987, Baˇzant, Prat and Tabbara 1990) and tough aluminum alloy (Baˇzant, Lee and Pfeiﬀer 1987); all tests are in mode I except the cylinder test, which is in mode III

228

Scaling of Structural Strength

10.2. Scaling of Original Phenomenological Theory of Strain-Gradient Plasticity The development of strain-gradient plasticity for micrometer scale was pioneered by Fleck and Hutchinson (1993). Their ﬁrst version, called the couple-stress theory (CS theory), was later improved under the name of stretch and rotation gradients theory (SG theory) (Fleck and Hutchinson 1997). In this section, which closely follows the exposition in Baˇzant and Guo (2002a), the scaling of this, by now classical, theory, will be examined.

Fleck and Hutchinson’s Formulation In CS and SG theories, the strain energy density W is assumed to depend on the strain gradient tensor η of components ηijk ≡ uk,ij as well as the linearized strain tensor of components ij ≡ 12 (ui,j + uj,i ) (attention is here restricted to small strains). This assumption comes from the classical work of Toupin (1962) and Mindlin (1965), conﬁned to elastic behavior, and is expressed as 1 W = λii jj + µij ij + a1 ηijj ηikk + a2 ηiik ηkjj 2 + a3 ηiik ηjjk + a4 ηijk ηijk + a5 ηijk ηkji

(10.25)

where λ and µ are the normal Lam´e constants and an are additional elastic stiﬀness constants of the material. As in the classical theory, Cauchy stress σij is deﬁned as ∂W/∂ij , and is work-conjugate to ij . Furthermore, a higherorder stress tensor τ , work-conjugate to the strain gradient tensor η, is deﬁned as τijk = ∂W/∂ηijk . If W is deﬁned by (10.25), the constitutive relation is of course linear. So (10.25) is appropriate to linear isotropic elastic materials only. To extend it to general nonlinear elastic materials, a new variable, an invariant named combined strain quantity, E, is introduced by Fleck and Hutchinson (1997); it is deﬁned as a function of both the strain tensor and the strain gradient tensor, while the strain energy density W is assumed, for general nonlinear elastic material, to be a nonlinear function of E. To deﬁne E, Fleck and Hutchinson (1997) decompose the strain gradient tensor η into its hydrostatic part η H and deviatoric part η ; H ≡ ηijk

1 (δik ηjpp + δjk ηipp ); 4

η = η − ηH

(10.26)

To simplify the problem, only incompressible materials are considered in the H = 0 (which implies devimodeling of metals, in which case ij = ij and ηijk atoric strain gradient ηijk = ηijk ). Furthermore, Fleck and Hutchinson (1997)

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale

229

introduce the orthogonal decomposition η = η (1) + η (2) + η (3)

(10.27)

in which the three tensors are deﬁned in the component form as (1)

S ηijk = ηijk − (2)

1 S S S δij ηkpp + δki ηjpp + δjk ηipp 5

(10.28)

1 eikp ejlm ηlpm (10.29) + ejkp eilm ηlpm + 2ηijk − ηjki − ηkij 6 1 −eikp ejlm ηlpm = − ejkp eilm ηlpm + 2ηijk − ηjki − ηkij 6 1 S S S δij ηkpp + (10.30) + δjk ηipp + δki ηjpp 5

ηijk = (3)

ηijk

Here η S is a fully symmetric tensor deﬁned as S ηijk =

1 ηijk + ηjki + ηkij 3

(10.31)

Using the foregoing three tensors η (i) , Fleck and Hutchinson (1997) deﬁne the combined strain quantity E as E2 =

2 (1) (1) (2) (2) (3) (3) + 21 ηijk ηijk + 22 ηijk ηijk + 23 ηijk ηijk 3 ij ij

(10.32)

where i are three length constants which are given diﬀerent values in the CS and SG theories (which is the only major diﬀerence between these two theories): 5 1 CS (10.33) For CS: 1 = 0, 2 = CS , 3 = 2 24 5 1 CS For SG: 1 = CS , 2 = CS , 3 = (10.34) 2 24 Here CS is called the material characteristic length. Based on the combined strain quantity E as deﬁned, the strain energy density W can be deﬁned as a function of E instead of . Then Cauchy stress tensor σ and the higher-order stress tensor τ (couple stress tensor) can be expressed as: ∂W dW ∂E = ∂ik dE ∂ik ∂W dW ∂E = = ∂ηijk dE ∂ηijk

σik =

(10.35)

τijk

(10.36)

230

Scaling of Structural Strength

Using (10.32) and the condition of incompressibility, one has 2ik ∂E (10.37) = ∂ik 3E (1) (2) (3) ∂E 1 (1) ∂η (2) ∂η (3) ∂η 21 ηlmn lmn + 22 ηlmn lmn + 23 ηlmn lmn = ∂ηijk E ∂ηijk ∂ηijk ∂ηijk =

2CS Cijkmnl ηmnl E

(10.38)

where Cijkmnl is a six-dimensional constant dimensionless tensor which could be determined from (10.28), (10.29), (10.30) and (10.38). Obviously, the CS and SG theories will be characterized by diﬀerent tensors C, although, for each of them, tensor C is constant, that is, independent of , η and CS . For the sake of simplicity, the following power law is assumed for the strain energy density W (Fleck and Hutchinson 1997): n Σ0 E0 W = n+1

E E0

(n+1)/n (10.39)

where Σ0 , E0 and the strain hardening exponent n are taken to be material constants (and, for hardening materials, n ≥ 1; typically n ≈ 2 to 5). Thus (10.35) and (10.36) yield the constitutive relations σik τijk

1/n 1 2 = Σ0 E (1−n)/n ik 3 E0 1/n 1 = Σ0 2CS E (1−n)/n Cijklmn ηlmn E0

(10.40) (10.41)

The principle of virtual work yields the following ﬁeld equations of equilibrium (Fleck and Hutchinson 1997): σik,i − τijk,ij + fk = 0

(10.42)

Dimensionless Variables To analyze scaling, conversion to dimensionless variables (labeled by an overbar) is needed. Among many possible sets of such variables, the following

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale

231

will be convenient: x ¯i = xi /D, η¯ijk

u ¯i = ui /D, ¯ij = ij , = ηijk D, f¯k = fk D/σN

τ¯ijk = τijk /(Σ0 CS ), (l)

(l)

η¯ijk = ηijk D

where

σ ¯ik = σik /Σ0 ,

(10.43) E¯ = E

l = 1, 2, 3

(10.44) (10.45)

Here D is the characteristic length of the structure and σN is the nominal strength. Using these dimensionless variables, the constitutive law of the SGP theory can be rewritten as: 1/n 2 1 (10.46) σ ¯ik = E¯(1−n)/n ¯ik 3 E0 1/n CS 1 τ¯ijk = (10.47) Cijklmn E¯(1−n)/n η¯lmn E0 D The ﬁeld equations of equilibrium transform as ∂i σ ¯ik −

CS σN ¯ ∂i ∂j τ¯ijk + fk = 0 D Σ0

(10.48)

¯i = derivatives with respect to the dimensionless coordinates. where ∂i = ∂/∂ x After substituting (10.46) and (10.47) into (10.48), we obtain the diﬀerential equations of equilibrium in the form: 1/n 2 1 ∂i E¯(1−n)/n ¯ik 3 E0 2 1/n CS 1 σN ¯ − ∂i ∂j Cijklmn E¯(1−n)/n η¯lmn = − fk (10.49) D E0 Σ0 To avoid struggling with the formulation of the boundary conditions, consider ﬁrst that they are homogeneous, i.e., the applied surface tractions and applied couple stresses vanish at all parts of the boundary where the displacements are not ﬁxed as 0. All the loading characterized by nominal stress σN is applied as body forces fk whose distributions are assumed to be geometrically similar; σN is considered as the parameter of these forces, all of which vary proportionally to σN . Then the transformed boundary conditions are also homogeneous. In terms of the dimensionless coordinates, the boundaries of geometrically similar structures of diﬀerent sizes are identical. When the structure is not at maximum load but is hardening, one must decide which are the σN values that are comparable. What is meaningful is to compare structures of diﬀerent sizes for the same dimensionless displacement ﬁeld u ¯k . Thus, the comparable structures will have same ¯ik and η¯ijk .

232

Scaling of Structural Strength

Scaling and Size Eﬀect The problem of scaling and size eﬀect can now be fully discussed. The limit D/CS → ∞ is simple because the dimensionless third-order stresses τ¯ijk vanish and all the equations reduce to the standard ﬁeld equations of equilibrium on the macroscale. The combined strain quantity E reduces to the classical eﬀective strain, and (10.39) becomes the normal strain energy density function. The opposite asymptotic behavior for D/CS → 0 is a little more complex. From (10.32) we know that when D/CS → 0, 2 1 (1) (1) (2) (2) (3) (3) E¯ = ij ij + 2 21 η¯ijk η¯ijk + 22 η¯ijk η¯ijk + 23 η¯ijk η¯ijk ∝ D−1 (10.50) 3 D It is useful to deﬁne another dimensionless variable as follows:

(1) (1) (2) (2) (3) (3) ¯ = 1 H 21 η¯ijk η¯ijk + 22 η¯ijk η¯ijk + 23 η¯ijk η¯ijk CS

(10.51)

¯ is independent of size D, and we have Obviously H CS ¯ H E¯ ≈ D

when D/CS → 0

(10.52)

After substituting (10.52) into (10.49), we obtain the diﬀerential equations of equilibrium in the form: (1−n)/n 1/n 2 CS 1 ¯ (1−n)/n ¯ik ∂i H 3 D E0 (1+n)/n 1/n CS 1 ¯ (1−n)/n η¯lmn − ∂i ∂j Cijklmn H D E0 σN ¯ (10.53) =− fk Σ0 Now we multiply this equation by (D/CS )(n+1)/n and take the limit of the left-hand side for D → 0. This leads to the following asymptotic form of the ﬁeld equations: ∂i ∂j

¯ (1−n)/n η¯lmn = χf¯k , Cijklmn H

1 σ N with χ = E¯0n Σ0

D CS

n+1 n

(10.54)

Since D is absent from the foregoing ﬁeld equation (and from the boundary conditions, too, because they are homogeneous), the dimensionless displacement ﬁeld as well as the parameter χ must be size independent. Thus we obtain the following small-size asymptotic scaling law for Fleck and Hutchinson’s theories

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale

of gradient plasticity: σN or

−1/n = Σ0 χE¯0

CS D

233

(n+1)/n

σN ∝ D−(n+1)/n

(10.55) (10.56)

For hardening materials, we have 1 < (n + 1)/n ≤ 2. Since the surface loads may be regarded as the limit case of body forces applied within a very thin surface layer, the same scaling law must also apply when the load is applied at the boundaries. Although the result (10.56) applies only to the special case of strain energy density function (10.39), the same analytical technique can be used for general strain energy functions. Equation (10.56) indicates that the asymptotic behavior on the microscale depends on the hardening relation on the macroscale since the macro-strain-hardening exponent n is involved. Moreover, the asymptotic behavior depends only on that exponent. Generally, the present technique can be used for any strain energy function deﬁned in terms of the strain and strain gradient tensors, even if no combined strain quantity were deﬁned. For example, a similar technique can also be used for the strain energy density function (10.25) deﬁned for linear isotropic elastic material for which the combined strain quantity is not used. The constitutive relation in that case is: ∂W σik = = λδik ll + 2µik = (2µδil δkm + λδik δlm ) lm ∂ik = Diklm lm ∂W τijk = = [2a1 δil δjk δlm + a2 (δin δjk δlm + δij δkl δmn ) (10.57) ∂ηijk + 2a3 δij δlm δkn + 2a4 δil δjm δkn + 2a5 δin δjm δkl ]ηlmn =

Cijklmn ηlmn

(10.58)

where the dimension of tensor Diklm is that of a stress, and the dimension of tensor Cijklmn is that of a force. The dimensionless variables deﬁned in (10.43) can again be adopted. In terms of the dimensionless variables, the diﬀerential equations of equilibrium are: 1 1 1 ∂i (Diklm ¯lm ) − 3 ∂i ∂j Cijklmn η¯lmn + f¯k σN = 0 (10.59) D D D ¯ will vanish and (10.59) will become the For suﬃciently large D, the term with η classical diﬀerential equation of equilibrium. For the opposite case, for which

234

Scaling of Structural Strength

D is suﬃciently small, the term with ¯ will vanish, and we get the following asymptotic behavior: σN ∝ D−2

(10.60)

Of course, (10.60) is a special case of (10.56) because, for a linear material, the strain hardening exponent n = 1.

Examples It is instructive to verify the scaling law in (10.56) for the basic types of experiments. One important test is that of micro-torsion. It was initially the size eﬀect in this test (Fleck et al. 1997) which motivated the development of gradient plasticity. An eﬀective stress measure Σ may be deﬁned as the work conjugate to E: Σ=

dW (E) dE

(10.61)

A simple power law relationship between Σ and E may be adopted; Σ = Σ0 E N

(10.62)

Compared with (10.39), one sees that N = 1/n. For the analysis of size eﬀect, the radius of the wire, D, may be chosen as the characteristic dimension (size). The deformation is characterized by the twist per unit length, κ. For geometrically similar structures of diﬀerent sizes, we compare the nominal stresses corresponding to the same dimensionless twist κ ¯ = κD. The nominal stress σN may be deﬁned as T /D3 , where T is the torque. If the CS theory is used, one has 1 2 (N +3)/2 N +3 T 6π CS CS Σ0 κ + σN = 3 = (10.63) ¯N − 3 D N +3 D D For CS /D → ∞,

1 + 3

CS D

2 (N +3)/2 N +3 N +3 2 D CS CS N +3 − ≈ D 2 3CS D

(10.64)

σN ∝ D−N −1 = D−(n+1)/n

(10.65)

from which

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale

235

Small-Size Asymptotic Load-Deﬂection Response For some special cases such as the pure torsion of a long thin wire or the bending of a slender beam, the displacement distribution can be ﬁgured out by the arguments of symmetry and the relative displacement proﬁle remains constant during the loading process. For such problems, the asymptotic loaddeﬂection curve for a very small size D can be determined very easily (Baˇzant 2001, 2002). For such loading, all the dimensionless displacements u ¯k at all the points in a structure of a ﬁxed geometry increase in proportion to one parameter, w, such that u ¯k = wˆ uk where u ˆk is not only independent of D but also invariable during the proportional loading process. Parameter w may be deﬁned as the displacement norm, w = u ¯k . From (10.31), (10.28), (10.29), (10.30) and (10.32), we know that E¯ = wEˆ

(10.66)

where Eˆ is a function of dimensionless coordinates that does not change during the loading process when size D is very small. Substituting this into the dimensionless constitutive law (10.46) and (10.47), we have σ ¯ik = w1/n σ ˆik ,

τ¯ijk = w1/n τˆijk

(10.67)

where σ ˆik and τˆijk are constant during the loading process if the size D is small enough. Thus the load fk can now be expressed as a function of w as well as the size D. Since the ﬁrst two terms on the left-hand side of (10.48) are proportional, respectively, to the functions w1/n D(n−1)/n ,

w1/n D−(n+1)/n

(10.68)

one reaches the conclusion that f¯k ∝ w1/n

(10.69)

For hardening materials, we have 1/n ≤ 1. So the load deﬂection curve begins with a vertical tangent, similar to the MSG theory. We conclude that the smallsize asymptotic load-deﬂection response is similar to the stress–strain relation for the macroscale, except that the initial elastic response gets wiped out when D → 0.

236

Scaling of Structural Strength

10.3. Scaling of Strain-Gradient Generalization of Incremental Plasticity Finally, a brief look at the theory of Acharya and Bassani (2000) and Bassani (2001) is appropriate. These authors developed a simple gradient theory which diﬀers signiﬁcantly from the previous four theories. It is a generalization of the classical incremental theory of macro-scale plasticity, rather than the deformation (total strain) theory. In contrast to the previous four theories, in which the strain gradient tensor η is deﬁned as a third-order tensor representing the gradient of total strain, the lattice incompatibility is measured by a second-order tensor deﬁned by the following contraction of the gradient of plastic strain pij : αij = ejkl pil,k (10.70) where ejkl is the alternating symbol. The plastic hardening is assumed to be governed by the invariant: α = 2αij αji (10.71) Then the basic equations of the classical J2 ﬂow theory are modiﬁed as follows: σ σij ij τ= (10.72) = τcr , τ˙ = τ˙cr = h(γ p , α)γ˙ p 2 p 2 p p γ˙ p p p σij , σ˙ ij = Cijkl (˙kl − ˙kl ), γ = ˙ij = (10.73) 2τ 3 ij ij The variables used in the above are almost the same as in the classical J2 ﬂow theory except that the instantaneous hardening-rate function h depends not only on plastic strain invariant γ p but also on α. The following hardening function h(γ p , α) is used by Bassani (2001) for numerical simulation of the micro-torsion test: p 1/2 N −1 γ l2 (α/γ0 )2 1+ h(γ p , α) = h0 +1 (10.74) γ0 1 + c(γ p /γ0 )2 where l is a material length introduced for dimensionality reasons, and h0 , γ0 , c and N are further material constants (all positive). Although a full analysis of scaling of this theory is beyond the scope of this paper, some simple observations can be made. From the scale transformations u ¯i = ui /D, ¯il,k = il,k D, it follows that αij = α ¯ ij /D, where the overbars again denote the dimensionless variables. Since γ¯ p = γ p , the plastic hardening modulus deﬁned by (10.74) scales for D → 0 as p N −1 −1/2 α γ ¯ l h(γ p , α) = h0 1 + c(γ p /γ0 )2 +1 (10.75) ∝ D−1 γ0 γ0 D

Size Eﬀect at Continuum Limit on Approach to Atomic Lattice Scale

237

This means that, at the same strain level, the slope of the plastic hardening curve increases as D−1 when D → 0. When the plastic strain becomes much larger than the elastic strain, and when the strain distributions and history are similar, then of course the nominal stress σN must also scale asymptotically as D−1 . This is again a curiously strong asymptotic size eﬀect, not much less strong than that found for the MSG and CS theories. Even though this excessive size eﬀect is approached only outside the range of applicability of the theory, one must expect that it would impair the representation of test data in the middle range. The excessive asymptotic size eﬀect could be avoided by redeﬁning the plastic hardening modulus in (10.74) as follows: h(γ p , α) = h0

1/2 N −1 γp lα/γ0 1+ +1 γ0 1 + c(γ p /γ0 )

(10.76)

With this revision, which should be checked against test data, the asymptotic scaling would become h(γ p , α) ∝ D−1/2

when D → 0

(10.77)

which seems more reasonable and similar to Baˇzant’s (2000) proposal for revision of MSG theory, as well as to the TNT theory.

10.4. Closing Observations The small-size asymptotic scaling laws for the nominal stress σN in all the existing theories are power laws, but there are wide disparities among them. For Gao et al.’s (1999) MSG theory, in general, σN ∝ D−5/2 , which is an unreasonably strong size eﬀect. For two special cases of this theory, σN ∝ D−2 and D−3/2 , which is also very strong. For the classical Fleck and Hutchinson (1963, 1997) CS and SG theories, σN ∝ D−(n+1)/n where n is the exponent of the strain hardening law on the macroscale, and typically σN ∝ D−1.3 , which is also quite strong. For the TNT theory, as well as for the modiﬁcation of the MSG theory proposed by Baˇzant (2002, 2000), σN ∝ D−1/2 , which seems reasonable. The plastic hardening modulus in the theory of Acharya and Bassani (2000) scales asymptotically as D−1 , which also seems excessive. However, a simple modiﬁcation can achieve the scaling of D−1/2 .

238

Scaling of Structural Strength

Although the small-size asymptotic behavior is closely approached only at sizes much smaller than the range of applicability of the strain-gradient theories of plasticity (which is about 0.1 µm–100 µm), the knowledge of this behavior is useful for developing asymptotic matching approximations for the realistic middle range. Knowledge of both the large-size and small-size makes it possible to obtain good analytical approximations for the middle range of interest, agreeing with experimental as well as numerical results (see Baˇzant and Guo 2002a). The availability of such formulae means that the stress analysis for the middle range, which is much more diﬃcult than the asymptotic analysis, can in principle be avoided. Such an approach is, of course, possible only if the small-size asymptotic behavior is realistic. The detrimental consequence of unrealistic small-size asymptotic properties is that the possibility of asymptotic matching approximations is lost.

Addendum Most of the manuscript for the ﬁrst printing was completed in 2000. Since then research in strength scaling has been progressing rapidly; recent advances are brieﬂy described in this Addendum, and some additional references are added at the end of the bibliography. A1. Size Eﬀect Derivation by a New Method for Asymptotic Matching Summary of asymptotic properties of cohesive crack model A simpler, more general and more fundamental derivation of the scaling laws can be obtained by combining dimensional analysis with a new method of asymptotic matching of the known asymptotics of the cohesive crack model (Baˇzant 2004a). Asymptotic matching is a broad range of diverse techniques used for a long time in ﬂuid mechanics (Barenblatt 1996, 2003), none of which, however, seems suited for fracture mechanics of solids. The basic hypothesis is that the cohesive crack model represents a good enough compromise between reality and simplicity. The fracture process zone (FPZ) at the crack front is modeled as a ﬁctitious line crack transmitting cohesive (crack-bridging) stresses σ = f (w); w = crack opening (separation), f (w) = monotonically decreasing (softening) function characterizing the material (Fig. A.1 bottom left), with f (0) = ft = tensile strength of material. The initial tangent of f (w) is assumed to have a ﬁnite negative slope f (0), which is proportional to fracture energy Gf . In Chapter 2 and 9 it was shown that, depending on the ﬁrst two non-zero terms of the asymptotic expansions of σN in terms of powers of D and of D−1 , there exist three and only three types of size eﬀect (Baˇzant 2001): For D → 0 : σN = b0 − c0 D + · · · For D → ∞: σN = b1 + c1 D−1 + · · · σN = D

−1/2

σN = D

−1/2

(all types)

(A1.1)

(type 1)

(A1.2)

[b2 − c2 D

−1

+ · · · ] (type 2)

(A1.3)

[b3 − c3 D

−2

+ · · · ] (type 3)

(A1.4)

where b0 , c0 , . . . , c3 are positive constants determined by structure geometry. Type 1 (Fig. A.1 left) occurs if the geometry is such that Pmax is reached at crack initiation from an FPZ attached to a smooth surface, i.e., as soon as the FPZ is fully formed. Type 2 (Fig. A.1 right) occurs if there is a large notch or preexisting stress-free (fatigued) crack and if the geometry is positive, i.e., such

242

Scaling of Structural Strength

1

Type 1

log(σN/σ0)

r

Type 3

1

FM LE

1

Type 2 0.1

Weibu m n ll 1

10

100

2 1

0.1 0.1

1

10

100

log (D/D0) Figure A.1: Size eﬀects of types 1, 2, and 3, and their asymptotes

that Pmax occurs while the FPZ is still attached to the tip. Type 3 occurs if a large crack can grow stably prior to Pmax (negative geometry). The size eﬀect types 1 and 2 are very diﬀerent, but types 2 and 3 are quite similar and hardly distinguishable in fracture testing (note that, in Chapter 9, type 1 was called Case 2, type 2 Case 1, and type 3 Case 3).

Asymptotic matching law for the case of large notch or crack From Buckingham’s Π-theorem of dimensional analysis (Barenblatt 1979), two special size eﬀects have been proven in section 1.7:

(a) If the failure depends on ft (dimension N/m2 ) but not Gf , then there is no size eﬀect, i.e., σN = constant (this is so for all elasto-plastic failures). (b) If the failure depends on Gf (dimension J/m2 ) but not on ft , then there is a size eﬀect of the type σN D−1/2 (this is so for LEFM, if the cracks or notches are geometrically similar).

Addendum

243

Nothing more can be deduced from dimensional analysis alone. We can, however, deduce more information upon considering the physical meaning of the material characteristic length governing the FPZ size, l0 = EGf /ft2 , introduced by Irwin (1958). The length and width of the FPZ for D → ∞ are ηl0 and η l0 , in which η and η are constants of the order of 1, depending on microstructure characteristics (note that the parameter le = Gf /E, which is also a length, is irrelevant for failure and controls only the ratio of deformation to stress intensity factor KI in LEFM). Depending on the ratio D/l0 , two asymptotic cases may be distinguished: (a) If D/l0 → 0, the body is much smaller than a fully developed FPZ. Then a derivative of potential energy with respect to the crack length makes no sense, and so Gf cannot matter. Therefore, the case of no size eﬀect, σN = constant, is the small-size asymptote. (b) If D/l0 → ∞, the FPZ becomes a point in dimensionless coordinates ξ = x/D and the stress ﬁeld approaches the LEFM singularity. So, ft cannot matter. Therefore, the LEFM scaling, σN ∝ D−1/2 , is the largesize asymptote of quasibrittle failure (which is represented by a straight line of slope −1/2 in the plot of log σN versus log D). The size eﬀect curve for the intermediate sizes may be expected to be a gradual transition between these two asymptotes. The approximate form of this transition can be deduced upon noting how the asymptotes are approached, i.e., by exploiting the higher-order asymptotic terms in (A1.1) and (A1.3). By transformation to dimensionless variables in the formulation of the boundary value problem with cohesive crack, one concludes that (if the ratios of structural dimensions characterizing the structure geometry are ﬁxed) σN depends on only three parameters, ft , D and Kc , where, for plane stress states, Kc =(EGf )1/2 = mode I fracture toughness and E = Young’s modulus (for plane strain states, E needs to be replaced by E = E/(1 − ν 2 ) where ν = Poisson ratio). Therefore, we have now four governing parameters, σN , D, ft and Kc . Since they involve 2 independent physical dimensions (length and force), the Π-theorem (Barenblatt 1979) implies that there can be only 4 − 2, i.e., 2 independent dimensionless parameters, Π1 and Π2 . So, the equation governing failure may be written as F (Π1 , Π2 ) = 0 where function F may be assumed to be suﬃciently smooth. Although many diverse choices of Πi (i = 1, 2) are possible, the key idea was to make a choice for which, in each asymptotic case, all Πi vanish except one (Baˇzant 2004a). If consideration is limited to dimensionless monomials, this can be most generally achieved by choosing: Π1 = (σN /ft )p (D/l0 )u ,

Π2 = (σN /ft )q (D/l0 )v

where p, q, u, v are four unknown real constants.

(A1.5)

244

Scaling of Structural Strength

If we let Π1 = 0 correspond to D → 0, then F (0, Π2 ) = 0. This implies that Π2 = constant or σN q Dv = constant for D → 0, which must be the case of no size eﬀect; hence v = 0. If we let Π2 = 0 correspond to D → ∞, then F (Π1 , 0) = 0, which implies that Π1 = constant or σN p Du = constant, or σN ∝ D−u/p for D → ∞. This must be the LEFM scaling; hence u/p = 1/2 or u = p/2. To ﬁnd p and q, we expand function F into Taylor series about the state Π1 = Π2 = 0, and truncate this series after the linear terms; i.e., F (Π1 , Π2 ) ≈ F0 + F1 Π1 + F2 Π2 = 0 √ or F1 (σN D/ft l0 )p + F2 (σN /ft )q = −F0

(A1.6) (A1.7)

where F1 = [∂F/∂Π1 ]0 and F2 = [∂F/∂Π2 ]0 (evaluated at Π1 = Π2 = 0) and F0 = F (0, 0) (F0 , F1 , F2 = 0). Now we need to compare the last equation with the asymptotic expansion in (A1.3). But this cannot be done in general because, for general p/q, the last equation cannot be solved explicitly for σN . But it can be solved for D, which gives 2/p

D = l0 ft 2 (−F0 /F1 )2/p σN −2 [1 + (F2 /F0 ftq )σN q ]

(A1.8)

which may be compared to the inverse expansion of the large-size asymptotic expansion in (A1.3). This inverse expansion has the form D = B2 σN −2 [1 − C2 σN 2 + · · · ]

for σN → 0

(A1.9)

where B2 and C2 are positive constants. Evidently, matching of the ﬁrst two terms of this expansion requires that p = q = 2. Then Eq. (A1.7) can be solved for σN . This yields, and veriﬁes, the size eﬀect law, Eq. (2.8), i.e., σN = σ0 ( 1 + D/D0 )−1/2 in which

Bft = ft (−F0 F2 )−1/2 ,

D0 = l0 F2 /F1

(A1.10) (A1.11)

For D → 0, Eq. (2.8) has the approximation: σN ≈ Bft (1 − D/2D0 )

(A1.12)

which veriﬁes that the form of the second term of small-size expansion in (A1.1) can be matched, too. So, Eq. (A1.10) is the simplest formula for type 2 size eﬀect that can match the form of four asymptotic terms, two for D → 0 and two for D → ∞. If, however, not only the form of the second-order terms but also the values of all four coeﬃcients b0 , c0 , b2 , c2 are given, a slightly more general formula with four adjustable parameters is needed. This formula was recently developed and examined in Baˇzant and Yu (2002), with the purpose of a identifying fracture

Addendum

245

energy Gf from the maximum load of notched and unnotched test specimens of relatively small sizes. More complex formulas of the same asymptotic accuracy, but more ﬂexible in data ﬁtting, can be obtained by replacing (A1.5) with dimensionless polynomials (or other monotonic functions of Π1 and Π2 ). Such formulas can make a signiﬁcant diﬀerence only if the size eﬀect needs to be modeled for a size range exceeding about 1 21 order of magnitude of D. Their merit is that they can capture a spectrum of fracture energies (Baˇzant 2002f), each of which is associated with a diﬀerent order of magnitude of D (see section 9.7). The type 3 (Case 3) size eﬀect formula (Fig. A.1 right) can be derived similarly. Asymptotic matching law for failures at crack initiation (type 1 scaling) The deterministic (type 1) size eﬀect for failures at macrocrack initiation from a smooth surface necessitates a somewhat diﬀerent approach. As explained in section 2.8 (Fig. 2.13), the source of this size eﬀect is the stress redistribution due to a boundary layer of cracking (or formation of the FPZ at the surface), which is associated with energy release. The deterministic type 1 size eﬀect is also called the strain gradient eﬀect, but this is not quite accurate because, aside from the local strain gradient at the surface, the geometry of the whole structure also has some (albeit small) inﬂuence on the strain redistribution and energy release. This is clear from the alternative approach used in section 2.7, in which the type 1 failure has been treated as a limit case of ﬁnite crack for a0 → 0 (Baˇzant 1997, 1998), with the energy release rate approaching zero. For general dimensional analysis, we need a slightly diﬀerent procedure than for type 2. Let us consider the deterministic type 1 ﬁrst (m → ∞). Because, according to (A1.1) and (A1.2), both asymptotes in the plot of log σN versus log D must be horizontal, the size eﬀect curve of σN versus log D must have an inﬂexion point. Thus it is convenient to postulate the existence of what is called an intermediate asymptote (Barenblatt 1979, 2003), which consists of some unknown power law. Because the intermediate asymptote separates the large-size and small-size asymptotics, we must ﬁrst match the large-size asymptotic terms alone (which was the approach taken in sections 2.7 and 9.4.2). We choose the large-size asymptote to correspond to Π1 = 0, i.e., to F (0, Π2 ) = 0. This requires that Π2 = constant for D → ∞, and so v = 0 in (A1.5). We again truncate the Taylor series expansion of function F (Π1 , Π2 ) after the linear terms, i.e., use the linear approximation (A1.6). This equation cannot, in general, be solved

246

Scaling of Structural Strength

for σN , but it can for D, which yields: l0 /D = (−F0 /F1 )−1/u [(ft /σN )p + (F2 /F0 )(ft /σN )p−q ]−1/u

(A1.13)

The large-size expansion (A1.2) may be generalized as σN = (b1 + rc1 D−1 + · · · )1/r (r = arbitrary constant = 0). Although we cannot match the asymptotic expansion (A1.2) directly, we can match the inverse expansion, which can be shown to be 1/D = (−b1 + σN r + · · · )/rc1

(A1.14)

Matching of (A1.13) obviously requires that u = −1 and p = q = −r in (A1.5). So (A1.15) Π1 = (ft /σN )r l0 /D, Π2 = (ft /σN )r With these particular expressions, Eq. (A1.6) can be solved for σN . This yields, and thus also veriﬁes, the type 1 size eﬀect law 1/r

σN = fr0 (1 + rλ/D)

(type 1, m → ∞)

(A1.16)

(equivalent to Eq. 2.39), in which λ = F1 /rF2 ,

fr0 = ft (−F2 /F0 )1/r

(A1.17)

Second, consider the statistical generalization, i.e., Weibull modulus m < ∞. Instead of the horizontal asymptote (A1.1), the mean large-size asymptotic size eﬀect (as explained in section 3.1, Eq. 3.6) is now given by the Weibull power law (A1.18) for D → ∞ : σN = k0 D−n/m + · · · (type 1) where m = Weibull modulus, k0 = constant, and n = number of dimensions in which the structure is scaled (n = 1, 2, 3); typically, m = 10 to 40 and n/m 1. In the plot of log σN versus log D, this power law represents an inclined straight line asymptote of slope −n/m. The Weibull power law size eﬀect (A1.18) must apply for failures at crack initiation if the FPZ is negligible compared with D. We again choose the large size asymptote to correspond to Π1 = 0 and Π2 = constant. To match (A1.18), it is necessary that σN = C1 D−n/m ∝ ft (D/l0 )−v/q , and so, v/q = n/m. If we should not loose the deterministic limit already ﬁgured out, we must keep p = q = −r and u = −1. With these values, Eq. (A1.6) can now be solved for σN . This leads to the mean type 1 energetic-statistical size eﬀect: 1/r σN = fr0 (λl0 /D)rn/m + rκ(λl0 /D) (A1.19) equivalent to Eq. 3.9; here fr0 = λ−n/m (−F2 /F0 )1/r , κ = λrn/m−1 F1 /F2 r, and r is a parameter of the order of 1, sensitive to structure geometry. For

Addendum

247

large D, the ﬁrst term dominates, and so σN ∝ D−n/m , which agrees with the asymptotic requirement in (A1.18). Furthermore, for m → ∞, the asymptotic scaling of Eq. (A1.2) is matched because Eq. (A1.19) takes the form σN = s0 (1 + κrλl0 /D)1/r ≈ s0 (1 + κλl0 /D). Eq. (A1.19), however, is separated by the intermediate asymptote from the small-size asymptotics in (A1.1), and does not match that asymptotics. It must, therefore, be further modiﬁed, but without aﬀecting the ﬁrst two large-size asymptotic terms. To bridge the small-size and intermediate asymptotes, we could engage in similar arguments as we did for bridging the large-size and intermediate asymptotes. Suﬃce to say, the complete law for the mean size eﬀect of type 1 (Fig. A.1 left), matching the small-size asymptotics in (A1.1), can simply be obtained by replacing λl0 /D in Eq. (A1.19) with θ, as follows: 1/rs σN = fr0 θrn/m + rsκθ , θ = (1 + D/sηl0 )−s λ/η (A1.20) where η = positive constant of the order of 1, and s may be taken as 1. Note that the intermediate asymptote is deﬁned by inﬁnite separation of the characteristic lengths involved, ηl0 and λl0 . If we let ηl0 D λl0 , i.e., if we consider the limiting process λ/η → ∞, Eq. (A1.20) converges to an intermediate asymptote, given by the power law σN = fr0 (la /D)1/r

(A1.21)

in which la = sη(rsκλ/η)1/r = constant, and becomes inﬁnitely close to the small-size asymptote of (A1.19), as well as to the large size asymptote of σN = fr0 θn/m (given by Eq. 3.6), which passes through the aforementioned inﬂexion point. The physical reason for the existence of an intermediate asymptote is that normally the size of averaging domain in nonlocal Weibull theory (roughly equal to FPZ width) is much smaller than the FPZ length. Eq. (A1.20) is supported by ﬁnite element simulations with nonlocal Weibull theory, as well as test data from ten diﬀerent labs (all combined in one dimensionless plot in Fig. 3.6). However, test data for concrete and composites show that the D values for which the diﬀerence between (A1.19) and (A1.20) is signiﬁcant are less than the material inhomogeneities, which means that (A1.19) should mostly suﬃce in practice. For bending of laminates or unreinforced concrete beams, the Weibull statistical component in (A1.19) or (A1.20) is usually insigniﬁcant for normal sizes (Baˇzant Zhou, Nov ’ak and Daniel 2004). It becomes signiﬁcant only for bending of very large structures, such as arch dams. For bending of unreinforced concrete beams or plates, for which the size eﬀect is generally of type 1, the Weibull statistical component normally becomes signiﬁcant only for cross sections at least several meters thick (as typical of arch dams).

248

Scaling of Structural Strength

Universal Size Eﬀect Law The size eﬀect for crack initiation from a smooth surface (a0 = 0) has been shown to be very diﬀerent from the size eﬀect for large notches or large stressfree (fatigued) cracks at maximum load (for which a0 /D is not too small). As far as the mean nominal strength of structure, σN , is concerned, the former is always energetic (i.e. purely deterministic), while the latter is purely energetic only for small enough sizes and becomes statistical for large enough sizes. It is of interest to ﬁnd a universal size eﬀect law that includes both of these size eﬀects and spans the transition between them. A formula for this purpose was proposed in Baˇzant and Li (1996) (also Baˇzant and Chen 1997); see Eq. (2.52) and Fig. 2.14. However, that formula is not smooth and does not include the statistical (Weibull) part for crack initiation failures. A better formula (Baˇzant and Yu 2004) is shown in Fig. A.2—on the left (Fig. A.2a) without, and on the right (Fig. A.2b) with, the statistical (Weibull)

Figure A.2: Universal size eﬀect law (improvement of Fig. 2.14); top left—without, and top right—with Weibull statistics; bottom—proﬁles obtained from the universal size eﬀect law, compared to Duan and Hu’s (2003) approximation

Addendum

249

part (E = eﬀective Young’s modulus for plane stress or plane strain), ft = local tensile strength of material; g0 , g0 , g0 are values of dimensionless energy release function g(a) and its derivatives at α0 = a0 /D; l0 = E Gf /f t2 = Irwin’s characteristic length (corresponding to the initial fracture energy Gf ); g(a) = [k(a)]2 , k(a) is the dimensionless stress intensity factor; m = Weibull modulus of concrete (about 24), n = number of dimensions for scaling; r, k = empirical positive constants; and cf = constant (the ratio cf /l0 depends on the softening curve shape, and cf ≈ l0 /2 for triangular softening). The formulas in Figs. F1a,b were derived by asymptotic matching of 7 cases: the small-size and large-size asymptotic behaviors (ﬁrst two terms of expansion for each), of the large-notch and vanishing-notch behaviors, and of Weibull size eﬀect. A2. Size Eﬀect of Finite-Angle Notches In elastic bodies, a sharp notch of a ﬁnite angle (Fig. A.3) causes stress singularity σ ≈ rλ−1 that is weaker than the crack singularity (i.e., λ > 0.5) and is given by Williams’ (1952) formulas (a)–(e) shown in Fig. A.3, in which r, φ = polar coordinates and σ = σrr , σφφ , σrφ = near-tip stresses. If the structure has a positive geometry, it will fail as soon as a FPZ of a certain characteristic length 2cf is fully formed at the notch tip. In the limit of D → ∞, the structure will fail as soon as a crack can start propagating from the notch tip, in which case the critical energy release rate must equal Gf . Experiments show that the load (or nominal stress σN ) at which this occurs increases with angle γ. In previous studies (e.g., Carpinteri 1987, Dunn et al. 1997a,b), some arguments in terms of a non-standard ‘stress intensity factor’ Kγ corresponding to singularity exponent 1−λ < 0.5 were used to propose that the nominal stress σN ∝ Dλ−1 . A notch of ﬁnite angle cannot propagate, and a stress singularity of a power other than 1/2 cannot supply a ﬁnite energy ﬂux. So, a realistic approach requires considering that a cohesive crack must propagate from the notch tip (Fig. A.3 left; Baˇzant and Yu 2004). Circular bodies with notches of various angles 2γ (and ligament dimension D, Fig. A.3a) were simulated by ﬁnite elements with a mesh progressively reﬁned as r → 0 (the ﬁrst and second rings of elements spanned from 0 to r = D/6000 and then to D/3000). The circular boundary was loaded by normal and tangential surface tractions equal to stresses σrr and σrφ taken from Williams symmetric (mode I) solution; P = load parameter representing the resultant of these tractions; and σN = P/bD = nominal stress (b = 1). First, ligament D was considered to be so large that the length of the FPZ, lc , was less than 0.01D. In that case, the angular distribution of stresses along each circle with r ≥ 0.1D ought to match Williams functions frr , frφ , fφφ . Indeed, the numerical results cannot be visually

250

Scaling of Structural Strength

Figure A.3: (a) Angle-notched circular specimen considered for analysis. (b) Numerically computed singularity exponent compared to Williams’ elastic solution. (c) Computed variation of nominal strength with notch angle. (d) Curve of analytical size eﬀect law for angular notches compared to the results of cohesive crack model distinguished from these functions. The logarithmic plots of the calculated stress versus r for any ﬁxed φ (and any γ) were straight lines, and their slopes agreed with the exponent λ − 1 required by Williams solution; see Fig. A.3 (right). This serves to conﬁrm the correctness of the cohesive ﬁnite element simulation. From Eqs. (b), (f), and (g) of Williams’ LEFM solution in Fig. A.3, σN = (r/D)1−λ σφφ ψ(γ)/fφφ (0, γ)

(8)

(A2.1)

According to the equivalent LEFM approximation of cohesive fracture, σφφ for r = cf (the middle of FPZ), should be approximately equal to material tensile strength ft . This condition yields σN = ft (D/Hr )λ(γ)−1 ,

Hr = cf [fφφ (0, γ)/ψ(γ)]

(9)

(A2.2)

Addendum

251

which is for D ≥ 250l0 indistinguishable graphically. Eq. (A1.19), however, violates the small-size asymptotics in (A1.1), and must therefore be further modiﬁed, but without aﬀecting the ﬁrst two large-size asymptotic terms. To bridge the small-size and intermediate asymptotes, we could engage in similar arguments as we did for bridging the large-size and intermediate asymptotes. Suﬃce to say, the complete law for the mean size eﬀect of type 1 (Fig. A.1d), matching the small-size asymptotics in (A1.1), is obtained by replacing λ/D in Eq. (A1.19) with θ: 1/r σN = fr0 θrn/m + rκθ , θ = (1 + D/sη)−s λ/η (A2.3) where η = positive constant of the order of 1 and s may be taken as 1; λ(γ) is the λ value for angle γ. To check this equation, geometrically similar scaled circular bodies of diﬀerent ligament dimensions D (Fig. A.3) were analyzed by ﬁnite elements for various angles γ using the same linear softening stressseparation diagram of cohesive crack. The numerically obtained values of log σN for various ﬁxed D/cf are plotted in Fig. A.3c as a function of angle γ. We see that this size eﬀect curve matches perfectly the curve of Eq. (A2.2) for D/cf > 500, conﬁrming that the equivalent LEFM approximation obtained for r = cf is good enough. A general approximate formula for the size eﬀect of notches of any angle, applicable to any size D, may be written as follows: λ(γ)−1 H0 D σN = σ0 1 + (A2.4) Hγ D0 where H0 = hγ -value for γ = 0, and D0 is given in terms of g(α) and is the same as for a crack (γ = 0). Eq. (A2.4), which is of course valid only for large enough notches penetrating through the boundary layer of concrete, has been derived by asymptotic matching of the following asymptotic conditions: 1. for γ → 0, the classical size eﬀect law σN = σ0 (1 + D/D0 )−1/2 must be recovered; 2. for D/l0 → 0, there must be no size eﬀect; 3. for D/l0 → ∞, Eqs. A2.4 and A2.2 must coincide; 4. for γ = π/2 (ﬂat surface), the formula must give no size eﬀect for D → ∞. In reality, there is of course a size eﬀect in the last case, but it requires a further generalization of Eq. (A2.4) (which will be presented separately). Therefore, Eqs. (A2.4) and (A2.2) can be applied only when the notch is deeper than

252

Scaling of Structural Strength

the boundary layer, which is at least one aggregate size. Complete generality will require amalgamating Eq. (A2.4) with the universal size eﬀect law in Fig. A.2. The plot of log σN versus log D for γ = π/3 according to Eq. (F28) is compared to the ﬁnite element results for notched circular bodies with cohesive cracks in Fig. A.3d. The agreement is seen to be excellent.

A3. Size Eﬀect on Flexural Strength of Fiber-Composite Laminates The failure of ﬁber-polymer laminates is in general practice still treated according to the strength theory or plastic limit analysis, which exhibits no size eﬀect, and all the size eﬀects are considered as purely statistical. A recent systematic analysis by Baˇzant, Zhou and Daniel (2003), based on the ﬂexural strength tests of Jackson (1992), Johnson et al. (2000), Wisnom (1991), Wisnom and Atkinson (1997) and others, conﬁrms that such practice in unrealistic. The problem is that if the available size eﬀect data on ﬂexural strength of ﬁber-polymer laminates are considered alone, they can be ﬁtted well enough by Weibull statistical size eﬀect theory. However, to conclude that this theory applies is deceptive for two reasons: (1) the size range of the existing data is quite limited, and the energetic theory for size eﬀect at crack initiation due to a boundary layer can ﬁt these data equally well; and (2) checks of the coefﬁcient of variation of ﬂexural strength, ωW , have been omitted. These checks are essential. Weibull statistical theory cannot be correct if the ωW -value does not agree with the value of Weibull modulus m, and if this agreement is not obtained for every size. The ωW values must satisfy the well-known formula of Weibull theory, Eq. (3.3), i.e., ωW = [(Γ(1 + 2/m))/(Γ2 (1 + 1/m) − 1]−1/2 . Even though the available size eﬀect data for laminate ﬂexure did not include measurements of ωW , it is easy to ascertain that the foregoing equation is not satisﬁed. For example, Jackson et al.’s (1992) tests included four diﬀerent layups—unidirectional, quasi-isotropic, cross-ply and angle ply. To ﬁt these size eﬀect data, the optimum m values vary widely from case to case, ranging from m = 5 to m = 30. According to the foregoing relation, ωW = 22.8% for m = 5,

ωW = 4.18% for m = 30

(A3.1)

for angle-ply and unidirectional laminates, respectively. Although the coeﬃcient of variation of ﬂexural strength has not been reported for the test data considered, such huge diﬀerences in scatter go against all experience, and are evidently implausible. The angle-ply laminate, due to its greater ductility

Addendum

253

Figure A.4: Type 1 size eﬀect plot for Jackson’s data from ﬂexural tests of laminates of four diﬀerent layups, in dimensionless coordinates

(lower brittleness), might be expected to give a somewhat smaller scatter (larger m) than the unidirectional, cross-ply or quasi-isotropic laminate, but the opposite is systematically noted in pure Weibull ﬁtting of the data. Therefore, the classical hypothesis of a purely statistical size eﬀect in ﬂexural strength of laminates is untenable. On the other hand, as shown by Baˇzant, Zhou and Daniel (2003), the data of Jackson can be ﬁtted consistently by the energetic-statistical theory, with the same value of m for all the data; see Fig. A.4 in which the data for various layups are plotted in dimensionless coordinates, after optimal ﬁtting for each individual layup. However, it must further be noted that these data can be ﬁtted about equally well by a purely energetic theory. From this it follows that the Weibull-type statistical part of size eﬀect becomes signiﬁcant only for laminate thicknesses well beyond the normal usage (this observation is similar to that made for ﬂexural strength of concrete, for which the statistical part of size eﬀect becomes important only for concrete thickness found, for example, in arch dams).

254

Scaling of Structural Strength

A further implication is that fracture mechanics, rather than some strength criterion (or material failure criterion expressed in terms of stresses and strains), needs to be used for evaluating the strength of laminates. The fracture analysis of laminates must take into account the quasibrittle (or cohesive) nature of fracture.

A4. Size Eﬀect in Fracture of Closed-Cell Polymeric Foam Very light closed-cell polymeric (vinyl) foam is a favored material for the core of sandwich structures for ships. In classical works (e.g., Gibson and Ashby 1997, Shipsha et al. 2000, Gdoutos et al. 2001), the failure of this material in tension or compression has usually been described as ductile, involving a yield plateau followed by locking, and failure criteria expressed in terms of stresses have been used. Such failure can exhibit no size eﬀect. Such ductile response, however, does not take place when high tensile stress concentrations exist, induced for example by notches in laboratory specimens, or various structural holes or accidental damage of real structures. In such a case, the failure of the foam may be brittle. This was ﬁrst revealed by the notched specimen tests of Zenkert and B¨acklund (1989) in which the fracture toughness of foam was measured, by the tests of holed panels tests by Fleck and co-workers in Cambridge in (2001), and by the ﬁnite element studies of foam based on microplane model for foam by Brocca et al. (2001). Consequently, the foam, when notched or damaged, must be expected to exhibit size eﬀect, and this is what is conﬁrmed by a recent study (Baˇzant, Zhou, Nov´ ak and Daniel 2004), in which the size eﬀect in Divinycell H100 foam, both the case of failure with large cracks or notches (type 1) and failure at crack initiation (type 2). In this study, geometrically similar single edge-notched prismatic specimens of various sizes were tested under tension. The results were shown to agree with Baˇzant’s size eﬀect law. Fitting this law to the test results furnished the values of the fracture energy Gf of the foam as well as the characteristic size cf of the fracture process zone. Fracture analysis based on these properties was shown to match the test data of Fleck, Olurin and co-workers (2001) obtained on dissimilar panels with holes of diﬀerent sizes. These results were also matched using the eigenvalue method for ﬁnite element analysis based on the cohesive crack model with properties corresponding to the size eﬀect law. Finally, compressed foam specimens with V-shaped notches (with an angle wide enough to prevent the notch faces from coming into contact) were found to exhibit no size eﬀect. This implies that the cell collapse at the tip of the notch must be essentially a plastic process rather than a softening damage process.

Addendum

255

The results demonstrate that the current design practice, in which the tensile failure of foam is generally predicted on the basis of strength criteria or plasticity, is acceptable only for small structural parts. In the case of large structural parts, the size eﬀect must be taken into account, especially if the foam can suﬀer large fatigue cracks or large damage zones prior to critical loading to failure.

A5. Variation of Cohesive Softening Law Tail in Boundary Layer of Concrete It has been well established experimentally that the total fracture energy GF of a heterogeneous material such as concrete, deﬁned as the area under the cohesive softening curve, is not constant but varies during crack propagation across the ligament. The variation of GF at the beginning of fracture growth, which is described by the R-curve, is known to be only an apparent phenomenon which is perfectly consistent with the cohesive crack model (with a ﬁxed softening stress-separation law), and can in fact be calculated from it. However, the variation during crack propagation through the boundary layer at the end of the ligament is not consistent with the cohesive crack model and implies that the softening curve of this model is not an invariant property in the boundary layer. The analysis of this problem by Baˇzant and Yu (2004) will now be presented. The fact that the fracture energy representing the area under the softening curve should decrease to zero at the end of the ligament was pointed out in a paper by Baˇzant (1996), motivated by the experiments of Hu and Wittmann (1991 and 1992a), and was explained by a decrease of the fracture process zone (FPZ) size, as illustrated on the left of Fig. A.5a reproduced from Baˇzant’s (1996) paper. An experimental veriﬁcation and detailed justiﬁcation of this property was provided in the works of Hu (1997, 1998), Hu and Wittmann (1992b, 2000), Duan, Hu and Wittmann (2002, 2003), and Karihaloo, Abdalla, and Imjai (2003). As mentioned by Baˇzant (1996), as well as Hu and Wittmann, the consequence of these experimental observations is that: ∞ D 1 ¯ G(a) = P du = Γ(x) dx < GF (A5.1) D − a0 0 a0 ¯ where G(a) = average fracture energy in the ligament (Fig. A.5b), D = specimen size (Fig. A.5a), a0 = notch depth, P = load, u = load-point deﬂection, Γ(x) = local fracture energy ∞ as a function of coordinate x along the ligament (Fig. A.5a left), GF = 0 σ dw = Γ(x)-value at points x remote from the

256

Scaling of Structural Strength

Figure A.5: (a) Variation of local fracture energy Γ(x) across the ligament, decreasing in the boundary layer (reproduced from Baˇzant 1996). (b) Average fracture energy GF . (c) Required modiﬁcation of cohesive (or ﬁctitious) crack model boundary (= area under the complete σ(w)-diagram, Fig. A.5c), σ = cohesive (crack-bridging) stress, and w = crack opening = separation of crack faces. Is this behavior compatible with the cohesive crack model? To check it, consider a decreasing FPZ attached to the boundary at the end of ligament, Fig. A.5a. Extending to this situation Rice’s (1968) approach, we calculate the J-integral along a path touching the crack faces as shown in Fig. A.6a,b:

D ∂ui dv(x) ¯ J= U − ti σ (A5.2) ds (2) = 2 ds − [t2 ∆w]end dx dx xtip ∞ = σ(w)dw − [σ∆w]end = Area below σend (A5.3) 0

= Jend (D) or Jtail (x) or Jmiddle [(x + D)/2]

(A5.4)

in which s = integration contour length; x = x1 , y = x2 are the cartesian coordinates; ui = displacements; ti = tractions acting on the contour from the

Addendum

257

Figure A.6: (a,b) J-integral path. (c,d,e) Ambiguity in J-integral variation. (f,g,h,i) Fracture energies corresponding to J-integral. (j) Test data ﬁtted by modiﬁed cohesive crack model with variable tail

outside; U = strain energy density; v = w/2; x = D is the end point of the ligament; wend is the opening at the end of ligament (Fig. A.6b). From these equations, we see that the instantaneous ﬂux of energy, J, into the shrinking FPZ attached to the end of ligament (Fig. A.5a) represents the area below the line σ = σend in the softening diagram, cross-hatched in Fig. A.6i. It is, however, a matter of choice with which coordinate x in the FPZ this ﬂux J should be associated. If we associate J with the front, the tail, or the middle (Fig. A.6b) of the FPZ, we get widely diﬀerent plots of Γ = Jend , Jtail , Jmiddle , as shown in Fig. A.6(c,d,e), respectively (the ﬁrst one terminating with Dirac delta function). This ambiguity means that the boundary layer eﬀect, experimentally documented by Hu and Wittmann, cannot be represented by the standard cohesive crack model, with a ﬁxed stress-separation diagram. Can the cohesive crack model be adapted for this purpose? It follows from Eq. (A5.4) and Fig. A.6(h,i) (and has been computationally veriﬁed)

258

Scaling of Structural Strength

that Wittmann et al.’s (1990) and Elices et al.’s (1992) data can be matched (Fig. A.6j) if the slope of the tail segment of the bilinear stress-separation diagram for concrete is assumed to decrease (Fig. A.5c) in proportion to diminishing distance r = D − x (Fig. A.6b) from the end of ligament. After such an adaptation, the cohesive (or ﬁctitious) crack model has a general applicability, including the boundary layer. However, the consequence is that the total fracture energy GF (area under the complete stress-separation curve) is not constant. Noting that, the larger the structure, the smaller is the length fraction of the boundary layer, one must conclude that the diminishing tail slope in Fig. A.5c automatically implies a certain size eﬀect on the apparent GF , as given by Eq. (A5.4). It further follows from Fig. A.6(h,i), and has been computationally veriﬁed, that the initial tangent of the stress-separation diagram, the area under which represents the initial fracture energy Gf (Baˇzant 2002f, Baˇzant and BecqGiraudon 2002, Baˇzant, Yu and Zi 2002), can be considered as ﬁxed—in other words, Gf , unlike GF , is a material constant. Aside from the fact that the maximum loads of specimens and structures are generally controlled by Gf , not GF , this suggests that the standard fracture test that should be introduced is that which yields not GF but Gf (the size eﬀect method, as well as the method of Guinea, Planas and Elices, 1994a,b, and the zero brittleness method of Baˇzant, Yu and Zi 2002, serve this purpose, while the work-of-fracture method does not). This conclusion is not surprising in the light of the abundance of experimental data revealing that GF is statistically much more variable than Gf (Baˇzant and Becq-Giraudon 2002, Baˇzant, Yu and Zi 2002). Jir´ asek (2003) showed that Hu and Wittmann’s data can be matched by a nonlocal continuum damage model in which the characteristic softening curve is kept ﬁxed. Consequently the nonlocal model is a more general, and thus more fundamental, characterization of fracture than the cohesive (or ﬁctitious) crack model. This ﬁnding should be taken into account in fracture testing. It appears that GF would better be deﬁned by the area under the softening curve of the nonlocal model, multiplied by the characteristic length of material corresponding to the eﬀective width of FPZ, which equals the minimum possible spacing of parallel cracks (Baˇzant 1985, Baˇzant and Jir´ asek 2002), to be distinguished from Irwin’s characteristic length l0 = EGf /f t2 . A6. Can Fracture Energy Be Measured on One-Size Specimens with Diﬀerent Notch Lengths? The fact that specimens of diﬀerent sizes are needed for the size eﬀect method of measuring Gf is considered by some a disadvantage. For this

Addendum

259

reason, Baˇzant and Kazemi (1990), Baˇzant and Li (1996) and Tang et al. (1996) generalized the size eﬀect method to dissimilar specimens, the dissimilarity being caused by the use of diﬀerent notch lengths a0 in specimens of one size. If the random scatter of test data were small (coeﬃcient of variation CoV < 4%), this approach would work. However, for the typical scatter of maximum loads of concrete specimens (CoV = 8%), the range of brittleness numbers attainable by variation of notch length in a specimen of any geometry (about 1:3, Baˇzant and Li 1996) does not suﬃce to get a sharp trend in the regression of test data, and thus prevents determination of Gf accurately. Recently, this problem was considered independently by Duan and Hu (2003). They proposed the semi-empirical formula: σn = σ0 (1 + a/a∗∞ )−1/2

(A6.1)

where σ0 = ft for small 3PB specimens; a∗∞ is a certain constant; and σn represents the maximum tensile stress in the ligament based on a linear stress distribution over the ligament, σn = σN /A(a0 ). This alternative formula, intended for specimens of the same size when the notch length a0 is varied, in eﬀect attempts to replace the proﬁle of the universal size eﬀect law (Fig. A.2) at constant size D, scaled by the ratio σn /σN = 1/A(a0 ), where A(a0 ) depends on specimen geometry; A(a0 ) = (1 − a0 )2 for notched three-point bend beams. However, the curve of the proposed formula has, for a0 → 0, a size independent limit approached, in log a0 scale, with a horizontal asymptote, while the correct curve, amply justiﬁed by tests of modulus of rupture (or ﬂexural strength) of unnotched beams (Baˇzant and Li 1995, Baˇzant 1998, 2001, 2002f, Baˇzant and Nov´ ak 2000a,b,c), terminates with a steep slope for a0 → 0 and has a size dependent limit, as seen in the aforementioned proﬁles in Fig. A.2a,b, and better in Fig. A.2c. Fig. A.2d,e shows the proﬁles in D and in a, and it is seen that they cannot be matched well by Duan and Hu’s approximation converted from σn to σN . The test data on the dependence of σn on a0 , which Duan and Hu ﬁtted by their formula, should be ﬁtted, more accurately, with the usual size eﬀect law (Baˇzant and Kazemi 1990, Baˇzantand Planas 1998, and Baˇzant 1997, 2002f) σn = σN /A(a0 ) in which σN = E Gf [g (α0 )cf + g(α0 )D]−1/2 where D is constant and α0 = a0 /D is varied (and function g(α0 ) is available from handbooks). However, very short or zero notches (α0 < 0.15D) must be excluded, which means that the value of strength ft cannot be used with Duan and Hu’s approach. To use it, it is necessary to adopt either the approach of Guinea et al. (1994a,b) or the zero-brittleness method (Baˇzant, Yu and Zi 2002).

260

Scaling of Structural Strength

A7. Notched–Unnotched Size Eﬀect Method and Standardization of Fracture Testing Accurate simulations with the cohesive crack model (Guinea et al. 1997, Baˇzant and Yu 2002) revealed that, at maximum load, the cohesive stresses through the entire process zone in concrete fracture specimens (as well as normal-size structures) remain on the initial straight sloping segment of the stress-separation curve (Fig. 9.1, bottom left, Fig. A.7 top left). This means that (for type 2 fracture), the long tail of the stress-separation curve, and thus also the total fracture energy GF representing the area under the entire curve, do not matter. The maximum load depends only on the initial fracture energy Gf , representing the area under the initial tangent of this curve. Furthermore, statistical studies of published test data (Baˇzant and Becq-Giraudon 2002) as well as lattice particle simulations of microstructure (Cusatis et al. 2003a,b) revealed that the scatter of Gf has a much smaller coeﬃcient of variation than the scatter of GF (about one half). For these two reasons, it is preferable that a standard fracture test of concrete would yield directly Gf rather than GF . This means that the size eﬀect method is, in principle, preferable because it provides directly Gf , rather than GF . However, the need to use in this method specimens of very diﬀerent sizes may be seen as inconvenient. When GF is measured directly by the work-offracture method, one can roughly estimate Gf ≈ 0.4GF (Baˇzant 2002f, Baˇzant and Becq-Giraudon 2002). But this relation involves a large error. So, together with greater scatter of GF , this leads to a much greater uncertainty in Gf (and thus maximum load prediction), compared to direct measurement of Gf . Guinea et al. (1997) found that, if an accurate solution with the cohesive crack model is available for the given specimen geometry, then the initial slope of the stress-separation curve (and thus Gf ) can be easily obtained by measuring only the maximum loads of: (1) the maximum load of a small notched specimen (the smallest practical), and (2) an unnotched specimen. No testing method can be simpler and more robust. However, in view of large random scatter in fracture testing of concrete, statistical evaluation is important. In this regard, the simple method of Guinea et al. (1997) can still be improved—by recasting it in the form of zero-brittleness size eﬀect method (Baˇzant and Li 1996b), in a way that permits simultaneous statistical regression of the data for notched and unnotched tests. The key is to realize that the maximum load of unnotched specimens is independent of Gf , and thus depends only on material tensile strength ft . This is the property of the zero-size limit, σN = Bft , of the size eﬀect curve. So it suﬃces to relate B to the zero-size limit B0 ft of the exact size eﬀect curve of the cohesive crack

Addendum

261

model for the given geometry, which can be computed once for all for a chosen standardized specimen geometry (Baˇzant, Yu and Zi 2002). This exact size eﬀect curve is, for normal sizes, very close to the classical size eﬀect law σN = Bft (1 + D/D0 )−1/2 (Eq. 2.8) (and is identical to it for very large sizes). But for extrapolation to zero size, D → 0, a correction is needed. To this end, the size eﬀect curve of cohesive crack model for any ﬁxed specimen geometry may be written in a dimensionless form as (ft /σN )2 = g(α0 )ξ + B −2 − ∆(ξ),

with ξ = D/l1 , l1 = E Gf /ft

(A7.1)

where g(α0 ) = dimensionless energy release rate for the given geometry, and ∆(ξ) = deviation from the classical size eﬀect law in Eq. (2.8), which is calculated accurately from the cohesive crack model (and vanishes for large ξ); ∆(ξ) can be ignored in the usual size eﬀect method (section 2.5) (Baˇzant, Yu and Zi 2002) (l1 must not be confused with l0 = E GF /ft ). The statistical regression of test data may proceed as follows: m 1 1. Calculate the mean tensile strength f¯t = m i=1 ft i . Then, for each of the notched tests (j = 1, 2, . . . , n), calculate ηj = (f¯t /σN j )2 . After that, from the inverse relation of (A7.1) (determined explicitly once for all in advance), calculate ξj = ψ(ηj ) (the vertical line on the right of each plot on the top of Fig. A.7). Then calculate ∆j = ∆(ξj ) (j = 1, 2, . . . , n), and compute the notched specimen data for linear regression (Fig. A.7 right): (j = 1, 2, . . . , n) (A7.2) Yν+j = (ηj + ∆j )/(f¯t )2 (these are the points that would ideally lie on the straight size eﬀect asymptote, if there were no scatter). Set Yi = 1/(Bft i )2 (i = 1, 2, . . . , ν). 2. Consider the standard linear regression relation Y = AX + C of the size eﬀect method (Fig. A.7, top) where X = D, and set Xi = 0 for i = 1, 2, . . . , ν and Xi = D for i = ν + 1, ν + 2, . . . , ν + n. Then run linear regression of all data points (Xi , Yi ), i = 1, 2, . . . , ν + n, using the weights wi = 1/ν for i = 1, . . . , ν and wi = 1/n for i = ν + 1, ν + 2, . . . , N (N = ν + n). The well known regression formulas yield the mean slope A¯ ¯ and also the coeﬃcients of variation of regression and mean intercept C, N slope and intercept, ωA , ωC where ωA = [ i=1 (Yi − Yi )2 /(N − 2)]1/2 /Y¯ , N Y¯ = i=1 (Yi − Yi ) /N and Yi = AXi + C = values on the regression line. Finally, according to the formulas of the size eﬀect method (section 2.5), estimate the mean fracture energy and its coeﬃcient of variation: ¯ f ≈ g(α0 ) / E ¯ A, ¯ ωG ≈ ω 2 + αE ω 2 . G f A E

262

Scaling of Structural Strength

Figure A.7: Left bottom: Regression line based on classical size eﬀect law (Eq. 2.8, dashed line) and deviation ∆(ξ) from this line for small specimen sizes (solid line), computed from the cohesive crack model (the ﬁst vertical dash-dot line indicates the smallest possible specimen for which D ≈ 6 aggregate sizes, and the second one the smallest size for the deviation ∆(ξ) can be ignored). Left top: The smallest cohesive stress in the FPZ, calculated for a standard bilinear softening law with GF = 2.5Gf (‘knee’ = point of slope). Right: Regression of data for notched and unnotched specimens randomly generated according to Weibull distribution with modulus m = 24 (after Baˇzant, Yu and Zi 2002)

A minor weak point of the foregoing procedure is that the initial calculation of ξj is based on the mean of the ft rather than the random ft -data. This may be avoided by a certain kind of iteration (Baˇzant, Yu and Zi 2002).

A8. Designing Reinforced Concrete Beams against Size Eﬀect The time has become ripe for adding size eﬀect in a rational form to all the design speciﬁcations dealing with brittle failures of concrete structures

Addendum

263

Figure A.8: Improved design formula for shear failure of reinforced concrete beams without stirrups (the circle areas represents the weights, which are taken inversely proportional to the histogram of beam depths in the database) (shear and torsion of R.C. beams with or without stirrups, slab punching, column failure, bar embedment length, splices, bearing strength, plain concrete ﬂexure, compression failure of prestressed beams, etc.). In ACI Standard 318, so far, only the recently introduced formula for anchor pullout (which is of the LEFM type) includes size eﬀect. By analysis of the latest ACI 445 database with 398 data (Reineck et al. 2003), representing an update of 1984 and 1986 Northwestern University databases (with 296 data), an improved formula for shear failure of reinforced concrete beams without stirrups, having the simplicity desired by concrete designers, has recently been developed by second-order asymptotic matching (Baˇzant and Yu 2003); see the comparison with database in Fig. A.8, with CoV of the vertical deviations from data points (the solid line is the mean formula, the dashed line is a formula scaled down to achieve additional safety, as practiced in ACI; vc = σN = mean shear stress in the cross section at failure, d = beam depth from top face to the reinforcement centroid, fc = standard compression strength of concrete).

264

Scaling of Structural Strength

In the derivation of these formulas, the following three principles were adhered to: 1. Only theoretically justiﬁed formulas must be used in data ﬁtting because the size eﬀect (which is of main interest for beam depth d ranging from 1 m to 10 m) requires enormous extrapolation of the ACI 445 database (in which 86% of data pertain to d ≤ 0.6 m, 99% to d ≤ 1.1 m and 100% to d ≤ 1.89 m). 2. The validity of the formula must be assessed by comparing it only with (nearly) geometrically scaled beams of broad enough size range (only 11 such test series exist, among 398). 3. The entire database must be used only for the ﬁnal calibration of the chosen formula (but not for choosing the best formula, because data for many diﬀerent concretes and geometries are mixed in the database, and only 2% of the data have a non-negligible size range). A9. Scaling of Probability Density Distribution (pdf ) of Failure Load In practice, structures must typically be designed for failure probabilities pf of the order of 10−7 . Such a low probability cannot be determined experimentally, especially for large structures. It can be assessed only theoretically. One must deduce the size eﬀect on the pdf of σN by a rational argument. This can be done on the basis of the nonlocal Weibull theory expounded in section 3.2. For D → 0, failure is non-propagating and must occur nearly simultaneously along the entire failure surface. So the pdf of σN must be Gaussian (except in far-oﬀ tails), as deduced from Daniels’ (1945) ﬁber bundle model. With increasing D, the asymptotic size eﬀect on the mean strength is nil and the coeﬃcient of variation (CoV) asymptotically decreases as D−1/2 . For D → ∞, the pdf must be Weibull, corresponding to the weakest-link chain model, which implies a size-independent CoV. The gradual transition of pdf from Gaussian to Weibull, exempliﬁed by various load-sharing models (Phoenix and Beyerlein 2000, Mahesh et al. 2002), can be obtained by asymptotic matching (Baˇzant 2004a, 2004b) and calibrated by a chain-of-bundles model (Fig. A.1f middle) (Baˇzant and Pang 2004). A10. Recent Debates on Fractal Theory of Size Eﬀect and Their Impact on Design Codes An engineering ﬁeld such as aeronautical can exist without simple design codes because only a few large aircraft are designed annually. But structural

Addendum

265

engineering, in which many thousands of structures are designed annually, each of them diﬀerent, cannot get by without codes. During the last few years, the need to introduce the size eﬀect into the design code speciﬁcations guarding against brittle failures of concrete structures has ﬁnally been widely recognized on all continents. Members of the code-making committees of course notice that there are currently promulgated two radically diﬀerent theories of size eﬀect in concrete structures—the energetic-statistical theory expounded here and a purely fractal theory. Therefore, unless the conﬂict between the proponents of these two theories is resolved, these committees would opt for a purely empirical approach. Yet, an empirical approach is doomed to yield an incorrect formula because a statistically signiﬁcant set of test results on a suﬃciently large number of identical large structures can hardly ever be acquired, because of prohibitive cost. The largest concrete structures, sea ice bodies or rock formations are way beyond the range of failure testing, and small-size data vastly dominate, because of cost. For instance, 86% of the data for shear failure of beams pertain to beam depths less than 0.6 m, and 99% less than 1.1 m, while the main interest is in beam depths from 1 m to 10 m. Consequently, the design of large structures must rely on extrapolation from the range of testing. A theoretical basis for such an extrapolation is, therefore, imperative. But progress on the design code appears impossible unless the fractal-nonfractal conﬂict is resolved. Motivated by the need to resolve the conﬂict, an extensive critical study has recently been undertaken (Baˇzant and Yavari 2004). It greatly expands the analysis of fractal approach in sections 3.5 and 3.6, and focuses on the recent arguments.

A11. Boundary Layer Size Eﬀect in Thin Metallic Films at Micrometer Scale Recent pure tension tests of free polycrystal thin metallic ﬁlms of Au, Al and Cu, conducted by H. Espinosa at Northwestern University revealed a surprising and very strong size eﬀect. The strength of these ﬁlms increases by a factor of 3 to 5 when the thickness is reduced from 5 µm to 0.5 µm, while for smaller thickness the size eﬀect in pure tension apparently disappears. This size eﬀect can be explained by the existence of a boundary layer of a ﬁxed thickness, located at the face of ﬁlm that was during deposition in contact with the substrate. The boundary layer, having a thickness of the order of the crystal grain size of metal, has a signiﬁcantly higher yield strength than the rest of ﬁlm. The layer forms during ﬁlm deposition on the face of the substrate and is inﬂuenced by the epitaxial eﬀects of crystal growth on the dislocation density and texture.

266

Scaling of Structural Strength

The increase of yield strength of the epitaxial boundary layer is considered to be caused partly by a diﬀerence in the mean density of statistically stored dislocations due to blockage of dislocation movements at grain boundaries and formation of dislocation pile-ups near grain boundaries, compared to the rest of ﬁlm, and partly also by prevalent crystal orientation unfavorable to dislocation glide, which are engendered in the granular epitaxial boundary layer by the substrate during ﬁlm deposition. Assuming a simple error function decay of the yield strength across the ﬁlm thickness from the substrate side leads to a good agreement with pure tension tests, and well as other kinds of experimental observations. The characteristic length l0 governing the boundary layer size eﬀect is the natural grain size of the metal, l0 ≈ 0.5 µm. Therefore the boundary layer size eﬀect is expected to vanish for ﬁlm thickness D < l0 and D > 10l0 , and this is what is observed in tests. The boundary layer size eﬀect does not conﬂict with Hutchinson and Fleck’s strain gradient size eﬀect. That size eﬀect, which has been used to explain micro-indentation tests down to 1 µm, dominates for the range 5–100 µm. In the range from 1 to 5 µm, in which both kinds of size eﬀect overlap, the ﬁt of the micro-indentation and micro-bending test data by the strain gradient theory is not very close. The epitaxial boundary layer model captures the extra plastic hardening due to statistically stored dislocations, whereas the strain gradient theory explained in section 10.1 captures the eﬀect of geometrically necessary dislocations. A combined theory is found to be necessary in order to ﬁt with the same theory the ﬁlm test data on both pure tension and bending. Thin metallic ﬁlms of thickness less than 5 µm are found to fail in a quasibrittle manner, exhibiting gradual postpeak softening, which can also be explained and ﬁtted by the epitaxial boundary layer model if the damage due to void or microcrack growth is taken into account. The classical Hall-Petch relation for the dependence of yield strength on the natural grain size, as well as Nix’s model for the strength of ﬁlms thinner than the grain size, needs to be included in the formulation to obtain a general model with proper asymptotics, the former for very thick ﬁlms (D > 100 µm) and the latter for extremely thin ﬁlms (D < 0.3 µm). Inclusion of the Hall-Petch formula is important when not only the ﬁlm thickness but also the grain size is varied. To this end, the HallPetch formula is enhanced by a smooth approach to a cutoﬀ yield strength for very small grain size. In the case of ﬁlms thinner than than the natural grain size, in which the crystal grains are ﬂattened to ﬁt the ﬁlm thickness, the grain size to be substituted into the Hall-Petch formula is the ﬁlm thickness, which means that the Hall-Petch eﬀect disappears for very thin ﬁlms (being replaced by Nix’s eﬀect).

Addendum

267

A12. Size Eﬀect on Triggering of Dry Snow Slab Avalanches A size eﬀect model analogous to that expounded in this book has recently been formulated for dry snow slab avalanches in a study by Baˇzant, Zi and McClung (2003). The ratio of the thickness of snow layer to the length is, in that study, assumed to be small enough for one-dimensional analysis to be applicable. Equivalent LEFM is used to obtain the law of the decrease of the nominal shear strength of the snow layer with an increasing thickness of snow. This law is shown to closely agree with two-dimensional numerical solutions according to the cohesive crack model for mode II fracture with ﬁnite residual shear stress. By ﬁtting these solutions for various snow thicknesses D with the structural size eﬀect law, an approximate one-to-one relationship between the material parameters in the size eﬀect law and the cohesive crack model is established. The failure mode and size eﬀect are found to depend on the pre-existing (initial) shear stress τi in a fracture-triggering weak layer that normally exists at the base of snow slab. There exists a critical stress τi = τcr and a critical snow depth Dcr such that, for D > Dcr or τi < τcr , there is no structural size eﬀect, no peak load, and no postpeak softening. The value of τcr is approximately 85% of the residual shear stress at the base of a sliding layer. Because the fracture process zone can be many meters long, it is not easy to perform laboratory experiments simulating avalanches. Direct measurement of the size eﬀect per se is next to impossible because the eﬀects of snow weight and snow aging prevent ﬁnding diﬀerent-sized samples with similar mechanical properties. The size eﬀect law needs to take into account the dependence of snow properties in the weak layer at base on the snow slab thickness. This is achieved by replacing the constant fracture toughness and the limiting zero-size strength with quantities that increase with snow slab thickness. Fitting of the data from over a hundred ﬁeld observations of avalanches suggests that this increase is very strong, with the toughness increasing roughly as (snow thickness)1.8 .

Bibliography

305

Relevant Author’s Works after the First Printing (up to 2004) Baˇzant, ZP (2001a), “Probabilistic modeling of quasibrittle fracture and size eﬀect” (principal plenary lecture), (Proc., 8th Int. Conf. on Structural Safety and Reliability (ICOSSAR), held at Newport Beach, Cal., 2001), RB Corotis, GI Schueller and M Shinozuka, eds., Swets & Zeitinger (Balkema), 1–23. Baˇzant, ZP (2001b), “Scaling of failure of beams, frames and plates with softening hinges.” Meccanica (Kluwer Acad. Publ.) 36, 67–77, 2001 (special issue honoring G Maier). Baˇzant, ZP (2001c), “Size eﬀects in quasibrittle fracture: Apercu of recent results.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-4 Int. Conf., Paris), R de Borst, J Mazars, G Pijaudier-Cabot and JGM van Mier, eds., Swets & Zeitlinger (A.A. Balkema Publishers), Lisse, 651–658. Baˇzant, ZP (2001d), “Scaling laws for sea ice fracture.” Proc., IUTAM Symp. on Scaling Laws in Ice Mechanics and Ice Dynamics (held in Fairbanks, June 2000), ed. by JP Dempsey and HH Shen, Kluwer Academic Publ., Dordrecht, 195–206. ˇ Baˇzant, ZP, Caner, FC, and Cervenka, J (2001), “Vertex eﬀect and conﬁnement of fracturing concrete via microplane model M4.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-4 Int. Conf., Paris), R de Borst, J Mazars, G Pijaudier-Cabot and JGM van Mier, eds., Swets & Zeitlinger (A.A. Balkema Publishers), Lisse, 497–504. ˇ Baˇzant, ZP, Cervenka, J, and Wierer, M (2001), “Equivalent localization element for crack band model and as alternative to elements with embedded discontinuities.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-4 Int. Conf., Paris), R de Borst, J Mazars, G Pijaudier-Cabot and JGM van Mier, eds., Swets & Zeitlinger (A.A. Balkema Publishers), Lisse, 765–772. Baˇzant, ZP and Nov´ ak, D (2001a), “Proposal for standard test of modulus of rupture of concrete with its size dependence.” ACI Materials Journal 98 (1), 79–87. Baˇzant, ZP and Nov´ ak, D (2001b), “Nonlocal Weibull theory and size eﬀect in failures at fracture initiation.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-4 Int. Conf., Paris), R de Borst, J Mazars, G PijaudierCabot and JGM van Mier, eds., Swets & Zeitlinger (A.A. Balkema Publishers), Lisse, 659–664.

306

Scaling of Structural Strength

Baˇzant, ZP and Nov´ ak, D (2001c), “Nonlocal model for size eﬀect in quasibrittle failure based on extreme value statistics.” (Proc., 8th Int. Conf. on Structural Safety and Reliability (ICOSSAR), Newport Beach, Cal., 2001), RB Corotis, ed., Swets & Zeitinger (Balkema), 1–8. Brocca, M and Baˇzant, ZP (2001), “Size eﬀect in concrete columns: Finite element analysis with microplane model.” J. of Structural Engineering ASCE 127 (12), 1382–1390. Carol, I, Jir´ asek, M, and Baˇzant, ZP (2001), “A thermodynamically consistent approach to microplane theory. Part I: Free energy and consistent microplane stresses.” Int. J. of Solids and Structures 38 (17), 2921–2931. Planas, J, Baˇzant, ZP, and Jir´ asek, M (2001), “Reinterpretation of Karihaloo’s size eﬀect analysis for notched quasibrittle structures.” Intern. J. of Fracture 111, 17–28. Baˇzant, ZP, Zhou, Y, Nov´ ak, D, and Daniel, IM (2001), “Size eﬀect in fracture of sandwich structure components: foam and laminate.” Proc., ASME Intern. Mechanical Engrg. Congress (held in New York), Vol. AMD-TOC (paper 25413), Am. Soc. of Mech. Engrs., New York, pp. 1–12. Baˇzant, ZP (2002a), “Reminiscences on four decades of struggle and progress in softening damage and size eﬀect”. Concrete Journal (Tokyo) 40 (2), 16–28 (JCI Anniversary); Expanded version republished in Mechanics (Am. Academy of Mech.) 32 (5–6), 2003, 1–10. Baˇzant, ZP (2002b), “Size eﬀect theory and its application to fracture of ﬁber composites and sandwich plates.” Continuum Damage Mechanics of Materials and Structures, O Allix and F Hild, eds., Elsevier, Amsterdam, pp. 353–381. Baˇzant, ZP (2002c), “Size eﬀect theory and its application to fracture of ﬁber composites and sandwich plates.” Continuum Damage Mechanics of Materials and Structures, O Allix and F Hild, eds., Elsevier, Amsterdam, pp. 353–381. Baˇzant, ZP (2002d), “Scaling of sea ice fracture—Part I: Vertical penetration.” J. of Applied Mechanics ASME 69 (Jan.), 11–18. Baˇzant, ZP (2002e), “Scaling of sea ice fracture—Part II: Horizontal load from moving ice.” J. of Applied Mechanics ASME 69 (Jan.), 19–24. Baˇzant, ZP (2002f), “Concrete fracture models: testing and practice.” Engineering Fracture Mechanics 69 (2), 165–206 (special issue on Fracture of Concrete and Rock, M Elices, ed.).

Bibliography

307

Baˇzant, ZP (2002g), “Scaling of dislocation-based strain-gradient plasticity.” J. of the Mechanics and Physics of Solids 50 (3), 435–443 (based on Theor. & Appl. Mech. Report No. 2000-12/C699s, Northwestern University 2000; see also Errata, Vol. 52, 2004, p. 975). Baˇzant, ZP and Becq-Giraudon, E (2002), “Statistical prediction of fracture parameters of concrete and implications for choice of testing standard.” Cement and Concrete Research 32 (4), 529–556. Baˇzant, ZP and Frangopol, DM (2002), “Size eﬀect hidden in excessive dead load factor.” J. of Structural Engrg. ASCE 128 (1), 80–86. Baˇzant, ZP and Guo, Z (2002a), “Size eﬀect and asymptotic matching approximations in strain-gradient theories of micro-scale plasticity.” Int. J. of Solids and Structures 39, 5633–5657; see also Errata, Vol. 40 (2003), p. 6215). Baˇzant, ZP and Guo, Z (2002b), “Size eﬀect on strength of ﬂoating sea ice under vertical line load.” J. of Engrg. Mechanics 128 (3), 254–263. Baˇzant, ZP and Jir´ asek, M (2002), “Nonlocal integral formulations of plasticity and damage: Survey of progress.” ASCE J. of Engrg. Mechanics 128 (11), 1119–1149 (ASCE 150th anniversary article). Baˇzant, ZP, Yu, Q, and Zi, G (2002), “Choice of standard fracture test for concrete and its statistical evaluation.” Int. J. of Fracture 118 (4), Dec., 303–337. Caner, FC and Baˇzant, ZP (2002), “Lateral conﬁnement needed to suppress softening of concrete in compression.” J. of Engrg. Mechanics ASCE 128 (12), 1304–1313. Jir´ asek, M and Baˇzant, ZP (2002), Inelastic Analysis of Structures. J. Wiley & Sons, London and New York (735 + xviii pp.). Lin, F-B, Yan, GY, Baˇzant, ZP, and Ding, F (2002), “Nonlocal strain-softening model of quasibrittle materials using boundary element method.” Engrg. Analysis with Boundary Elements 26, 417–424. Baˇzant, ZP (2003a), “Asymptotic matching analysis of scaling of structural failure due to softening hinges. I. Theory.” J. of Engrg. Mech. ASCE 129 (6), 641–650. Baˇzant, ZP (2003b), “Asymptotic matching analysis of scaling of structural failure due to softening hinges. II. Implications.” J. of Engrg. Mech. ASCE 129 (6), 651–654. Baˇzant, ZP and Nov´ ak, D (2003), “Stochastic models for deformation and failure of quasibrittle structures: recent advances and new directions.”

308

Scaling of Structural Strength

Computational Modelling of Concrete Structures (Proc., EURO-C Conf., St. Johann im Pongau, Austria), N Bi´cani´c, R de Borst, H Mang and G Meschke, eds., A.A. Balkema Publ., Lisse, Netherlands, 583–598. Baˇzant, ZP, Zhou, Y, Zi, G, and Daniel, IM (2003), “Size eﬀect and asymptotic matching analysis of fracture of closed-cell polymeric foam.” Int. J. of Solids and Structures 40, 7197–7217. Baˇzant, ZP and Zi, G (2003), “Asymptotic stress intensity factor proﬁles for smeared-tip method for cohesive fracture.” Int. J. of Fracture 119 (2), 145–159. Baˇzant, ZP, Zi, G and McClung, D (2003), “Size eﬀect law and fracture mechanics of the triggering of dry snow slab avalanches.” J. of Geophysical Research 108 (B2), 2119–2129. Cusatis, G, Baˇzant, ZP, and Cedolin, L (2003a), “Conﬁnement-shear lattice model for concrete damage in tension and compression: I. Theory.” J. of Engrg. Mechanics ASCE 129 (12), 1439–1448. Cusatis, G, Baˇzant, ZP, and Cedolin, L (2003b), “Conﬁnement-shear lattice model for concrete damage in tension and compression: I. Computation and validation.” J. of Engrg. Mechanics ASCE 129 (12), 1449–1458. Nov´ ak, D, Baˇzant, ZP, Voˇrechovsk´ y, M (2003), “Computational modeling of statistical size eﬀect in quasibrittle structures.” Applications of Statistics and Probabiltity in Civil Engineering (Proc., 9th Int. Conf., ICASP-9, held in San Francisco), A Der Kiureghian, S Madanat and JM Pestana, eds., Millpress, Rotterdam, 621–628. Sl´ adek, J, Sl´ adek, V, and Baˇzant, ZP (2003), “Non-local boundary integral formulation for softening damage.” Int. J. for Numerical Methods in Engrg. 57, 103–116. Zi, G and Baˇzant, ZP (2003), “Eigenvalue method for computing size eﬀect of cohesive cracks with residual stress, with application to kink bands in composites.” Int. J. of Engrg. Science 41 (13–14), 1519–1534 (special issue honoring K Willam, ed. by ZP Baˇzant, I Carol and P Steinmann). Baˇzant, ZP, Caner, FC, Cedolin, L, Cusatis, G, and Di Luzio, G (2004), “Fracturing material models based on micromechanical concepts: Recent advances.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-5, 5th Int. Conf. on Fracture Mech. of Concrete and Concr. Structures, Vail, Colo.), Vol. 1, VC Li, KY Leung, Willam, KJ, and Billington, SL, eds., IA-FraMCoS, 83–90. Baˇzant, ZP, Pang, SD, Voˇrechovsk´ y, M, Nov´ ak, D and Pukl, R (2004), “Statistical size eﬀect in quasibrittle materials: Computation and extreme value

Bibliography

309

theory.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-5, 5th Int. Conf. on Fracture Mech. of Concrete and Concr. Structures, Vail, Colo.), Vol. 1, VC Li, KY Leung, Willam, KJ, and Billington, SL, eds., IA-FraMCoS, 189–196. Baˇzant, ZP and Yu, Q (2004), “Size eﬀect in concrete specimens and structures: New problems and progress.” Fracture Mechanics of Concrete Structures (Proc., FraMCoS-5, 5th Int. Conf. on Fracture Mech. of Concrete and Concr. Structures, Vail, Colo.), Vol. 1, VC Li, KY Leung, Willam, KJ, and Billington, SL, eds., IA-FraMCoS, 153–162. Baˇzant, ZP, Zhou, Y, Nov´ ak, D, and Daniel, IM (2004), “Size eﬀect on ﬂexural strength of ﬁber-composite laminate.” J. of Engrg. Materials and Technology ASME 126 (Jan.), 29–37. Baˇzant, ZP (2004a), “Scaling theory for quasibrittle structural failure.” Proc., National Academy of Sciences 101, in press. Baˇzant, ZP (2004b), “Probability distribution of energetic-statistical size eﬀect in quasibrittle fracture.” Probabilistic Engineering Mechanics, in press. Baˇzant, ZP and Caner, FC (2004), “Microplane model M5 with kinematic and static constraints for concrete fracture and anelasticity.” J. of Engrg. Mech. ASCE, in press. Baˇzant, ZP, Guo, Z, Espinosa, H, Zhu, Y and Peng, B (2004), “Epitaxially Inﬂuenced Boundary Layer Model for Size Eﬀect in Thin Metallic Films.” Theor. & Appl. Mech. Report, Northwestern University; J. of Appl. Physics, submitted to. Baˇzant, ZP and Yu, Q (2004), “Designing against size eﬀect on shear strength of reinforced concrete beams without stirrups.” J. of Structural Engineering ASME, in press. Baˇzant, ZP and Yavari, A (2004), “Is the cause of size eﬀect on structural strength fractal or energetic-statistical?” Engrg. Fracture Mechanics 43, in press.

Additional References for Addendum (up to 2004) Acharya, A and Bassani, JL (2000), “Lattice incompatibility and a gradient of crystal plasticity.” J. of the Mechanics and Physics of Solids 48, 1565–1595. Carpinteri, A (1987), “Stress-singularity and generalized fracture toughness at the vertex of re-entrant corners.” Engineering Fracture Mechanics 26, 143–155.

310

Scaling of Structural Strength

Daniels, HE (1945), “The statistical theory of the strength of bundles & threads.” Proc. Royal Soc. A183, London, 405–435. Duan, K and Hu, XZ (2003), “Scaling of quasi-brittle fracture: Boundary eﬀect.”, submitted to Engineering Fracture Mechanics. Duan, K, Hu, XZ, and Wittmann, FH (2002), “Explanation of size eﬀect in concrete fracture using non-uniform energy distribution.” Materials and Structures 35, 326–331. Duan, K, Hu, XZ, and Wittmann, FH (2003), “Boundary eﬀect on concrete fracture and non-constant fracture energy distribution.” Engrg. Fracture Mechanics 70, 2257–2268. Dunn, ML, Suwito, W, and Cunningham, SJ (1997), “Stress Intensities at notch singularities.” Engineering Fracture Mechanics 57(4), 417–430. Dunn, ML, Suwito, W, and Cunningham, SJ (1997), “Fracture initiation at sharp notches: correlation using critical stress intensities.” Int. J. Solids Structures 34(29), 3873–3883. Elices, M, Guinea, GV, and Planas, J (1992), “Measurement of the fracture energy using three-point bend tests: Part 3-inﬂuence of cutting the P-d tail.” Materials and Structures 25, 327–334. Fleck, NA and Hutchinson, JW (1993), “A phenomenological theory for strain gradient eﬀects in plasticity.” J. of the Mechanics and Physics of Solids 41, 1825–1857. Fleck, NA and Hutchinson, JW (1997), “Strain gradient plasticity.” Advances in Applied Mechanics, vol. 33, JW Hutchinson and TY Wu, eds., Academic Press, New York, 295–361. Fleck, NA, Olurin, OB, Chen, C, and Ashby, MF (2001), The Eﬀect of Hole Size upon the Strength of Metallic and Polymeric Foams. Journal of the Mechanics and Physics of Solids 49, 2015–2030. Gibson, LJ and Ashby, MF (1997), Cellular Solids: Structure and Properties, 2nd ed. Cambridge University Press, Cambridge, UK. Guinea, GV, Planas, J, and Elices, M (1994a), “Correlation between the softening and the size eﬀect curves.” Size Eﬀect in Concrete (edited by Mihashi, H, Okamura, H, and Baˇzant, ZP), E&FN Spon, London, 233–244. Guinea, GV, Planas, J, and Elices, M (1994b), “A general bilinear ﬁtting for the softening curve of concrete.” Materials and Structures 27, 99–105. Guinea, GV, Elices, M, and Planas, J (1997), “On the initial shape of the softening function of cohesive materials.” Int. J. of Fracture 87, 139–149.

Bibliography

311

Hu, XZ (1997), “Toughness measurements from crack close to free edge. “International Journal of Fracture 86(4), L63–L68. Hu, XZ (1998), “Size eﬀects in toughness induced by crack close to free edge.” Fracture Mechanics of Concrete Structures (ed. by Mihashi, H, and Rohugo, K), Proc. FraMCoS-3, Japan, 2011–2020. Hu, XZ and Wittmann, FH (1991), “An analytical method to determine the bridging stress transferred within the fracture process zone: I. General theory.” Cement and Concrete Research 21, 1118–1128. Hu, XZ and Wittmann, FH (1992a), “An analytical method to determine the bridging stress transferred within the fracture process zone: II. Application to mortar.” Cement and Concrete Research 22, 559–570. Hu, XZ and Wittmann, FH (1992b), “Fracture energy and fracture process zone.” Materials and Structures 25, 319–326. Hu, XZ and Wittmann FH (2000), “Size eﬀect on toughness induced by crack close to free surface.” Engineering Fracture Mechanics 65, 209–221. Jackson, KE (1992), “Scaling Eﬀects in the Flexural Response and Failure of Composite Beams,” AIAA Journal, Vol. 30(8), pp, 2099–2105. Johnson, DP, Morton, J, Kellas, S, and Jackson, KE (2000), “Size Eﬀect in Scaled Fiber Composites Under Four-Point Flexural Loading,” AIAA Journal, Vol. 38(6), 1047–1054. Jir´ asek, M (2003), Keynote lecture presented at EURO-C, St. Johann in Pongau, Austria. Karihaloo, BL (1999), “Size eﬀect in shallow and deep notched quasi-brittle structures.” International Journal of Fracture 95, 379–390. Karihaloo, BL, Abdalla, HM, and Imjai, T (2003), “A simple method for determining the true speciﬁc fracture energy of concrete.” Magazine of Concrete Research 55(5), 471–481. Karihaloo, BL, Abdalla, HM, and Xiao, QZ (2003), “Size eﬀect in concrete beams.” Engineering Fracture Mechanics 70, 979–993. Lavoie, JA, Soutis C, and Morton, J (2000), “Apparent Strength Scaling in Continuous Fiber Composite Laminates.” Composite Science and Technology, Vol. 60, pp. 283–299. Mahesh, S, Phoenix, SL and Beyerlein, IJ (2002), “Strength distributions and size eﬀects for 2D and 3D composites with Weibull ﬁbers in an elastic matrix.” Int. J. of Fracture 115, 41–85.

312

Scaling of Structural Strength

Mindlin, RD (1965), “Second gradient of strain and surface tension in linear elasticity.” Int. J. Solids Struct. 1, 417–438. Phoenix, SL and Beyerlein, IJ (2000), “Distribution & size scalings for strength in a one-dimensional random lattice with load redistribution to nearest & next nearest neighbors.” Phys. Review E 62, 1622–1645. Reineck, K, Kuchma, DA, Kim, KS, and Marx, S (2003), “Shear database for reinforced concrete members without shear reinforcement.” ACI Structural Journal 100, No. 2, 240-249; with discussions by Baˇzant and Yu, Vol. 101, No. 1 (Jan.-Feb. 2004). Rice, RJ (1968), “Mathematical analysis in the mechanics of fracture.” Fracture-An Advanced Treatise, Vol. 2 (ed. by Liebowitz, H), Academic Press, New York, 191–308. RILEM Committee QFS (ZP Baˇzant, chairman) (2004), “Quasibrittle fracture scaling and size eﬀect.” Materials and Structures (Paris) 37, in press. Tang, T, Baˇzant, ZP, Yang, S, and Zollinger, D (1996), “Variable-notch one-size test method for fracture energy and process zone length.” Engrg. Fracture Mechanics 55(3), 383–404. Toupin, RA (1962), “Elastic materials with couple stresses.” Arch. Ration. Mech. Anal. 11, 385-414. Williams, ML (1952), “Stress singularities resulting from various boundary conditions in angular corners of plates in extension.” Journal of Applied Mechanics 74, 526–528. Wisnom, MR (1991), “The Eﬀect of Specimen Size on the Bending Strength of Unidirectional Carbon Fiber-Epoxy,” Composite Structures, Vol. 18, pp. 47–63. Wisnom, MR and Atkinson, JA (1997), “Reduction in Tensile and Flexural Strength of Unidirectional Glass Fiber-Epoxy with Increasing Specimen Size,” Composite Structures, Vol. 38, pp. 405–412. Wittmann, FH, Mihashi, H, and Nomura, N (1990), “Size eﬀect on fracture energy of concrete.” Engrg. Fracture Mech. 35, 107–115 Zenkert, D and B¨ acklund J (1989), PVC Sandwich Core Materials: Mode I Fracture Toughness. Composite Science and Technology 34, 225–242. Zenkert, D (1989), PVC Sandwich Core Materials: Fracture Behaviour under Mode II and Mixed Mode Loading. Materials Science and Engineering 108, 233–240.

Subject Index activation energy, 151, 152 asymptotic analysis, 21–49 power scaling law large sizes, 14 small sizes, 14 small sizes, 16 smeared-tip method, 177–217 transitional size, 17 boundary layer concrete, cohesive softening law tail, 255 eﬀect, 10 of cracking, 42, 43, 45 Prandtl’s theory, 1, 25, 193 stress redistribution, 38, 43, 44 boundary value problem, xi, 18, 78, 181 bridging stress and crack opening, 165, 180 and stress intensity factor, 205 deformations in the FPZ, 181 distribution, 166, 180 in kink band, 137, 145 residual, 133 brittleness concept, 26 inﬂuence of loading rate, 153, 154 of ﬂoating sea ice, 35 brittleness number analysis of size eﬀect tests, 29, 30, 47 Baˇzant’s, 25, 26, 47

characteristic length absence, 11, 18 characteristic material length absence, 7, 11–13, 17, 20, 56 and fracture process zone, 21, 22, 156 discrete elements, 174 eﬀect of viscosity, 156 ﬁnite elements, 172 ﬂoating sea ice, 78, 84 in nominal strength, 23 in stress distribution, 28 inelastic hinges, 90 Irwin’s, 93, 188 localization limiter, 174 microplane model, 167, 172 small structure sizes, 14 characteristic structure size, 11, 56, 89, 94, 99, 111, 135, 137, 182 characteristic time, 156 closed cell polymeric foam fracture, 254 CMOD, see crack mouth opening displacement cohesive crack model, 167, 177, 178 and Rice’s J-integral, 187 asymptotic analysis, 24, 26 basic hypothesis, 177 broad size range, 210 conversion to an eigenvalue problem, 165 crack opening, 165 energetic aspect, 178

314

Scaling of Structural Strength

ﬁtting formula, 193 for ﬁber composites, 148 fracture energy, 32, 180, 210, 211 in historical context, 7 kink band failure, 147 limitations, 179, 181, 193 nonstandard, 185, 187, 215, 216 plastic analysis, 202 small size asymptotics, 204 softening curve, 145 standard, 181, 182, 198, 199, 203, 204, 215 standard and nonstandard equivalence, 185 stress proﬁle resolution, 165 stress-displacement curve, 185 stress-displacement law, 179, 180 time dependent formulation, 152, 153 compliance calculation from KI expressions, 88 Green’s functions, 179, 204 method, for equivalent crack length, 21, 40 compression failure basic mechanisms, 121 buckling phenomena, 122 by splitting crack band, 91, 122, 124, 133 crushing phenomena, 92, 101, 116, 130, 131 hinge softening, 90 internal buckling phenomena, 122 of concrete beams, 90, 130, 131 of ice plate, 87 size eﬀect on nominal strength, 124

concrete structures design codes, 110–117 no-tension design, 117–119 plain, see unreinforced concrete reinforced, see reinforced concrete crack band model basic idea, 170, 178 comparison with cohesive crack model, 177, 178 comparison with test data, 45 in historical context, 7–9 mesh dependence, 125, 172 crack growth fatigue, see fatigue crack growth stable, 38, 47, 53, 55, 57, 59, 70, 71, 111 crack inﬂuence function, 171 crack initiation failures, 245 crack mouth opening displacement, 153 crack opening proﬁle and stress intensity factor, 184 calculation form KI expressions, 87 calculation from KI expressions, 182, 183 creep, 10, 153 viscoelasticity, 153, 156, 209 critical crack tip opening displacement, 32, 199 critical stress intensity factor, see fracture toughness CS theory, 237 cycling loading, see fatigue crack growth design codes, fractal theory, 264 dimensionless variables, 230 discrete element method, 37, 170, 174–176 dry snow slab avalanches, triggering, 267

Subject Index

eigenvalue analysis, 165, 166 energy balance, 16, 122, 124 energy release analysis of steel-concrete composite beams, 102, 104, 106, 107 complementary potential energy, 106 complementary shear strain energy, 106 slip of studs, 107, 109 and deterministic size eﬀect, 2, 15, 55 asymptotic analysis, 21, 29, 58 axial splitting cracks, 122–124, 131 complementary energy analysis, 22, 23 crack band, 124 for large structure sizes, 15 for small structure sizes, 16 in approximate analysis, 7 in breakout of boreholes in rock, 132 in continuum damage model, 170, 172, 173 in kink bands, 138, 140 142 inelastic hinge, 90–92, 95 potential energy analysis, 22 strain energy density, 29 stress redistributions, 55, 57 energy release function, 27, 40, 135, 179, 182, 196, 198, 206 energy release rate, 17, 22, 23 and material orthotropy, 135 at zero crack length, 40 critical, 19 dimensionless expression, 23, 24 for a system of loads, 48 for ﬂoating ice plates vertical penetration, 82, 84 in nonlocal LEFM, 206

315

equivalent LEFM analysis, 21, 27, 29, 40, 69, 86, 107, 133, 145, 148, 199, 203, 206, 216 Espinosa, H, 265 failure load (pdf), 264 fatigue crack growth, 7, 38, 154, 189 ﬁbre-composite laminates, ﬂexural strength, 252 ﬁnite angle notches, size eﬀect, 249 Fleck and Hutchinson’s formulation, 228 ﬂoating sea ice force applied to ﬁxed structures, 87–89 line load, 99–101 thermal bending fracture, 77–78 vertical penetration, 78–86 FPZ, see fracture process zone fractal curve, 69, 70, 72 dimension, 71–74 fracture energy, 71 lacunar, 72–76 fractal and multifractal scaling law, 42, 49, 73, 75, 111, 134 fracture energy, 29, 32, 76, 84, 138, 211 according to fractal theories, 70–72 and broad-range size eﬀect law, 210, 217 and characteristic material length, 22 deﬁnition, 15 for a splitting crack band, 91, 124, 131 for concrete, 32, 211 from the load-deﬂection curve of a notched beam, 211 from the load-deﬂection curve of a notched beam, 32, 211

316

Scaling of Structural Strength

in slip of studs, 107 in the cohesive crack model, 32, 180, 187, 206, 210 in the crack band model, 170 of a kink band, 141, 143, 145 relation to the J-integral, 68 fracture mechanics in historical context, 5, 7 linear elastic, see linear elastic fracture mechanics of fractal cracks, 71 fracture process zone and characteristic material length, see characteristic material length, fracture process zone and fractal theories, 72 and inhomogeneity size, 15, 38, 86 and stress proﬁle, 165, 167, 180, 181 and transition of behavior, 27 and Weibull theory, 60, 66 eﬀective length of the R-curve, 21 equivalent crack length, 21, 40 ﬂux of energy, 28 in a composite beam, 103 in fractal theories, 72 in historical context, 6 J-integral path, 67, 139, 187 Poisson eﬀect, 10 size, 60, 66, 77, 86, 92, 107, 153, 156, 167, 177, 183, 188 fracture testing, 260 fracture toughness, 17, 88, 118, 156, 183 G, see energy release rate Gb , see fracture energy GF , see fracture energy Gf , see fracture energy

geometry dependence, see shape dependence Hall-Petch formula, 266 incremental plasticity, scaling strain-gradient, 236 J-Integral, 27 and the cohesive crack model, 178, 180, 187 and Weibull size eﬀect, 67 application to kink bands, 137–140, 142, 143 calculation of a ﬂux of energy, 28 critical value, 138, 143 dimensionless expression, 29 expression, 142, 143 path, 28, 140 independence, 67 KI , see stress intensity factor Kc , see fracture toughness large notch or crack, 241 LEFM, see linear elastic fracture mechanics linear elastic fracture mechanics equivalent analysis, see equivalent LEFM analysis generalization to orthotropy, 135 nonlocal, 206, 217 power law exponent −1/2, 7, 12, 13, 24, 59, 60, 78, 109, 112 stress intensity factor, 17 localization, see strain softening localization limiter, see strain softening, localization limiter material characteristic length, 229 mesh bond slip, 125 dependence, 170, 172, 173, 175 discrete elements, 175 inclined crack band, 125, 172

Subject Index

reinforced concrete columns, 125, 127 remeshing, 170, 172 MFSL, see fractal and multifractal scaling law MSG theory, 237 micromechanical model, 72, 76, 121, 170, 172, 230 microplane model, 125, 167–169, 172 multifractal scaling law, see fractal and multifractal scaling law nominal strength, 23, 109 and elastic buckling, 19 asymptotic, 16, 21, 23, 26, 40, 66, 124, 198, 202 data, 31, 34–38, 95, 125, 126, 153 dimensionless, 89 expression, 40, 41, 43, 68, 91, 99, 124, 186 for transitional size range, 13, 14 in compression failure, 124 in historical context, 4, 5, 7 of a composite beam, 103 of sea ice, 20, 81 of stud, 109 pullout, 109 residual, 26 shear loading, 131 time dependence, 153 Weibull-type scaling law, 13, 68 nonlocal damage mechanics, see nonlocal model nonlocal model averging rule, 171 and ﬁnite element size, 172 characteristic length, 172 cohesive law, 181 ﬁnite element analysis, 15, 172, 176, 177

317

of cohesive crack, 26 for damage, 57, 171, 172, 174, 176, 177, 193, 205, 217 in historical context, 5, 9 generalization for Weibull statistical size eﬀect, see Weibull, statistical size eﬀect, nonlocal generalization in historical context, 172 nonlocal LEFM, see linear elastic fracture mechanics, nonlocal physical justiﬁcation, 171 theories for strain localization, 58, 62 with crack interactions, 37 notch length, fracture energy, 258 R-curve, 21–24, 48, 169, 170, 199, 203, 206 random particle model, see discrete element method rate dependence, see time dependence reinforced concrete beams compression failure, 90, 91 diagonal shear failure, 35, 37, 55, 57, 111, 113, 130, 131 torsional failure, 113 columns, 112, 113, 124–126, 128 cylinders double-punch loading, 36 ﬁber-reinforced concrete, 133 size eﬀect laws for, 110, 112 slabs punching shear failure, 113 relaxation, 153, 209, 212 scaling and size eﬀect, 232 shape dependence, 14, 24, 27, 40, 56, 62, 67, 69, 91, 110, 133, 148, 183–186, 188,

318

Scaling of Structural Strength

198, 199, 204, 207, 215–217 shrinkage, 10 SIF, see stress intensity factor small size asymptotic load-deﬂection response, 235 snapback, 16, 17, 96, 98, 157, 158, 161, 162, 167 splitting crack band, see compression failure, by splitting crack band steel-concrete composite beams, 101–110 strain-gradient plasticity, scaling of, 228 Fleck and Hutchinson formulation, 228 strain softening and distributed cracking, 43 and energy dissipation, 91, 173 and loading rate, 10, 156, 157, 173 and wave speed propagation, 173 eﬀective numerical methods, 172 eﬃcient numerical methods, 169 elasto-plastic stability, 89, 90 in cohesive crack model, 181, 217 in elasto-plastic stability, 20 in historical context, 7 in microplane model, 168 loading rate, 173 localization limiter, 170, 173, 174 nonlocal theories, 58, 60 stress intensity factor, 87, 194, 204, 207, 208, 215 at fracture initiation, 196 case of many loads, 133

critical, see fracture toughness density proﬁles, 179, 183, 184, 187, 207 dimensionless, 182 ductility analysis, 162 eccentric loading, 118 fatigue loading, 154 function, 179, 189, 198 of cohesive crack, 166, 178, 183, 184, 204, 207 sea-ice radial bending crack, 81 shape dependence, 198 sharp craft without FPZ, 135 stress relief zone, 15 stud, see steel-concrete composite beams surface energy, 72, 151 thermal bending fracture, 77, 78 thin metallic ﬁlms, boundary layer eﬀect, 265 three-point bend notched beams experimental results, 8, 21, 26, 30, 61, 162 time dependence, 151 creep, 10, 153 due bond ruptures, 154 due to bond ruptures, 151, 152 due to diﬀusion phenomena, 10 due to viscosity, 10, 151, 154, 156, 157 dur to bond ruptures, 154 fatigue, see fatigue crack growth of cohesive crack, 152, 153 of fracture growth, 151 of length scale, 10, 156 TNT theory, 237 toughness, see fracture toughness universal size eﬀect law, 248 unreinforced concrete beams, 113 torsional failure, 113 beams or plates, 90

Subject Index

dams, 57, 113, 117 retaining walls, 113, 117 viscoelasticity, 151, 152, 156, 209, 211, 212 Weibull distribution, 53, 55, 56, 60, 73 energetic-statistical approach, 66–68 nominal strength, 68 size eﬀect law parameters, 57, 59, 62, 66, 74 statistical size eﬀect, 4, 6, 7, 13 and fractality, 72–74, 76 asymptotic analysis, 66 basic hypothesis, 53 for concrete, 35, 57, 111 for quasibrittle structures, 53, 56 limitations, 13, 38, 56, 59, 62 nonlocal generalization, 58–60, 62 stress, 54, 67 weakest link model, 6, 55, 67, 198 Weibull modulus, 53, 57, 66, 67, 74 Weibull theory, 247 weight function, 169, 171, 181, 206 yield plateau, 138

319

Reference Citation Index Acharya and Bassini (2000), 236, 237 ACI 318 (1989), 112 Argon (1972), 134 Ashby and Hallam (1986), 121 Assur (1963), 78 Bao, Ho, Suo and Fan (1992), 135 Barenblatt (1959), 7, 177 Barenblatt (1962), 7, 177 Barenblatt (1979), 12, 17, 25, 193 Barenblatt (1987), 17, 20, 193 Barenblatt (1979, 2003), 245 Barenblatt (1996, 2003), 241 Barr (1995), 9 Bassini (2001), 245 Baˇzant (1967), 122 Baˇzant (1976), 7, 161, 170, 177 Baˇzant (1982), 9, 170 Baˇzant (1983), 18, 19, 25, 145, 191, 216 Baˇzant (1984), 5, 15, 18, 25, 145 Baˇzant (1984a), 7, 10, 86, 191, 216 Baˇzant (1984b), 9, 171, 172 Baˇzant (1984c), 168 Baˇzant (1985), 258 Baˇzant (1985a), 193 Baˇzant (1985b), 193, 209 Baˇzant (1986), 29 Baˇzant (1987), 25 Baˇzant (1987a), 144 Baˇzant (1990a), 179, 184 Baˇzant (1992a), 79

Baˇzant (1992b), 77, 78 Baˇzant (1993), 12, 13, 78, 122, 124, 152 Baˇzant (1994b), 171 Baˇzant (1995), 42 Baˇzant (1995c), 152 Baˇzant (1995d), 32, 38, 46, 69 Baˇzant (1996), 130, 255, 256 Baˇzant (1996a), 23, 32, 46, 131 Baˇzant (1996b), 113, 117, 118 Baˇzant (1997a), 21, 57, 133, 191, 206 Baˇzant (1997b), 9, 42, 71 Baˇzant (1997c), 42 Baˇzant (1998), 42 Baˇzant (1998a), 133, 197, 216 Baˇzant (1998b), 133 Baˇzant (1999a), 11 Baˇzant (1999b), 11, 212 Baˇzant (2000), 114, 115, 179, 191, 237 Baˇzant (2001, 2002), 235, 259 Baˇzant (2001a), 51, 212 Baˇzant (2001b), 219, 223 Baˇzant (2001c), 55 Baˇzant (2001d), 212 Baˇzant (2001e), 230 Baˇzant (2002), 245, 258, 259, 260 Baˇzant (2004a), 241 Baˇzant and Xi (1991), 62 Baˇzant and S ¸ ener (1997), 113 Baˇzant and Becq-Giraudon (1999), 162

322

Scaling of Structural Strength

Baˇzant and Becq-Giraudon (2001), 32 Baˇzant and Becq-Giraudon (2002), 258, 260 Baˇzant and Beissel (1994), 184 Baˇzant and Cao (1986a), 130 Baˇzant and Cao (1986b), 130 Baˇzant and Cao (1987), 113, 130 Baˇzant and Cao (2002a), 238 Baˇzant and Cedolin (1979), 7, 177 Baˇzant and Cedolin (1980), 7 Baˇzant and Cedolin (1991), 7, 17, 20, 90, 98, 158, 161, 173 Baˇzant and Chen (1997), 1, 12, 191, 248 Baˇzant and Estenssoro (1979), 10 Baˇzant and Frangopol (2000), 114, 117 Baˇzant and Gettu (1990), 32 Baˇzant and Gettu (1992), 151, 153, 173 Baˇzant and Jir´ asek (2001), 92 Baˇzant and Jir´ asek (1994a), 171 Baˇzant and Jir´ asek (1994b), 171 Baˇzant and Jir´ asek (2002), 258 Baˇzant and Kazemi (1990), 259 Baˇzant and Kazemi (1991), 216 Baˇzant and Kazemi (1991a), 35, 130 Baˇzant and Kazemi (1991b), 32, 206 Baˇzant and Kim (1991), 10 Baˇzant and Kim (1997), 79, 80 Baˇzant and Kim (1998), 85, 86 Baˇzant and Kwon (1994), 112, 113, 125 Baˇzant and Li (1995), 145, 259 Baˇzant and Li (1995), 43, 80, 165 Baˇzant and Li (1995a), 166, 178, 197 Baˇzant and Li (1995b), 36, 166, 178 Baˇzant and Li (1996), 47, 259

Baˇzant and Li (1996), 47, 248, 259, 260 Baˇzant and Li (1997), 151–153, 197, 210 Baˇzant and Lin (1988a), 9, 36 Baˇzant and Lin (1988b), 9, 172 Baˇzant and Nov´ ak (2000a), 57, 62 Baˇzant and Nov´ ak (2000b), 13, 56, 62, 66, 73, 197, 198 Baˇzant and Nov´ ak (2000a), 60, 125 Baˇzant and Nov´ ak (2000b), 125 Baˇzant and Oh (1983), 9, 36, 170, 177 Baˇzant and Pang (2004), 264 Baˇzant and Pfeiﬀer (1987), 25 Baˇzant and Pijaudier-Cabot (1988), 9, 172 Baˇzant and Planas (1998), 3, 24, 29, 30, 32, 43, 47, 57, 62, 93, 145, 177, 178, 184, 186, 191, 193, 197, 199, 202, 206, 210 Baˇzant and Raftshol (1983), 10 Baˇzant and Rajapakse (1999), 9, 11 Baˇzant and Schell (1993), 156 Baˇzant and Sun (1987), 130 Baˇzant and V´ıtek (1999), 101, 102, 107 Baˇzant and Wu (1993), 151 Baˇzant and Xi (1991), 58, 60 Baˇzant and Xiang (1996), 124 Baˇzant and Xiang (1997), 122, 124, 144 Baˇzant and Xu (1991), 156 Baˇzant and Yavari (2004), 265 Baˇzant and Yu (2002), 244, 258 Baˇzant and Yu (2003), 263 Baˇzant and Yu (2004), 245, 249, 255 Baˇzant, Yu and Zi (2002), 261, 262 Baˇzant et al. (1984), 172 Baˇzant et al. (1999), 137, 142, 145, 147, 148

Reference Citation Index

Baˇzant et al. (1999a), 144 Baˇzant et al. (1999b), 144 Baˇzant, Belytschko and Chang (1984), 171 Baˇzant, Belytschko and Chang (1984), 9 Baˇzant, Caner, Carol, Adley and Akers (2000), 168 Baˇzant, Daniel and Li (1996), 135 Baˇzant, ed. (1992), 9 Baˇzant, Guo, and Faber (1995), 173 Baˇzant, Lin and Lippmann (1993), 132 Baˇzant, Tabbara et al. (1990), 36 Baˇzant, Tabbara, Kazemi and Pijaudier-Cabot (1990), 174 Baˇzant, Xi and Reid (1991), 74 Baˇzant, S ¸ ener and Prat (1988), 113 Baˇzant, S ¸ ener and Prat (1988), 130 Baˇzant and Planas (1998), 26 Baˇzant, Pijaudier-Cabot and Pan (1987a), 161 Baˇzant, Pijaudier-Cabot and Pan (1987b), 161 Baˇzant, Zhou and Daniel (2003), 252, 253 Baˇzant, Zhou, Novak and Daniel (2004), 247, 254 Baˇzant, Zi and McClung (2003), 262 Bender and Orszag (1978), 25 Beremin (1983), 54, 67 Biot (1965), 122 Borodich (1992), 9, 69, 71 Bouchaud, Lapasset et Planes (1990), 9, 69 Bridgman (1922), 17 Brocca and Baˇzant (2000), 125 Brocca et al. (2001), 254 Brown (1987), 9, 69 Buckingham (1914), 17 Buckingham (1915), 17

323

Budianski (1983), 134 Budianski and Fleck (1994), 134 Budianski, Fleck and Amazigo (1997), 134 Cahn (1989), 9 Cahn (1989), 69 Carpinteri (1984), 18 Carpinteri (1986), 6, 9, 18 Carpinteri (1987), 249 Carpinteri (1989), 6 Carpinteri (1994a), 9, 10, 69 Carpinteri (1994b), 9, 69 Carpinteri and Chiaia (1995), 9, 10, 42, 69, 73 Carpinteri and Chiaia (1995a), 9 Carpinteri and Ferro (1994), 9, 10, 42, 69 Carpinteri, Chiaia and Ferro (1994), 9, 10, 42, 69 Carpinteri, Chiaia and Ferro (1995), 9, 10, 42, 69 Carpinteri, Ferro and Intervenizzi (1995), 9, 10, 42, 69 Carter (1992), 121, 132 Carter, Lajtai and Yuan (1992), 132 ˇ Cervenka and Pukl (1994), 9, 170 Chelidze and Gueguen (1990), 9, 69 Chen and Runt (1989), 9, 69 Christensen and DeTeresa (1997), 134 Collins (1978), 130 Collins and Mitchell (1980), 130 Collins, Mitchell, Adebar and Vecchio (1996), 130 Costin (1991), 121 Cotterell (1972), 121 Cottrell (1963), 32 Cundall (1971), 174 Cundall and Strack (1979), 174 Cusatis et al. (2003a,b), 260

324

Scaling of Structural Strength

Daniels (1945), 264 da Vinci (1500s), 3 de Borst and Guti´errez (1999), 174 Dempsey, Adamson and Mulmule (1995), 33 Dempsey, Adamson and Mulmule (1999), 33, 35 Duan and Hu (2003), 248, 259 Duan, Hu and Wittmann (2002, 2003), 255 Dugdale (1960), 7, 177 Dunn et al. (1997a,b), 249 Elices et al. (1992), 258 Eligehausen and Oˇzbolt (1992), 109 Evans and Marathe (1968), 173 Fairhurst and Cornet (1981), 121 Feng, Ji, Zhuang and Ding (1995), 9, 70 Fisher and Tippett (1928), 5, 6, 56 Fleck and Hutchinson (1993), 219 Fleck and Hutchinson (1997), 219 Fleck and Hutchinson (1997), 137, 219, 228 Fleck and Hutchinson (1963, 1997), 237 Fleck and Olurin (2001), 254 Fleck and Shu (1995), 137 Freudenthal (1968), 5, 6 Fr´echet (1927), 5, 56 Galileo (1638), 4 Gao and Huang (2000), 219 Gao, Huang and Nix (1999), 219, 237 Gao, Huang, Nix and Hutchinson (1999), 219 Gibson and Ashby (1997), 254 Giles (1962), 17 Griﬃth (1921), 5

Guinea, Planas and Elices (1994a,b), 258, 259 Guinea et al. (1997), 260 Hadamard (1903), 173 Haimson and Herrick (1989), 132 Hawkes and Mellor (1970), 121 Hill (1962), 173 Hillerborg (1985a), 32 Hillerborg (1985b), 32 Hillerborg, Mod´eer and Petersson (1976), 7, 32, 165, 178 Hinch (1991), 25 Horii and Nemat-Nasser (1982), 121 Horii and Nemat-Nasser (1986), 121 Hornbogen (1989), 9, 69 Hsu (1988), 130 Hu (1997, 1998), 255 Hu and Wittmann (1991, 1992a), 255 Huang, Gao, Nix and Hutchinson (2000), 219 Hutchinson (1997), 219, 228 Iguro, Shiyoa, Nojiri and Akiyama (1985), 130 Ingraﬀea (1977), 121, 170, 172 Ingraﬀea and Heuz´e (1980), 121 Irwin (1958), 22, 135 Issa, Hammad and Chudnovsky (1992), 9, 69 Jackson (1992), 252 Jenq and Shah (1985), 32 Jir´ asek and Baˇzant (1995a), 36, 174 Jir´ asek and Baˇzant (1995b), 36, 174, 175 Jir´ asek (1996), 171 Jir´ asek (2003), 258 Johnson et al. (2000), 252

Reference Citation Index

Kachanov (1985), 171 Kachanov (1987), 171 Kani (1967), 130 Kaplan (1961), 6 Karihaloo, Abdalla and Imjai (2003), 255 Kemeny and Cook (1987), 132 Kemeny and Cook (1991), 121, 132 Kendall (1978), 122 Kesler, Naus and Lott (1971), 7 Kfouri and Rice (1977), 7, 178 Kittl and Diaz (1988), 6 Kittl and Diaz (1989), 6 Kittl and Diaz (1990), 6 Knauss (1973), 7, 178, 179 Knauss (1974), 7, 178, 179 Kuhlmann and Breuninger (1998), 102 Kupfer (1964), 130 Kyriakides et al. (1995), 134 Lange, Jennings and Shah (1993), 9, 69 Lehner and Kachanov (1996), 121 Leicester (1969), 6, 7 Leonhardt (1977), 130 Leonhardt and Walther (1962), 130 Li and Baˇzant (1997), 151, 152 Long, Suquin and Lung (1991), 9, 69 Mahesh et al. (2002), 264 Maier and Zavelani (1970), 98 M˚ aløy, Hansen, Hinrichsen and Roux (1992), 9, 69 Mandel (1964), 173 Mandelbrot (1984), 9 Mandelbrot et al. (1984), 69 Mariotte (1686), 4 Marti (1980), 130 Marti (1989), 36 Mecholsky and Mackin (1988), 9, 69

325

Mihashi (1983), 6 Mihashi and Izumi (1977), 6 Mihashi and Rokugo (1998), 9 Mihashi and Zaitsev (1981), 6 Mindlin (1965), 219 M¨ orach (1922), 130 Mosolov and Borodich (1992), 9, 69, 71 Mulmule et al. (1995), 33 Murakami (1987), 87 Nakayama (1965), 32 Needleman (1990), 178 Nesetova and Lajtai (1973), 121, 132 Nielsen and Braestrup (1975), 130 Nixon (1996), 121 Oˇzbolt and Baˇzant (1996), 36, 172 Palmer and Rice (1973), 138, 140, 143, 144 Paris and Erdogan (1967), 154 Peerlings, de Borst, Brekelmans and de Vree (1996), 174 Peirce (1926), 5 Peng and Tian (1990), 9, 69 Petersson (1981), 9, 166, 178 Pheonix and Beyerlein (2000), 264 Pijaudier-Cabot and Baˇzant (1987), 9, 172 Planas and Elices (1986), 179, 184 Planas and Elices (1988), 9 Planas and Elices (1989a), 9 Planas and Elices (1989b), 9 Planas and Elices (1992), 178, 179, 184, 199, 216 Planas and Elices (1993), 9, 10, 178, 179, 184, 199, 216 Planas, Baˇzant and Jir´ asek (2001), 11 Porter (1933), 17 Prandtl (1904), 1, 193

326

Scaling of Structural Strength

Reineck et al. (2003), 263 Reinhardt (1985), 178, 179 Rice (1968a), 140, 178, 187, 256 Rice (1968b), 143, 144 Rice (1992), 178 Rice and Levy (1972), 80 RILEM (1990), 32 Ritter (1899), 130 Rocco (1995), 67 Rokugo, Uchida, Katoh and Koyanagi (1995), 67, 197 Rosen (1965), 134 Rots (1988), 9 Ruggieri and Dodds (1996), 54 R¨ usch and Hilsdorf (1963), 173 Sammis and Ashby (1986), 121 Sanderson (1988), 121 Saouma and Barton (1994), 9, 70 Saouma, Barton and Gamal-el-Din (1990), 9, 39 Schlaich, Schafer and Jannewein (1987), 130 Schlangen and van Mier (1992), 175 Schulson (1990), 121 Schulson and Nickolayev (1995), 121 Sedov (1959), 20, 193 S ¸ ener, Baˇzant and Becq-Giraudon (1999), 113 Shioya and Akiyama (1994), 130 Shioya, Iguro, Nojiri, Akiayama and Okada (1989), 130 Shipsa et al. (2000), 254 Slepyan (1990), 78, 79 Sluys (1992), 10 Smith (1974), 178, 179 Soutis, Curtis and Fleck (1993), 147 Steif (1984), 121 Streeter and Wylie (1975), 17 Suo, Bao, and Fan (1992), 178

Tandon, Faber, Baˇzant and Li (1995), 173 Tang et al. (1996), 259 Tattersall and Tappin (1966), 32 Taylor (1938), 168 thermal bending fracture, 77 Th¨ urlimann (1976), 130 Timoshenko (1953), 5 Tippett (1925), 5 Toupin (1962), 219 Tvergaard and Hutchinson (1992), 178 van Mier and Schlangen (1993), 175 von Mises (1936), 5, 56 Walraven (1978), 130 Walraven (1995), 130 Walraven and Lehwalter (1994), 130 Walsh (1972), 7 Walsh (1976), 7 Weibull, 4, 66 Weibull (1939), 6, 10, 53, 62 Weibull (1949), 6, 53 Weibull (1951), 53 Weibull (1956), 6, 53 Wells (1961), 32 Williams (1952), 249 Willis (1967), 178, 179 Wisnom (1991), 252 Wisnom and Atkinson (1997), 252 Wittmann (1990), 255 Wittmann and Zaitsev (1981), 121 Wittmann, ed. (1994), 9 Wnuk (1974), 7, 178, 179 Xie (1987), 9, 69 Xie (1989), 9, 69 Xie (1993), 9, 69 Xie and Sanderson (1995), 9, 69 Xie, Sanderson and Peacock (1994), 9, 69

Reference Citation Index

Young (1807), 5 Yuan, Lajtai and Ayari (1992), 132 Yuan, Lajtai and Ayari (1993), 121 Zaitsev (1985), 121 Zaitsev and Wittmann (1974), 6 Zech and Wittmann (1977), 6, 13, 56, 67 Zenkert and B¨ acklund (1989), 254 Zubelewicz and Baˇzant (1987), 175

327

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close